This book is meant as an introduction to graphene plasmonics and aims at the advanced undergraduate and graduate student

*337*
*55*
*72MB*

*English*
*Pages 464
[462]*
*Year 2016*

- Author / Uploaded
- Paulo Andre Dias Goncalves
- Nuno Miguel Machado Reis Peres

*Table of contents : ContentsForewordPrefaceAcknowledgmentsList of FiguresList of Tables1. Introduction 1.1 Plasmonics: Generalities 1.2 Plasmonics: Recent Developments2. Electromagnetic Properties of Solids in a Nutshell 2.1 Classical Electrodynamics Basics 2.1.1 Maxwell’s equations 2.1.2 Boundary conditions 2.2 Drude Model 2.3 Preliminaries to Graphene Plasmonics 2.3.1 Elementary electronic properties 2.3.2 The optical conductivity of graphene 2.3.3 Lindhard function: Beyond the local approximation 2.3.4 Lindhard polarization function in relaxation-time approximation: The case of graphene 2.4 The Transfer-Matrix Method and the First Appearance of Plasmons in Graphene 2.4.1 Transfer-matrix for a graphene monolayer 2.4.2 Transmittance, reflectance and absorbance of electromagnetic radiation by a graphene monolayer 2.4.3 Transfer-matrix for a graphene double-layer 2.4.4 Transfer-matrix for multi-layer graphene structures 2.4.5 Plasmons: A transfer-matrix approach3. Surface Plasmon-Polaritons at Dielectric-Metal Interfaces 3.1 Single Dielectric-Metal Interface 3.1.1 Dispersion relation 3.1.1.1 Zero damping (γ = 0) 3.1.1.2 Finite damping (γ ≠ 0) 3.1.2 Propagation length and field confinement 3.2 Multilayer Structures 3.2.1 Double Interface 3.2.2 Dispersion relation 3.3 A Short Note on Perfect Conductors4. Graphene Surface Plasmons 4.1 Monolayer Graphene 4.1.1 Spectrum of GSPs 4.1.2 Field profile of GSPs in single-layer graphene 4.1.3 Plasmon dispersion revisited 4.1.4 Loss function 4.1.5 A word on TE surface waves 4.2 Double-Layer Graphene 4.2.1 Dispersion relation 4.2.2 Field profile of GSPs in double-layer graphene 4.2.3 Plasmon dispersion beyond the Drude model approximation 4.3 Surface Plasmon-Phonon-Polaritons in Graphene 4.3.1 Graphene on SiC 4.3.2 Graphene on SiO2 4.4 Magneto-Plasmons in Monolayer Graphene 4.4.1 Derivation of the spectrum’s condition 4.4.2 Solution of the semi-classical spectrum’s condition in a special limit 4.4.3 Spectrum of magneto-plasmons in the quantum regime: Landau quantization 4.5 A Detour: Surface Phonon-Polaritons in hBN 4.5.1 Solution of the electromagnetic problem 4.5.2 Guided phonon-polariton modes5. Excitation of Graphene Surface Plasmons 5.1 Grating Coupling 5.1.1 Graphene on Gallium-Arsenide: The role of SO phonons 5.2 Prism Coupling 5.2.1 Otto configuration: Single-layer graphene 5.3 Near-field Excitation and Imaging of GSPs 5.4 Others 5.5 Excitation of SPP’s by a Moving Line of Charge6. Launching Plasmons Using a Metallic Antenna 6.1 Theoretical Model and Integral Equation 6.2 Approximate Solution via Fourier Expansion 6.3 Results and Discussion7. Plasmonics in Periodic Arrays of Graphene Ribbons 7.1 A Seminal Paper 7.2 Theoretical Model 7.2.1 Setting up the model 7.2.2 The scattering problem 7.3 Applications and Results 7.3.1 Periodic array of graphene ribbon 7.3.2 Theory versus experiment 7.4 A THz Polarizer 7.5 Scattering From a Periodic Grid in the Regime kw < 18. Plasmons in Graphene Nanostructures and in One-dimensional Channels 8.1 Edge Plasmons in a Graphene Nanoribbon 8.1.1 Prelude: Green’s functions for a 2-layered medium 8.1.1.1 Homogeneous medium 8.1.1.2 2-layered medium 8.1.2 Plasmonic spectrum of a graphene nanoribbon 8.1.2.1 Plasmonic spectrum of a graphene nanoribbon: results 8.1.3 An extension: magneto-plasmons in a graphene ribbon 8.1.4 Scattering of THz radiation by a graphene micro-ribbon 8.2 Localized Surface Plasmons in a Graphene Ring 8.2.1 Spectrum of graphene plasmons in a graphene ring 8.2.1.1 Plasmonic spectrum of a graphene ring: results 8.3 Plasmonic Excitations in a Graphene Nanodisk 8.4 Scattering of Graphene Plasmons by a Conductivity Step 8.4.1 The mathematical problem 8.4.2 Solution of the Riemann-Hilbert problem 8.4.3 Further details 8.4.4 Calculation of the reflection amplitude 8.4.5 An alternative derivation of Eq. (8.137) 8.5 Localized Surface Plasmons in a Graphene Sheet with a Gaussian Groove 8.5.1 Few useful definitions 8.5.2 Formulation of the problem 8.5.3 Green’s theorem, Green’s functions, and the eigenvalue problem 8.5.4 Spectrum of surface plasmon-polaritons in the presence of a Gaussian groove9. Excitation of Surface Plasmon-Polaritons Using Dielectric Gratings 9.1 Some Basic Definitions and Results 9.2 Tangent and Normal Vectors, and Boundary Conditions 9.3 A Trivial Example: Recovering Previous Results 9.4 The Fields in D+ and D− 9.4.1 Reflectance and transmittance efficiencies 9.4.2 Particular limits for the transmittance and the reflectance 9.5 A Non-Trivial Example: A Grating with a Sine-Profile10. Excitation of Plasmons by an Emitting Dipole 10.1 Statement of the Problem and a Bit of Electrostatics 10.2 Calculation of the Non-Radiative Transition Rate: Particle-Hole Excitations Pathway 10.3 Calculation of the Total Transition Rate: Full Electromagnetic Calculation 10.4 Purcell Effect in Hyperbolic Materials11. Concluding RemarksAppendix A Derivation of the Susceptibility of Graphene A.1 Undoped Susceptibility A.1.1 The imaginary part of the undoped susceptibility A.1.2 The real part of the undoped susceptibility A.2 Doped Part: Fermi Sea Contributions A.2.1 Intraband term A.2.2 Interband term A.2.3 Imaginary part of A.2.4 Imaginary part of A.2.5 Real Part of and A.3 Summary for the Real and Imaginary Parts of Graphene Susceptibility A.3.1 Real part of the susceptibility A.3.2 Imaginary part of the susceptibility A.4 Some Useful IntegralsAppendix B Derivation of the Intra- and Inter-band Conductivity of GrapheneAppendix C Inhomogeneous Drude Conductivity C.1 Longitudinal Conductivity C.2 Transverse ConductivityAppendix D Derivation of the Expression Relating the Longitudinal Conductivity with the PolarizabilityAppendix E Derivation of the Polarization of Graphene in the Relaxation-Time Approximation E.1 Hamiltonian and Particle and Current Densities E.2 Local Equilibrium Density Matrix E.3 A Useful Identity E.4 Equation of Motion for the Density Matrix E.5 Polarization in the Relaxation-Time ApproximationAppendix F RPA for Double-Layer Graphene F.1 Equation of Motion Method F.2 Diagrammatic ApproachAppendix G Effective Dielectric Constants for Coulomb-Coupled Double-Layer GrapheneAppendix H Magneto-Optical Conductivity of GrapheneAppendix I Supplementary Material for Chapter 7 I.1 Derivation of the Expressions for the Transmittance and Reflectance I.2 Modes Contributing to Each ResonanceAppendix J The Method of ToigoAppendix K Boundary Condition in the Dipole ProblemAppendix L Fourier Transform of the Dipole PotentialAppendix M Non-Radiative Decaying Rate: Electrostatic Calculation M.1 Doped Graphene M.2 A Detour: Neutral GrapheneAppendix N Reflection Amplitude of an Electromagnetic Wave due to a Graphene Interface N.1 The Simple Case of Free Standing Graphene N.2 Reflection and Transmission Amplitudes: Fresnel Coefficients N.2.1 TE (transverse electric) / s−components N.2.2 TM (transverse magnetic) / p−componentsAppendix O Green’s Functions in the Rope Problem O.1 The Homogeneous Rope O.1.1 Response to a localized force O.2 The Inhomogeneous Rope O.2.1 Reflection and transmition coefficients O.2.2 Response to an external force in the inhomogeneous regimeAppendix P Derivation of the Transition Rate of a Quantum Emitter Near an Interface P.1 Polarization Vectors and Green’s Functions P.1.1 Definition of s− and p−polarization vectors and angular spectrum representation P.1.2 The free space Green’s function P.1.3 Green’s functions for problems with flat interfaces I P.2 Dipole Decaying Rate P.3 Explicit Form of the Tensor Product of the Polarization Vectors P.4 The Free Green’s Function in Real Space P.5 Green’s Function for Problems With Flat Interfaces II P.5.1 Free-space Green’s function revisited P.5.2 Electric field from a dipole in terms of Green’s functions P.5.3 Green’s functions: s−component P.5.4 Green’s functions: p−component P.5.5 Derivation of the matrix structure of the Green’s functionsBibliographyIndex*

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

9948_9789814749978_tp.pdf 1

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Graphene Plasmonics An Introduction to

P.A. Gonça

30/3/16 8:58 AM

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

May 2, 2013 14:6 BC: 8831 - Probability and Statistical Theory

This page intentionally left blank

PST˙ws

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

An Introduction to

Graphene Plasmonics

P.A.D Gonçalves University of Minho, Portugal

N.M.R Peres Univeristy of Minho, Portugal

World Scientific NEW JERSEY

•

LONDON

9948_9789814749978_tp.pdf 2

•

SINGAPORE

•

BEIJING

•

SHANGHAI

•

HONG KONG

•

TAIPEI

•

CHENNAI

•

TOKYO

30/3/16 8:58 AM

Published by World Scientific Publishing Co. Pte. Ltd. 5 Toh Tuck Link, Singapore 596224 USA office: 27 Warren Street, Suite 401-402, Hackensack, NJ 07601

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

UK office: 57 Shelton Street, Covent Garden, London WC2H 9HE

Library of Congress Cataloging-in-Publication Data Names: Gonçalves, P. A. D., author. | Peres, N. M. R., 1967– author. Title: An introduction to graphene plasmonics / P.A.D. Gonçalves (University of Minho, Portugal), N.M.R. Peres (University of Minho, Portugal). Description: Singapore ; Hackensack, NJ : World Scientific Publishing Co. Pte. Ltd., [2016] | 2016 | Includes bibliographical references and index. Identifiers: LCCN 2016003760| ISBN 9789814749978 (hardcover ; alk. paper) | ISBN 9814749974 (hardcover ; alk. paper) | ISBN 9789814749985 (softcover ; alk. paper) | ISBN 9814749982 (softcover ; alk. paper) Subjects: LCSH: Plasmons (Physics) | Graphene--Optical properties. | Nanophotonics. Classification: LCC QC176.8.P55 G66 2016 | DDC 530.4/4--dc23 LC record available at http://lccn.loc.gov/2016003760 British Library Cataloguing-in-Publication Data A catalogue record for this book is available from the British Library.

Copyright © 2016 by World Scientific Publishing Co. Pte. Ltd. All rights reserved. This book, or parts thereof, may not be reproduced in any form or by any means, electronic or mechanical, including photocopying, recording or any information storage and retrieval system now known or to be invented, without written permission from the publisher.

For photocopying of material in this volume, please pay a copying fee through the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, USA. In this case permission to photocopy is not required from the publisher. In-house Editor: Christopher Teo Typeset by Stallion Press Email: [email protected] Printed in Singapore

Christopher - An Introduction to Graphene Plasmonics.indd 1

15/2/2016 1:33:59 PM

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

To our families: (Inês and João Nuno, and Augusta, Augusto, and Filipa)

And our parents: (Clementina and João Paulo, and Cecília and Luís)

v

b2445-mas

page v

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

May 2, 2013 14:6 BC: 8831 - Probability and Statistical Theory

This page intentionally left blank

PST˙ws

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Foreword

The consequences of plasmons, collective excitations of the electron plasma in conductive materials, have been appreciated for centuries — if not millenia, just witness the beautiful ancient colored glasses which are found in museums and churches. There, the colors originate from localized surface plasmonic excitations in nanoscale metallic particles. This old example crystallizes the essence of modern plasmonics: on one hand, one needs surfaces, and on the other hand the active objects should be in the nanometer scale. Graphene, the wonder material of the 21st century, is twodimensional and therefore all surface; it is just one atomic layer thick and by using modern nanofabrication technologies it can be sculpted laterally to nanoribbons or nanoflakes. Graphene has very special optical properties, which stem from its fascinating Dirac-like electronic dispersion law its charge carriers obey. It is no wonder then that graphene plasmonics is an important and growing area of research. Most importantly, it holds the promise of many practical applications, for example in plasmonic circuitry, nanophotonics, and sensing, just to mention a few. This is a book on graphene plasmonics. It originates from a group that is world-known for its research in this area — who would be better qualified to write such a book? Students entering graphene plasmonics have had a difficult time in navigating between original research articles, which rarely are particularly pedagogical in their approach, and text books addressing plasmonics (many of which are excellent), but usually having conventional metals as the working material. The present book thus fills in an important gap. Now, all the relevant material is collected in a single volume. What is essential is that the material is thoroughly worked through: the approach is extremely systematic, all equations follow from previous equations in a manner that a dedicated student can easily follow. The technical

vii

page vii

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

viii

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

level of the book is accessible to an advanced undergraduate or a beginning graduate student, but experienced researchers will also benefit from the many insights it offers. It starts with an introduction to Maxwell’s equations, and thereafter works its way towards graphene, and the nanostructures made of graphene. The very important issue of interfaces and two-dimensionality is given an exhaustive treatment. Underway the quantum mechanical description of graphene’s electronic structure is developed, including effects due to applied magnetic fields, and central topics in manybody physics are discussed (and further explained and elaborated in useful appendices). With the basic concepts at hand, the reader is taken to the frontier of today’s research: plasmons in nanostructured two-dimensional materials, such as arrays of microribbons, nanorings, and gratings. The excitation mechanisms needed to launch plasmons and plasmon-polaritons are discussed, as well as methods that are required to observe the excited plasmons. The authors should be congratulated for having accomplished an important task: to offer a self-contained and complete, yet accessible, treatment of a modern area under rapid progress. Armed with the knowledge extracted from this book tomorrow’s students are ready to tackle the many exciting opportunities and challenges that plasmonics in two-dimensional materials offer.

Antti-Pekka Jauho, Technical University of Denmark, 2016

page viii

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Preface

Over the last few years, graphene plasmonics has emerged as a new research topic, positioned at the interface between condensed matter physics and photonics. This still young but rapidly growing field, resulting from the overlap between graphene physics and plasmonics, deals with the investigation and exploration of graphene surface plasmon-polaritons (GSPs) for controlling light-matter interactions and manipulating light at the nanoscale. In 2011, experimental research in plasmonics in graphene was in its infancy. Some theoretical papers had already been written, but the field was awaiting for some sort of experimental boost. In 2011 a seminal experimental paper (to be discussed in Section 7.1) emerged, demonstrating that plasmonic effects in graphene could be controlled optically, by shining electromagnetic radiation onto a periodic grid of graphene micro-ribbons. This opened a new avenue in graphene physics, launching the new flourishing field of graphene plasmonics. Since then, the field has been witnessing enormous developments at a rapid pace (to be described in Section 1.2). This is a book on plasmonics in graphene. It grew out of the authors’ own interest in the field. Many of the topics covered here refer to problems that were amongst the first to appear in the scientific literature, to which one of the authors has contributed to some extent. Throughout this monograph we have tried to make this book as self-contained as possible, and to provide substantial detail in all derivations. Indeed, with a pencil, some sheets of paper, a dose of enthusiasm, and, at times, a bit of effort, the interested reader should find it easy to reproduce all the results in the book (the Appendices will be most useful for such endeavor). Therefore, we hope that this book will serve as a springboard for any newcomer in graphene

ix

page ix

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

x

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

plasmonics. Hopefully, the advanced researcher may also find reasons to keep this book in her/his shelf and to recommend it to her/his students. This is also a book about theoretical techniques to deal with plasmonics in graphene. Many of these techniques have been applied to metal plasmonics before and have been adapted here to tackle plasmonic effects in graphene. The main difference is that metals are described by a complex dielectric function, whereas graphene is described by its complex (non-local whenever necessary) optical conductivity and its sheet (two-dimensional) current. The book is organized as follows: in Chapter 1 we introduce the theme of the book and present a short review of the literature. We have surely missed some important references and can only hope for the indulgence and comprehension of their authors. This might be specially true in what concerns theoretical and computational work (the literature is already too vast to be covered in a comprehensive way). In Chapter 2 we review some elementary concepts about electronic transport in solids, give a short introduction to graphene’s electronic properties, and present some tools to be used later in the book, with particular emphasis on a method to compute the non-local optical conductivity of graphene from the electronic susceptibility in the relaxation-time approximation. Chapter 3 discusses plasmonics at metaldielectric interfaces and in metal thin films. The results obtained there will be later compared with those found in graphene. Both the semi-infinite metal and the thin metal-film are discussed. In Chapter 4, we finally dive into the field of graphene plasmonics and discuss plasmons both in singleand double-layer graphene. The interesting problem of coupled surface plasmon-phonon-polaritons is also discussed in that Chapter. A short introduction of magneto surface plasmon-polaritons is included, considering both the semi-classical and quantum regimes. We close the chapter with the study of guided (bounded) surface phonon-polaritons in a crystal slab of hexagonal boron-nitride (hBN), a problem very recently considered in the literature and one for which many future developments are expected. As we shall see, surface plasmons cannot be directly excited in graphene by free propagating electromagnetic waves (as is also the case in planar metal-dielectric interfaces). Thus, in Chapter 5 we review some of the most popular methods of inducing surface plasmon-polaritons in this twodimensional material (which are also used in traditional metal-based plasmonics). We then move to a detailed study of two methods for exciting plasmons in graphene. These are discussed in Chapters 6 and 7, encompassing the excitation of GSPs by a metallic antenna and by coupling light

page x

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Preface

9in x 6in

b2445-mas

xi

to GSPs in a patterned array of graphene ribbons. The discussion of the periodic graphene ribbons system sets the stage for the discussion of the spectrum of surface plasmons in graphene micro-ribbons, micro-rings, and disks. This is done in Chapter 8, where the case of a micro-deformation of the graphene sheet is also discussed, taking as an example the problem of a Gaussian groove. This latter case can be considered an example of nano-structured graphene. These three problems are considered in the electrostatic limit, which turns out to be a rather good approximation when dealing with plasmons in graphene. As we shall show they exhibit scale invariance, a property of the electrostatic limit. It then follows, in Chapter 9, a discussion of the excitation of plasmons by a corrugated dielectric grating, which is a generalization of the single micro-deformation studied in the preceding chapter to the case of a periodic deformation. In this case, the calculation takes retardation into account, but could very well be treated within the electrostatic approximation. Despite some differences, the four methods discussed in Chapters 6, 7, 8, and 9 have in common the decomposition of the fields in a superposition of Fourier modes, either using a Fourier series, for periodic structures, or a Fourier integral for non-periodic systems. In Chapter 10 we discuss how an emitting dipole (for example, a dye, a quantum dot, or a Rydberg atom) can excite graphene plasmons by non-radiative energy transfer from the emitter to graphene. We will see that this is in principle possible, and we compute the non-radiative decaying rate of an emitter. The role of particle-hole processes and excitation of plasmons is discussed separately. We end this Chapter with the calculation of the Purcell factor which encodes information about the total decaying rate of the emitter in the presence of graphene. Finally, in Chapter 11, we conclude with a brief outlook and with the discussion of some topics that have been left out in this book, and which we believe will become rather important in the near future. Also, we have written a number of appendices with either details of the calculations or extensions of the materials discussed in the bulk of the book. To get a flavor of the main ideas, reading the appendices is unnecessary. However, they are a requisite for a working knowledge on the topics discussed in the main text. Our ultimate hope is that readers may find this book a valuable tool for their study and research in the exciting field of graphene plasmonics and nanophotonics, whether they are currently working on the topic or are about to enter on it. The book’s intended purpose is to bring together some of the main topics that are scattered throughout the already vast literature, and to do justice to this alluring field of graphene plasmonics.

page xi

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

xii

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

To conclude, we further hope that the readers may read this book with the same enthusiasm that we had writing it. Comments, suggestions, and corrections aiming at improving the book for future usage will be most welcome (these can be sent to [email protected]).

Paulo André Dias Gonçalves Nuno Miguel Machado Reis Peres Department of Physics University of Minho Braga, 2016

page xii

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Acknowledgments

The authors acknowledge B. Amorim, Y. V. Bludov, E. V. Castro, A. H. Castro Neto, A. Chaves, A. Ferreira, F. Guinea, J. Lopes dos Santos, V. Pereira, R. M. Ribeiro, J. E. Santos, T. Stauber, and M. I. Vasilevskiy for many years of collaboration and discussions about the physics of graphene in general and on plasmonics in graphene and other materials in particular. We thank B. Amorim, Y. V. Bludov, A. Chaves, A. Ferreira, J. Lopes dos Santos, R. M. Ribeiro, J. E. Santos, and M. I. Vasilevskiy for reading parts of the manuscript at different moments of writing. B. Amorim is acknowledged for providing the derivations in Appendices D, O, and P. A. Chaves is acknowledged for providing the derivation in Appendix A J. E. Santos is acknowledged for providing the derivation in Appendix K. Any error and/or inaccuracy that may remain in the text of these five Appendices (and, for that matter, in the rest of the text) is the authors’ own responsibility. Paulo André Gonçalves acknowledges the Calouste Gulbenkian Foundation for financial support through the grant “Prémio Estímulo à Investigação 2013 "1 (No. 132394) and the hospitality of the Centre of Physics of the University of Minho, where most of this book was written. Nuno Peres acknowledges financial support from the Graphene Flagship Project (Contract No. CNECT-ICT-604391).

1 "Gulbenkian

Prize for Stimulating Young Researchers 2013". xiii

page xiii

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

May 2, 2013 14:6 BC: 8831 - Probability and Statistical Theory

This page intentionally left blank

PST˙ws

June 16, 2016

10:32

An Introduction to Graphene Plasmonics

9in x 6in

b2445

page xv

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Errata can be found at http://www.worldscientific.com/worldscibooks/10.1142/9948

Contents

Foreword

vii

Preface

ix

Acknowledgments

xiii

List of Figures

xxiii

List of Tables

xxix

1.

2.

Introduction

1

1.1 1.2

1 4

Plasmonics: Generalities . . . . . . . . . . . . . . . . . . . Plasmonics: Recent Developments . . . . . . . . . . . . .

Electromagnetic Properties of Solids in a Nutshell

11

2.1

11 11 14 14 17 17 24 28

2.2 2.3

2.4

Classical Electrodynamics Basics . . . . . . . . . . . . . . 2.1.1 Maxwell’s equations . . . . . . . . . . . . . . . . . 2.1.2 Boundary conditions . . . . . . . . . . . . . . . . . Drude Model . . . . . . . . . . . . . . . . . . . . . . . . . Preliminaries to Graphene Plasmonics . . . . . . . . . . . 2.3.1 Elementary electronic properties . . . . . . . . . 2.3.2 The optical conductivity of graphene . . . . . . . 2.3.3 Lindhard function: Beyond the local approximation 2.3.4 Lindhard polarization function in relaxation-time approximation: The case of graphene . . . . . . . The Transfer-Matrix Method and the First Appearance of Plasmons in Graphene . . . . . . . . . . . . . . . . . . . . 2.4.1 Transfer-matrix for a graphene monolayer . . . . . xv

33 35 36

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

xvi

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

2.4.3 2.4.4 2.4.5

Transmittance, reflectance and absorbance of electromagnetic radiation by a graphene monolayer . Transfer-matrix for a graphene double-layer . . . . Transfer-matrix for multi-layer graphene structures Plasmons: A transfer-matrix approach . . . . . . .

Surface Plasmon-Polaritons at Dielectric-Metal Interfaces 3.1

3.2

3.3 4.

b2445-mas

An Introduction to Graphene Plasmonics

2.4.2

3.

9in x 6in

Single Dielectric-Metal Interface . . . . . . . . . . 3.1.1 Dispersion relation . . . . . . . . . . . . . 3.1.2 Propagation length and field confinement Multilayer Structures . . . . . . . . . . . . . . . . 3.2.1 Double Interface . . . . . . . . . . . . . . 3.2.2 Dispersion relation . . . . . . . . . . . . . A Short Note on Perfect Conductors . . . . . . .

. . . . . . .

39 40 42 45 47

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

47 48 54 57 57 59 64

Graphene Surface Plasmons

67

4.1

67 68 75 78 81 85 86 87 91

4.2

4.3

4.4

4.5

Monolayer Graphene . . . . . . . . . . . . . . . . . . . . . 4.1.1 Spectrum of GSPs . . . . . . . . . . . . . . . . . 4.1.2 Field profile of GSPs in single-layer graphene . . . 4.1.3 Plasmon dispersion revisited . . . . . . . . . . . . 4.1.4 Loss function . . . . . . . . . . . . . . . . . . . . 4.1.5 A word on TE surface waves . . . . . . . . . . . . Double-Layer Graphene . . . . . . . . . . . . . . . . . . . 4.2.1 Dispersion relation . . . . . . . . . . . . . . . . . . 4.2.2 Field profile of GSPs in double-layer graphene . . 4.2.3 Plasmon dispersion beyond the Drude model approximation . . . . . . . . . . . . . . . . . . . . . Surface Plasmon-Phonon-Polaritons in Graphene . . . . . 4.3.1 Graphene on SiC . . . . . . . . . . . . . . . . . . . 4.3.2 Graphene on SiO2 . . . . . . . . . . . . . . . . . . Magneto-Plasmons in Monolayer Graphene . . . . . . . . 4.4.1 Derivation of the spectrum’s condition . . . . . . . 4.4.2 Solution of the semi-classical spectrum’s condition in a special limit . . . . . . . . . . . . . . . . . . . 4.4.3 Spectrum of magneto-plasmons in the quantum regime: Landau quantization . . . . . . . . . . . . A Detour: Surface Phonon-Polaritons in hBN . . . . . . . 4.5.1 Solution of the electromagnetic problem . . . . . .

94 101 104 106 112 113 115 120 124 125

page xvi

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Contents

4.5.2

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

5.

5.2 5.3 5.4 5.5

. . . . of SO . . . . . . . . . . . . . . . . . . . . . . . .

7.3

7.4 7.5

8.2

132 134 134 140 142 143

Theoretical Model and Integral Equation . . . . . . . . . . 149 Approximate Solution via Fourier Expansion . . . . . . . 153 Results and Discussion . . . . . . . . . . . . . . . . . . . . 156

A Seminal Paper . . . . . . . . . . . . . . . . . . . . . Theoretical Model . . . . . . . . . . . . . . . . . . . . 7.2.1 Setting up the model . . . . . . . . . . . . . . 7.2.2 The scattering problem . . . . . . . . . . . . . Applications and Results . . . . . . . . . . . . . . . . . 7.3.1 Periodic array of graphene ribbons . . . . . . . 7.3.2 Theory versus experiment . . . . . . . . . . . . A THz Polarizer . . . . . . . . . . . . . . . . . . . . . Scattering From a Periodic Grid in the Regime kw < 1

163 . . . . . . . . .

. . . . . . . . .

Plasmons in Graphene Nanostructures and in Onedimensional Channels 8.1

131

149

Plasmonics in Periodic Arrays of Graphene Ribbons 7.1 7.2

8.

Grating Coupling . . . . . . . . . . . . . . . . . . . 5.1.1 Graphene on Gallium-Arsenide: The role phonons . . . . . . . . . . . . . . . . . . . . Prism Coupling . . . . . . . . . . . . . . . . . . . . 5.2.1 Otto configuration: Single-layer graphene . Near-field Excitation and Imaging of GSPs . . . . . Others . . . . . . . . . . . . . . . . . . . . . . . . . Excitation of SPP’s by a Moving Line of Charge .

131

Launching Plasmons Using a Metallic Antenna 6.1 6.2 6.3

7.

Guided phonon-polariton modes . . . . . . . . . . 128

Excitation of Graphene Surface Plasmons 5.1

6.

xvii

Edge Plasmons in a Graphene Nanoribbon . . . . . . . . 8.1.1 Prelude: Green’s functions for a 2-layered medium 8.1.2 Plasmonic spectrum of a graphene nanoribbon . . 8.1.3 An extension: magneto-plasmons in a graphene ribbon . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.4 Scattering of THz radiation by a graphene microribbon . . . . . . . . . . . . . . . . . . . . . . . . . Localized Surface Plasmons in a Graphene Ring . . . . .

163 167 167 170 172 172 178 183 185

193 195 196 199 210 211 218

page xvii

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

xviii

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

b2445-mas

An Introduction to Graphene Plasmonics

8.3 8.4

8.5

9.

9in x 6in

8.2.1 Spectrum of graphene plasmons in a graphene ring Plasmonic Excitations in a Graphene Nanodisk . . . . . . Scattering of Graphene Plasmons by a Conductivity Step 8.4.1 The mathematical problem . . . . . . . . . . . . . 8.4.2 Solution of the Riemann-Hilbert problem . . . . . 8.4.3 Further details . . . . . . . . . . . . . . . . . . . . 8.4.4 Calculation of the reflection amplitude . . . . . . 8.4.5 An alternative derivation of Eq. (8.137) . . . . . . Localized Surface Plasmons in a Graphene Sheet with a Gaussian Groove . . . . . . . . . . . . . . . . . . . . . . . 8.5.1 Few useful definitions . . . . . . . . . . . . . . . . 8.5.2 Formulation of the problem . . . . . . . . . . . . . 8.5.3 Green’s theorem, Green’s functions, and the eigenvalue problem . . . . . . . . . . . . . . . . . . . . 8.5.4 Spectrum of surface plasmon-polaritons in the presence of a Gaussian groove . . . . . . . . . . .

Excitation of Surface Plasmon-Polaritons Using Dielectric Gratings 9.1 9.2 9.3 9.4

9.5

Some Basic Definitions and Results . . . . . . . . . . . . . Tangent and Normal Vectors, and Boundary Conditions . A Trivial Example: Recovering Previous Results . . . . . The Fields in D+ and D− . . . . . . . . . . . . . . . . . . 9.4.1 Reflectance and transmittance efficiencies . . . . . 9.4.2 Particular limits for the transmittance and the reflectance . . . . . . . . . . . . . . . . . . . . . . . A Non-Trivial Example: A Grating with a Sine-Profile . .

10. Excitation of Plasmons by an Emitting Dipole 10.1 Statement of the Problem and a Bit of Electrostatics . . . 10.2 Calculation of the Non-Radiative Transition Rate: Particle-Hole Excitations Pathway . . . . . . . . . . . . . 10.3 Calculation of the Total Transition Rate: Full Electromagnetic Calculation . . . . . . . . . . . . . . . . . . . . . . . 10.4 Purcell Effect in Hyperbolic Materials . . . . . . . . . . .

218 232 239 241 242 244 245 247 250 251 253 254 259

267 268 270 271 272 274 274 275 281 282 287 289 292

11. Concluding Remarks

295

Appendix A

301

Derivation of the Susceptibility of Graphene

page xviii

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Contents

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

A.1

A.2

A.3

A.4

xix

Undoped Susceptibility . . . . . . . . . . . . . . . . . . . A.1.1 The imaginary part of the undoped susceptibility A.1.2 The real part of the undoped susceptibility . . . Doped Part: Fermi Sea Contributions . . . . . . . . . . A.2.1 Intraband term . . . . . . . . . . . . . . . . . . . A.2.2 Interband term . . . . . . . . . . . . . . . . . . . A.2.3 Imaginary part of χ1D . . . . . . . . . . . . . . . A.2.4 Imaginary part of χ2D . . . . . . . . . . . . . . . A.2.5 Real Part of χ1D and χ2D . . . . . . . . . . . . . Summary for the Real and Imaginary Parts of Graphene Susceptibility . . . . . . . . . . . . . . . . . . A.3.1 Real part of the susceptibility . . . . . . . . . . A.3.2 Imaginary part of the susceptibility . . . . . . . Some Useful Integrals . . . . . . . . . . . . . . . . . . .

. . . . . . . . .

301 302 303 303 303 304 306 306 307

. . . .

309 310 311 312

Appendix B Derivation of the Intra- and Inter-band Conductivity of Graphene

313

Appendix C

319

C.1 C.2

Inhomogeneous Drude Conductivity

Longitudinal Conductivity . . . . . . . . . . . . . . . . . . 320 Transverse Conductivity . . . . . . . . . . . . . . . . . . . 321

Appendix D Derivation of the Expression Relating the Longitudinal Conductivity with the Polarizability

323

Appendix E Derivation of the Polarization of Graphene in the Relaxation-Time Approximation

327

E.1 E.2 E.3 E.4 E.5

Hamiltonian and Particle and Current Densities . . . Local Equilibrium Density Matrix . . . . . . . . . . . A Useful Identity . . . . . . . . . . . . . . . . . . . . Equation of Motion for the Density Matrix . . . . . Polarization in the Relaxation-Time Approximation

Appendix F F.1 F.2

RPA for Double-Layer Graphene

. . . . .

. . . . .

. . . . .

327 328 330 330 332 333

Equation of Motion Method . . . . . . . . . . . . . . . . . 333 Diagrammatic Approach . . . . . . . . . . . . . . . . . . . 337

Appendix G

Effective Dielectric Constants for Coulomb-

page xix

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

xx

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Coupled Double-Layer Graphene

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Appendix H Appendix I I.1 I.2

Magneto-Optical Conductivity of Graphene Supplementary Material for Chapter 7

339 343 347

Derivation of the Expressions for the Transmittance and Reflectance . . . . . . . . . . . . . . . . . . . . . . . . . . 347 Modes Contributing to Each Resonance . . . . . . . . . . 349

Appendix J

The Method of Toigo

351

Appendix K

Boundary Condition in the Dipole Problem

355

Appendix L

Fourier Transform of the Dipole Potential

359

Appendix M

Non-Radiative Decaying Rate: Electrostatic Calculation361

M.1 Doped Graphene . . . . . . . . . . . . . . . . . . . . . . . 361 M.2 A Detour: Neutral Graphene . . . . . . . . . . . . . . . . 363 Appendix N Reflection Amplitude of an Electromagnetic Wave due to a Graphene Interface N.1 N.2

The Simple Case of Free Standing Graphene . . . . . . . 367 Reflection and Transmission Amplitudes: Fresnel Coefficients369 N.2.1 TE (transverse electric) / s−components . . . . . 372 N.2.2 TM (transverse magnetic) / p−components . . . . 373

Appendix O O.1 O.2

Green’s Functions in the Rope Problem

The Homogeneous Rope . . . . . . . . . . . . . . . . . . . O.1.1 Response to a localized force . . . . . . . . . . . . The Inhomogeneous Rope . . . . . . . . . . . . . . . . . . O.2.1 Reflection and transmition coefficients . . . . . . . O.2.2 Response to an external force in the inhomogeneous regime . . . . . . . . . . . . . . . . . . . . .

Appendix P Derivation of the Transition Rate of a Quantum Emitter Near an Interface P.1

367

375 375 375 377 377 378

383

Polarization Vectors and Green’s Functions . . . . . . . . 384

page xx

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Contents

Definition of s− and p−polarization vectors and angular spectrum representation . . . . . . . . . . P.1.2 The free space Green’s function . . . . . . . . . . P.1.3 Green’s functions for problems with flat interfaces I Dipole Decaying Rate . . . . . . . . . . . . . . . . . . . . Explicit Form of the Tensor Product of the Polarization Vectors . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Free Green’s Function in Real Space . . . . . . . . . . Green’s Function for Problems With Flat Interfaces II . . P.5.1 Free-space Green’s function revisited . . . . . . . . P.5.2 Electric field from a dipole in terms of Green’s functions . . . . . . . . . . . . . . . . . . . . . . . . . P.5.3 Green’s functions: s−component . . . . . . . . . . P.5.4 Green’s functions: p−component . . . . . . . . . . P.5.5 Derivation of the matrix structure of the Green’s functions . . . . . . . . . . . . . . . . . . . . . . .

xxi

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

P.1.1

P.2 P.3 P.4 P.5

384 386 388 391 392 393 394 394 395 396 398 399

Bibliography

403

Index

427

page xxi

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

May 2, 2013 14:6 BC: 8831 - Probability and Statistical Theory

This page intentionally left blank

PST˙ws

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

List of Figures

2.1 2.2 2.3 2.4 2.5 2.6 2.7 2.8

Real space and Brillouin zone of graphene. . . . . . . . . . . . Graphene’s band structure. . . . . . . . . . . . . . . . . . . . . Image of graphene viewed through an optical microscope. . . . Optical conductivity of graphene . . . . . . . . . . . . . . . . . Regions of the (q, ~ω)-space and contributions to the polarizability. Graphene’s 2D polarizability in the RT approximation. . . . . . Electromagnetic scattering at a single graphene 2D layer . . . . Transmittance, reflectance and absorbance of light through suspended single-layer graphene at normal incidence . . . . . . . . 2.9 Electromagnetic scattering at a graphene double-layer . . . . . 2.10 Transfer-matrix for multi-layer graphene structures . . . . . . . 2.11 Transmitance and reflectance of THz radiation across a N -layer graphene structure . . . . . . . . . . . . . . . . . . . . . . . . . 2.12 Intensity plots of the imaginary part of the Fresnel reflection coefficient indicating plasmons in single- and double-layer graphene

18 20 23 27 32 35 37

3.1 3.2

47

3.3 3.4 3.5 3.6 3.7 3.8

Dielectric-metal interface. . . . . . . . . . . . . . . . . . . . . . Dispersion relation of TM SPPs at a dielectric-metal interface (zero damping). . . . . . . . . . . . . . . . . . . . . . . . . . . . Dispersion relation of TM SPPs in air/Ag and SiO2 /Ag interfaces (finite damping). . . . . . . . . . . . . . . . . . . . . . . . 0 is the elementary charge. We are now looking for a steadystate solution exhibiting the same harmonic time dependence of the driving field, so that the Fourier transform of equation (2.27) yields − iωp(ω) = −

p(ω) − eE(ω) , τ

(2.28)

whose solution is eE(ω) . (2.29) iω − τ −1 Moreover, notice that the current density due to ne electrons per unit volume, travelling with net velocity v, is J = −ene v. Hence, one can write p(ω) =

J(ω) = −

ene p(ω) e2 ne 1 E(ω) , = me me γ − iω

(2.30)

where me is the mass of the electron and we have introduced the scattering rate, defined as γ = τ −1 . By comparing the result (2.30) with the relation (2.9), an expression for the optical conductivity can be determined: σ(ω) =

e2 ne /me . γ − iω

(2.31)

It will be useful for what follows to note that the conductivity and the dielectric function are linked through the following relationship2 σ(ω) , 0 ω

(2.32)

ωp2 , ω 2 + iγω

(2.33)

(ω) = 1 + i allowing us to write (ω) = 1 − where ωp2 =

e 2 ne me 0

denotes the plasma frequency of the free electron gas.

Despite its simplicity, the Drude model provides fairly good results for 2 This can be readily shown by working through Maxwell’s equation using the constitutive relation (2.30) [Ashcroft and Mermin (1976)].

page 15

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

16

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

many metals (specially alkali metals) in the infrared region of the electromagnetic spectrum, where their optical properties are frequently dominated by the role of intraband transitions. For noble metals, the model fails to a great extent due to the onset of interband transitions in the visible and ultraviolet regions, and to other details of the band structure. The interband transitions can be accounted for, while maintaining the classical picture, by adding a resonant contribution (whose resonant frequency corresponds to the transition energy) to the equation of motion, leading to a dielectric function which also contains a Lorentz-oscillator term. Nevertheless, a fully and accurate description of the physics governing the optical response of metals requires a quantum mechanical formulation. Still, this is often circumvented by employing clever effective/phenomenological parameters and/or extra terms added “by hand”. Let us end this section with a note on the longitudinal and transverse dielectric functions. From Maxwell’s equations it is not difficult to show [Li and Chu (2014)] that each component of the electric field obeys the wave equation [k 2 δij − ki kj − ij ω 2 /c2 ]Ej = 0, where k is the modulus of the wavevector k, ω is the frequency of the radiation, c is the velocity of light and ij is the dielectric tensor. Expressing, for an isotropic medium, the dielectric tensor3 as ij = (δij − ki kj /k 2 )t + ki kj /k 2 l , where t and l are the transverse and longitudinal components of the dielectric tensor, respectively. We can write a vector equation for the electric field in the form k × (k × E)(k 2 − ω 2 t /c2 ) + k(k · E)l = 0 .

(2.34)

Note that for finite k the dielectric function is a tensor even for an isotropic system [Wooten (1972)]. From the previous equation it is clear that a nontrivial solution for the existence of longitudinal waves requires the condition l (ω, k) = 0, where we have made explicit the dependence of the dielectric function on frequency and wavevector.4 For a two-dimensional system, the solution of the previous condition allow us to find the spectrum of the surface plasmons of the system [see, e.g., Eq. (4.61)]. For transverse fields the condition for their existence is [k 2 − ω 2 t (ω, k)/c2 ] = 0. 3 This is the most general tensor that can be built out of the vector k when the system is isotropic. For another way to intuit this result see footnote in Appendix D. 4 Note that for a bulk (three-dimensional) system, the previous condition gives the spectrum of the bulk plasmons (more on this on Chapter 3). For a two-dimensional system, such as graphene, the condition l (ω, k) = 0 grant us with the spectrum of the surface plasmons.

page 16

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Electromagnetic Properties of Solids in a Nutshell

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

2.3

b2445-mas

17

Preliminaries to Graphene Plasmonics

Graphene is a two-dimensional allotrope of carbon, where the carbon atoms are arranged in a honeycomb lattice. Being one-atom-thick, it can be regarded as a truly 2D material. Since its isolation in 2004 [Novoselov et al. (2004)], graphene has been capitalizing a lot of the scientific community’s attention due to its remarkable properties: it is stronger than steel and harder than diamond, but also flexible [Lee et al. (2008)]; it exhibits an extremely large thermal conductivity [Balandin et al. (2008)], and sustains high current densities; its charge carriers are massless Dirac fermions obeying a Dirac-like relativistic equation (more on this in what follows), showing ballistic transport with large electronic mobilities [Bolotin et al. (2008)] even at room temperature; and the list of properties goes on [Geim (2009)]. Owing to these unique properties, graphene has been dubbed a “wonder material”. Whether graphene will fulfill all the promises for new applications remains to be seen. For a prehistoric perspective about graphene see [Geim (2012)]. 2.3.1

Elementary electronic properties

For the sake of completeness and self-containedness of the text, this section introduces a few basic notions about graphene’s electronic and optical properties. However, this section is not meant to be a comprehensive presentation. The electronic configuration of a carbon atom is [C] = 1s2 2s2 2p2 .

(2.35)

Now, in what concerns graphene, three electrons from the 2s and 2p orbitals participate in the σ-bonds resulting from the hybridization of the sp2 orbitals, which in turn originate from the hybridization of the 2s, 2px , and 2py atomic orbitals. The remaining electron populates the 2pz orbital, and the hybridization of these orbitals originates the π-bonds, which lie above and below the graphene lattice. Thus, from the point of view of the π-orbitals, graphene is a half-filled electronic system, since each carbon atom has an associated electron. The hopping of the electrons along the π-orbitals allow us to define a tight-binding Hamiltonian for the system, from which the electronic and optical properties of the material follow. The minimal model Hamiltonian considers electron-hopping between nearest neighbors carbon atoms in the graphene lattice (see Fig. 2.1). In

page 17

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

18

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Figure 2.1: Real space and Brillouin zone of graphene. Top: Real space lattice of graphene together with the Wigner-Seitz cell (in pink color). The parameters t ' −2.7 eV and a0 ' 1.42 Å are the hopping integral and the carbon-carbon √ distance, respectively. The vectors a1 = √ a(1, 0) and a2 = a(−1/2, 3/2) are the primitive lattice-vectors, where a = a0 3. Bottom: Wigner-Seitz cell (in green) 0 and Brillouin zone (in pink) of graphene. The two special points K and K are

termed Dirac points. The vectors G1 =

4π √ a 3

√ 3 1 ,2 2

and G2 =

4π √ (0, 1) a 3

are the

primitive reciprocal-lattice vectors.

the Wannier basis, this Hamiltonian is written [Castro Neto et al. (2009); Peres (2010); Abergel et al. (2010)] as X H=t {|A, Ri [hB, R + δ1 | + hB, R + δ2 | + hB, R + δ3 |] + H.c.} , R

(2.36) where |A, Ri is the Wannier state in the carbon atom located at position R, in the sub-lattice A, and an equivalent definition holds for |B, R+δi i, where δi , with i = 1, 2, 3, are the vectors connecting a given carbon atom in sublattice A with its the three nearest neighbors carbon atoms in sub-lattice B. Here, H.c. stands for the Hermitian-conjugate. Next, we introduce

page 18

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Electromagnetic Properties of Solids in a Nutshell

b2445-mas

19

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

the representation of the Wannier states in terms of the Bloch states, of wavevector k = (kx , ky ), in the above Hamiltonian, thereby obtaining X H=t [|A, kihB, k|φ(k) + H.c.] , (2.37) k

which can also be written as H = Hk = and

Φ†k Hk Φk , where Φ†k = [|A, ki, |B, ki], 0 tφ(k) , (2.38) tφ∗ (k) 0 P

k

√

√

(2.39) φ(k) = eiky a0 + eikx 3a0 /2 e−iky a0 /2 + e−ikx 3a0 /2 e−iky a0 /2 , √ where a0 = a/ 3 is the carbon-carbon distance as defined in Fig. 2.1. It follows from Eq. (2.38) that the spectrum of the π-electrons is then given by Ek = ±t|φ(k)| , or, more explicitly, s

(2.40)

√ 3 3 kx a0 cos ky a0 . (2.41) 3kx a0 + 4 cos 2 2 Thus, we conclude that the spectrum is particle-hole symmetric. Furthermore, since the system is half-filled, the valence band Ek = −t|φ(k)| is completely filled and the conduction band Ek = t|φ(k)| is empty. A plot of the band structure of graphene is given in Fig. 2.2. From this figure it is clear that the valence and conduction bands touch each other at six points in the Brillouin zone. Since each point is shared by three Brillouin zones, we have two independent Dirac points (or Dirac cones, named after the shape of the spectrum in their vicinity; see right panel of Fig. 2.2). When we zoom-in close to one of the Dirac points, we see that the bands are conical. This hints that the low energy (around the Dirac point) Hamiltonian cannot be described by the usual effective-mass approximation used for semiconductors. Let us now derive the low energy Hamiltonian. We start by writing k = K + q, where K is the wavevector of the Dirac point and |q|/|K| 1, from where it follows that Ek = ±t 3 + 2 cos

√

φ(k) = eiq·δ1 + ei2π/3 eiq·δ2 + e−i2π/3 eiq·δ3 .

(2.42)

Expanding φ(k) to first order in q, we have φ(k) ≈ iq · δ1 + ei2π/3 iq · δ2 + e−i2π/3 iq · δ3 , and using the explicit values of δi , we thereby obtain 3 3 φ(k) ≈ a0 iqy − a0 qx . 2 2

(2.43)

(2.44)

page 19

April 5, 2016

14:13

20

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

k ya 0

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

k xa 0

Figure 2.2: Band structure of graphene, as given by Ek = ±t|φ(k)| [see Eqs. (2.40) and (2.41)]. Left: note that the valence and conduction bands touch each other at six-points in the Brillouin zone. These particular points of high-symmetry are termed Dirac points and correspond to the momentum values given by K and K0 (see Fig. 2.1). Right: close-up of the band structure near one of the Dirac points.

With this, the Hamiltonian (2.38) then becomes 3 0 −qx + iqy , Hk ≈ a0 t −qx − iqy 0 2

(2.45)

0 which leads to the spectrum E± (q) ≈ ± 3ta 2 |q| = vF p (up to first order in q/K), where p = ~q, and vF ≈ c/300 is the Fermi velocity, where c refers to the speed of light in vacuum. Notice that the electronic spectrum can be written only in terms of q, that is, the momentum measured with respect to the Dirac points. The Hamiltonian Hk is written in momentum space. We now want to write the corresponding Hamiltonian in real space. Since Hk is linear in q, intuition dictates that we should replace the momentum by spatial derivatives. We are then led to write 3 3ta0 0 i∂x + ∂y H = a0 t =− (σx px + σy py ) = −vF σ · p , i∂x − ∂y 0 2 2~

(2.46) where σx and σy are the Pauli matrices and the momentum operator is p = (px , py ). Clearly, the Hamiltonian (2.46) resembles the massless Dirac

page 20

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Electromagnetic Properties of Solids in a Nutshell

b2445-mas

21

Hamiltonian in two spatial dimensions. This justifies the terminology used above when referring to K and K0 as “Dirac points”. We can now work backwards and solve the eigenvalue problem Hψ = Eψ, where H is given by Eq. (2.46). To this end, we write 1 1 aα ψq,α (r) = √ (2.47) eiq·r = √ χα eiq·r , A bα A leading to an eigenvalue problem of the form 3 0 qx − iqy aα aα a0 t = Eq,α , (2.48) qx + iqy 0 bα bα 2 whose solution is 1 χα = √ 2

e−iθq /2 αeiθq /2

,

(2.49)

with eigenvalues E± (q) = ±~vF q ,

(2.50)

where in the above equations, A stands for the area of the system, α = sgn(E) is the band index, and θq = arctan (qy /qx ). As Eq. (2.50) plainly demonstrates, the dispersion of the Dirac fermions in graphene is linear with momentum, in the vicinity of the Dirac points. This result has many important implications, and will also have an impact on the dispersion of plasmons in graphene, as will become clear in later chapters. As an application of the previous solution, let us compute the transmittance of pristine graphene (a more complex application of the above results is done in Chap. 10). The physical idea is simple: an electron in the valence band is excited to the conduction band by the absorption of a photon of angular frequency ω. Since the conduction band is empty and the system has no energy gap, the electron can absorb a photon of an arbitrary low frequency. The rate per unit area at which the material absorbs energy from the electromagnetic field can be computed from Fermi’s golden rule [Zettili (2009)]. The coupling of the electrons to the electromagnetic field is made via the usual minimal coupling. Within this framework, we write the Hamiltonian as H = vF σ · (p + eA) ,

(2.51)

where A is the vector potential and e > 0 the elementary charge. We now choose the form of the vector potential as 1 (2.52) A = (A0 , 0)(eiωt + e−iωt ) , 2

page 21

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

22

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

which is appropriate for describing a monochromatic plane wave. In the spirit of first-order time-dependent perturbation theory, the perturbation, V , reads A0 V = evF σx . (2.53) 2 The wavefunctions to be used in the calculation of the matrix element of the perturbation are [cf. Eqs. (2.47) and (2.49)] −iθ /2 1 e q √ eiq·r , (2.54) ψ− (r) = iθq /2 −e 2A for the valence band and 1 ψ+ (r) = √ 2A

e−iθq /2 eiθq /2

eiq·r ,

(2.55)

for the conduction band. Thus, the matrix element of the perturbation can be readily determined, ivF e sin θ , (2.56) hψ+ |V |ψ− i = −A0 2 so that the transition rate, as given by Fermi’s golden rule, follows: 2π vF2 2 2 2 e A0 sin θ δ(2~vF k − ~ω) . (2.57) ~ 4 The rate of transition, W+− (k), is associated to a single momentum value, p = ~k. We now have to sum over all the momentum values in the Brillouin zone, and account for the spin degeneracy and for the existence of two Dirac points as well (also dubbed as valley degeneracy). Then, the total transition rate is Z 1 dk e2 |A0 |2 ω =4 W (k) = , (2.58) +− τ (2π)2 8~2 W+− (k) =

where the factor of four is due to the spin and valley degeneracies mentioned above. Therefore, from the previous equation, the power per unit area absorbed by the material reads ~ω e2 E02 = , (2.59) τ 8~ where we have expressed the amplitude of the vector potential A0 in terms of the corresponding amplitude of the external electric field E0 (A0 = −iE0 /ω). On the other hand, the power flux per unit area contained in the field is given by 1 Wi = c0 E02 . (2.60) 2 Wa =

page 22

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Electromagnetic Properties of Solids in a Nutshell

b2445-mas

23

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Having the quantities (2.59) and (2.60), we can obtain the transmittance of graphene via T =1−

Wa = 1 − πα ' 97.7% , Wi

(2.61)

where α = e2 /(4π0 ~c) is the fine structure constant of atomic physics. From the previous result, we conclude that the transmittance of graphene is independent of the frequency of the impinging radiation and also independent of any other material’s parameters. Naturally, this result holds

Figure 2.3: A hole drilled in a metallic scaffold is partially covered by graphene and its bilayer. The hole is illuminated by white light from behind. The covering of the hole is, from left to right, air, monolayer graphene, bilayer graphene. We can see by contrast the presence of the single and bilayer graphene sheets, due to the absorption of 2.3%/layer of the impinging radiation. The greyish colour is a consequence of the independence of the transmittance on the frequency of the incoming radiation (image courtesy of A. K. Geim).

true only as long as the momentum expansion around the Dirac point remains valid, and only applies to neutral (undoped) graphene. In Fig. 2.3 we show a graphene sheet (and its bilayer) partially covering a hole drilled in a metallic scaffold. Due to the absorption of 2.3% of the impinging radiation (reflection is negligible) we can see with the bare eye a single graphene sheet. Interesting enough, the previous result for the transmittance allow us to compute the conductivity of graphene. It is known that the transmittance

page 23

April 5, 2016

14:13

24

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

through a thin conducting film relates to the conductivity through5

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

T = 1/|1 + σ(ω)/(2c0 )|2 ,

(2.62)

where 0 is the vacuum permittivity. Since we have computed T we can invert this latter equation and obtain σ(ω). This procedure leads to6 σ(ω) = πe2 /2h ≡ σ0 ,

(2.63)

that is, a constant value, independent of the material parameters (a situation not very common in condensed matter). If the effect of temperature is included, then the conductivity of graphene has the form ~ω , (2.64) σ(ω, T ) = σ0 tanh 4kB T where the hyperbolic tangent is a consequence of the Fermi distribution function. For doped graphene at finite temperature, the previous expression further transforms to 1 ~ω + 2EF ~ω − 2EF σ(ω, T ) = σ0 tanh + tanh , (2.65) 2 4kB T 4kB T where EF is the Fermi energy. This latter expression includes only interband transitions. The intraband transitions can be described by the Drude model. The conductivity of graphene will be discussed ahead in more detail, specially the case of doped graphene, which we have considered here only in passing. In this book, we shall focus on graphene as being a plasmonic material. As far as graphene plasmonics is concerned, all we need to describe its electromagnetic properties and light-matter interactions is encompassed within graphene’s optical conductivity (which in turn could be extended to include non-local effects—more on this in Sec. 2.3.3). For a detailed treatment of graphene physics, please refer to [Geim (2009); Castro Neto et al. (2009); Peres (2010)]. 2.3.2

The optical conductivity of graphene

Along with its linear dispersion, graphene’s optical conductivity is the key ingredient in graphene optics and plasmonics, since it contains all the relevant information on the physics governing the electromagnetic interactions 5 See

derivation in Appendix N. reader should not confuse σ0 with the quantum of conductance. σ0 is termed the universal AC conductivity of graphene. 6 The

page 24

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Electromagnetic Properties of Solids in a Nutshell

b2445-mas

25

between graphene and external stimuli such as electromagnetic radiation or fast electrons. In order to better characterize the conductivity, it is useful to split this physical quantity into two distinct contributions: one describing intraband transitions (transitions within the conduction (or valence) band where the momentum is not conserved), and another accounting for interband transitions (vertical transitions from the valence to the conduction band, in which case there is momentum conservation), namely σg (ω) = σintra (ω) + σinter (ω) .

(2.66)

In writing the last expression it is implicit that we will ignore spatial dispersion (i.e. non-local effects) henceforth (later, non-local effects will be introduced). An analytical expression for the dynamical conductivity of graphene can be obtained under the framework of linear response theory and is computed via Kubo’s formula [Falkovsky and Varlamov (2007); Falkovsky (2008); Stauber et al. (2008); Wunsch et al. (2006); Gusynin et al. (2009)], using some sort of approximation. Traditionally the bare bubble [Mahan (2000)], which is related to the charge-charge susceptibility (or polarizability), is computed. Within the latter approach we have7 h i 4 σ0 EF + 2kB T ln 1 + e−EF /kB T , (2.67) σintra (ω) = π ~γ − i~ω characterizing intraband processes, where σ0 = e2 /(4~), kB is Boltzmann’s constant, γ is the relaxation rate (see discussion below), and EF the Fermi energy, while for interband transitions we have Z G(E) − G(~ω/2) 4~ω ∞ σinter (ω) = σ0 G(~ω/2) + i dE , (2.68) π 0 (~ω)2 − 4E 2 with x sinh k T B . G(x) = (2.69) EF x cosh + cosh kB T kB T At zero temperature, or as long as the condition EF kB T is fulfilled, the above equations reduce to σ0 4EF , (2.70) σintra (ω) = π ~γ − i~ω i ~ω − 2EF σinter (ω) = σ0 Θ(~ω − 2EF ) + ln , (2.71) π ~ω + 2EF 7A

derivation of Eqs. (2.67) and (2.68) is given in Appendix B.

page 25

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

26

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

where Θ(x) stands for the Heaviside step-function. Notice that for 2EF > ~ω the term describing interband transitions gives a negligible contribution to the conductivity due to Pauli blocking. Therefore, we note that for frequencies in the terahertz (THz) and mid-IR spectral region, at room temperature, and under typical doping levels, graphene’s optical conductivity is mostly dominated by the term describing intraband electronic processes, following a Drude-like expression [Stauber et al. (2007); Peres et al. (2007)]

σg (ω) ≈

σ0 4EF . π ~γ − i~ω

(2.72)

The results for the (local) optical conductivity of graphene are summarized in Fig. 2.4. We note, however, that in some conditions the previous expressions for the local conductivity are not enough and we are forced to use an expression for graphene’s dynamical conductivity including nonlocal effects8 . For example, it can be shown that the value of the decay length of surface plasmons as they propagate along a graphene sheet, depends on whether we use the local (homogeneous) or the non-local (nonhomogeneous) conductivity. Another important remark regards the interpretation of γ in the previous expressions for the conductivity. From an experimental point of view, γ should be considered as a phenomenological parameter that one uses to fit the experiments and that includes the different pathways by which an excited electron can relax to the ground state. On the other hand, from a theoretical point a view, the calculation of γ from first principles is an important and complex task, but which, in the end, should agree with the experimentally obtained value. Clearly, γ will depend on intrinsic aspects of the physics of graphene, such as electron-impurity, electron-phonon, and electron-electron interactions [Principi et al. (2013)], but it will also depend on extrinsic aspects, such as the substrate on which graphene is deposited. Whether the calculated value of γ will agree with its phenomenological counterpart remains an open question. We now turn to the discussion of the non-local conductivity of graphene, as computed from Kubo’s formula. In addition, we will also consider an extension of the bare polarizability that includes the effects of relaxation due to γ. 8 See Appendix C for a derivation of the non-local optical conductivity of graphene in the context of Drude model. We shal use these results in Chap. 10.

page 26

April 8, 2016

11:53

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Electromagnetic Properties of Solids in a Nutshell

27

2.5

a)

1.5 1 0.5 0 -0.5 -1 -1.5 -2

0

1

0.5

2

1.5

2.5

125

3

3.5

c)

b)

Re{σ(ω)}, Kubo Im{σ(ω)}, Kubo Re{σ(ω)}, Drude Im{σ(ω)}, Drude

100

intraband

75

interband

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

2

50

25

0

0

0.02

0.04

0.06

0.08

0.1

Figure 2.4: Optical conductivity of graphene: a) real and imaginary parts of the conductivity computed using the local (that is, in long-wavelength limit) Kubo expression [Eqs. (2.67) and (2.68)] at T = 300 K (solid lines) and at T = 0 K (dashed lines); b) graphene’s optical conductivity in the THz regime, obtained via Kubo’s formula (solid lines) and using Drude’s expression (2.72) (dashed); c) schematic illustration of the transition processes in doped graphene. Parameters: EF = 0.3 eV and ~γ = 3.7 meV. Cross over the arrows indicate processes prevented by Pauli blocking.

page 27

April 5, 2016

14:13

28

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

2.3.3

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Lindhard function: Beyond the local approximation

In the preceding subsection we have shown that, for typical values of doping (EF ∼0.2-0.5 eV), the conductivity of graphene in the THz and mid-IR is well described by the Drude model expression, given by Eq. (2.72), and ignoring non-local effects. This conclusion is also supported by a number of experimental works [Lee et al. (2011); Rouhi et al. (2012); Sule et al. (2014)], which have reported that in the spectral range spanning 100 GHz – 10 THz the optical response of the material is well described by the Drude model [Sule et al. (2014)]. These results do give confidence in the theoretical description of SPP in graphene based on the Drude model (in that window of the electromagnetic spectrum, and up to the mid-IR for samples with higher doping concentrations). While the simple description of the optical (frequency-dependent) conductivity of graphene suffices for most experimental and theoretical scenarios, one needs to be equipped with a more general theory for situations falling outside the aforementioned regime or in circumstances where q-dependent, that is non-local effects, emerge, such as in the case of graphene surface plasmons (GSPs) with large wavevectors approaching kF = EF /(~vF ) and for a quantum emitter in the vicinity of a graphene sheet (see Chap. 10). One of the most popular models in the nanophotonics community capable of delivering the dependence of the linear response on the entire (q,ω)space is the Lindhard dielectric function [Lindhard (1954)], which can be obtained from the polarization bubble. The Lindhard dielectric function is also often dubbed as the dielectric function in the random-phase approximation (RPA) [Mahan (2000)]. This theoretical framework follows from a microscopic, quantum mechanical (perturbative) description, whose main assumption is that the electrons respond not to the bare Coulomb potential, VC , but to an effective potential — Veff (q, ω) = VC (q, ω) + Vs (q, ω) (here written in Fourier space) — comprising both VC and the screening potential, Vs , produced by the electronic polarization, resulting from the dynamical rearrangement of charges in response to VC . Note that this model includes electron-electron interactions by virtue of the screening interaction term. The random-phase approximation can be obtained either by writing the Hamiltonian of the electron gas in the presence of an external potential and solving the equation of motion9 using a self-consistent method for the 9 The derivation follows along the lines of Appendix F, which provides the calculation of the same quantity for double-layer graphene.

page 28

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Electromagnetic Properties of Solids in a Nutshell

b2445-mas

29

potential [Ehrenreich and Cohen (1959)], or by the diagrammatic technique using Green’s functions [Mahan (2000)]. In what follows, we will summarize the procedure towards the calculation of the bare polarizability (or noninteracting dynamical susceptibility) of graphene, which will allow us to compute the RPA dielectric function. The interested reader is thus advised to refer to G. Mahan’s textbook on many-body physics [Mahan (2000)] for further details (where the RPA results for the 3D electron gas are given). In addition, a thorough description of the derivation of the 2D polarizability of graphene can be found in [Wunsch et al. (2006); Hwang and Sarma (2007)] and in the textbook by Jishi [Jishi (2014)] (see also [Mihaila (2011)]). Generically, the retarded density-density correlation function may be defined as10 i χρρ (r − r0 , t − t0 ) = − Θ(t − t0 ) h[n(r, t), n(r0 , t0 )]i , ~

(2.73)

together with its momentum space version, i χρρ (q, t − t0 ) = − Θ(t − t0 ) h[n(q, t), n(−q, t0 )]i , ~

(2.74)

corresponding to the Fourier transformed response function with respect to P the spatial coordinate, with n(q, t) = kσ c†kσ (t)ck+qσ (t) being the electronic density operator written in the second quantization formalism11 . In the language of quantum field theories, Eq. (2.74) simply relates the probability amplitude for an electron-hole pair created at time t0 with momentum q (and spin σ), to be found at a later time t with the same momentum (and spin). During its propagation, the pair can experience a number of scattering processes owing to electron-electron interactions (e.g. represented by self-energies and vertex correction diagrams [Fetter and Walecka (2003); Mahan (2000); Abedinpour et al. (2011)]). The random-phase approximation ignores these corrections, and approximates the proper density-density correlation function by the summation of all bare bubble diagrams connected by Coulomb lines. Working from Eq. (2.74) and to lowest order in perturbation theory, one arrives to the 2D polarizability12 at finite doping, defined by the non-interacting (bare) bubble diagram as [Wunsch et al. 10 The retarded “two-point” correlation function preserves causality (the system’s response is only triggered after the perturbation is switched on, hence the name). We further assume a translational invariant system, so that the response function only depends on the difference between spatial variables, i.e. χρρ (r, r0 , t−t0 ) ≡ χρρ (r−r0 , t−t0 ). 11 This form of n(q, t) holds for the jellium model [Fetter and Walecka (2003)]. 12 An explicit calculation of the integrals in Eq. (2.75) is given in Appendix A.

page 29

April 5, 2016

14:13

30

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

(2006); Shung (1986); Hwang and Sarma (2007); Jablan et al. (2009)] χ0ρρ (q, ω) ≡ P (q, ω) Z 1 d2 k = 2 π

X

Fα,α0 (k, q)

α,α0 =±1

fα (k) − fα0 (|k + q|) , ~ω + Eα (k) − Eα0 (|k + q|) + iη (2.75)

with the energies being E± (k) = ±~vF k − EF , and f± (k) = E (k)/k T −1 B e ± +1 expresses the Fermi-Dirac distribution, and where the form factor 2 1 0 k + kq cos θ Fα,α0 (k, q) = 1 + αα , (2.76) 2 k|k + q| comes from the overlap of the wavefunctions of Dirac electrons [see Eq. (2.47)], and θ refers to the angle formed by the wavevectors k and q. Additionally, we note that in writing Eq. (2.75) we have already included the spin (gs = 2) and valley (gv = 2) degeneracies. At T = 0 K the Fermi distributions reduce to step functions, easing the evaluation of the integral in Eq. (2.75). Furthermore, one may apply Sokhotsky’s formula13 to the polarizability (2.75), thereby separating its real and imaginary parts, P (q, ω) = Pre (q, ω) + iPim (q, ω) ,

(2.77)

and then computing Pre (q, ω) and Pim (q, ω) separately. After some lengthy algebra (see Appendix A), these read: 2k y+2 2−y 1 kF √ x2 − π~vFF + 4π C − C , in region 1B h h ~v x x 2 2 F y −x − 2kF , in region 1A π~vF Pre (x, y) = , y+2 2kF 1 kF √ x2 , in region 2B − π~vF + 4π ~vF y2 −x2 Ch x − 2kF + 1 kF √ x2 C 2−y , in region 2A π~vF 4π ~vF x 2 2 x −y

(2.78) for the real part of the polarizability, and 0 2 1 kF √ x Ch 2−y − Ch 4π ~vF x 2 2 x −y 2 Pim (x, y) = 1 kF √ x C 2−y 4π ~vF x y 2 −x2 1 kF √ x2 − 4π Ch y+2 ~v x 2 2 F

x −y

, in region 1B y+2 x

, in region 1A , in region 2B

,

, in region 2A (2.79)

13 Sokhotsky’s

1 limη→0+ x+iη

result: principal value [Vladimirov (1971)].

= P

1 x

− iπδ(x), where P denotes the Cauchy

page 30

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Electromagnetic Properties of Solids in a Nutshell

b2445-mas

31

for the corresponding imaginary part. Note that both quantities are defined by branches, whose domains are depicted in 2.5. Also, in writing Eqs. (2.78) and (2.79) we have defined x = q/kF , y = ~ω/EF , as well as the (real) auxiliary functions p Ch (a) = a a2 − 1 − arccosh(a) , (2.80) p C(a) = a 1 − a2 − arccos(a) . (2.81) At this point, let us anticipate that long-lived plasmons can only exist in region 1B, that is, where ={P (q, ω)} = 0. Outside this region, the imaginary part of the polarizability (which relates to absorption) is non-zero and the plasmons become severely damped, quickly decaying into excited electron-hole pairs. For this reason, zones 2B, 2A and 1A are usually designated by electron-hole continuum or Landau damping 14 regions (interband Landau damping takes place in region 2B, whilst areas 2A and 1A lie in the intraband Landau damping regime—see Fig. 2.5). The results contained in Eqs. (2.77)-(2.79) describe the bare polarizability of doped graphene, in the whole (q, ω)-plane depicted in Fig. 2.5. Having finally obtained the response function P (q, ω), we find ourselves just a stone’s throw away from building the RPA dielectric function and the full, non-local, conductivity. Once in possession of these quantities, we have all the essential ingredients to fully characterize and compute the spectrum of plasmonic excitations in graphene. The RPA dielectric function can be written in terms of the Lindhard polarization as [Mahan (2000)] εRPA (q, ω) = r − νq P (q, ω) , 14 This

(2.82)

terminology is somewhat loose. Strictly speaking, Landau damping is a reversible process occurring when the phase velocity of an electromagnetic wave (SPP, in our case) matches that of a free electron. The electrons moving slightly slower than the wave are accelerated and remove energy from the wave. The condition for it to occur is vphase = ~ω/q ≤ vF (where vF is the Fermi velocity). Thus, the region on the right of the line ~ω = ~qvF is where Landau damping can take place (see regions 1A and 2A in Fig. 2.5). Alternatively, SPPs can lose their energy by creating electron-hole pairs. Contrary to usual electromagnetic wave (free radiation), SPPs have large momenta and can participate in indirect (or non-vertical) interband electron-hole transitions. The minimal energy of an electron-hole pair in doped graphene is Ee−h = 2EF −~qvF , where q is the total momentum of the pair (see Fig. 2.5 – region 2B). Therefore it becomes possible to satisfy the momentum and energy conservation restriction for creation of an electron-hole pairs at the expenses of one SPP when ~ω > 2EF − ~qvF and q ≤ kF . This process is somewhat different from Landau damping. It is just resonant absorption of plasmons by generation of electron-hole pairs. However, and despite this comment, we will keep using the terminology “Landau damping” in a broad sense to conform with its use in the literature on plasmons in graphene.

page 31

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

32

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Figure 2.5: Regions of the (q, ~ω)-space corresponding to the polarizability as given by Eqs. (2.78) and (2.79). Some of the processes characterizing the polarizability are also portrayed in a pictorial fashion.

where r is the relative permittivity of the medium in which graphene is 2 embedded, and νq = 2e0 q stands for the Fourier transform of the Coulomb interaction (here 0 denotes the permittivity of free space). Collective excitations coincide with the zeros of the dynamical dielectric function, that is, they correspond to solutions of the equation εRPA (q, ω) = 0. With this end in view, it is possible to calculate the dipersion of GSPs via [Wunsch et al. (2006); Jablan et al. (2009)] 2r 0 0 half-space is occupied by medium 2. The graphene sheet is located at the z = 0 plane.

4.1.1

Spectrum of GSPs

Let us assume a solution of Maxwell’s equations, in the form of a p-polarized electromagnetic wave (TM wave). As in Chapter 3, we use the ansatz Ej = (Ej,x x ˆ + Ej,z ˆ z) eiqx e−κj |z| , Bj = Bj,y e

iqx −κj |z|

e

y ˆ,

(4.1) (4.2)

where j = 1, 2 refers to the dielectric media with relative permittivities 1 , 2 . Equations (4.1) and (4.2) describe an electromagnetic surface wave which is confined to the neighborhood of the graphene sheet and propagates along the x ˆ-direction. Due to the translational invariance of the system, the linear momentum along the propagation direction must be conserved, enabling us to write q ≡ q1 = q2 . Moreover, we note that in writing these equations it should be understood that they correspond to the spatial components of the fields. The time dependence, in what follows, is assumed to be of the typical harmonic form, i.e. e−iωt . Introducing Eqs. (4.1) and (4.2) into Maxwell’s equations for dielectric media ∂Bj ∇ × Ej = − , (4.3) ∂t j ∂Ej ∇ × Bj = 2 , (4.4) c ∂t yields − sgn(z)κj Ej,x − iqEj,z = iωBj,y ,

(4.5)

2

(4.6)

2

(4.7)

sgn(z)κj Bj,y = −iωj /c Ej,x , iqBj,y = −iωj /c Ej,z ,

page 68

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Graphene Surface Plasmons

b2445-mas

69

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

which can be rewritten with respect to the magnetic field amplitudes, while also obtaining an expression for κj (q, ω) Ej,x = i sgn(z) Ej,z = −

κj c2 Bj,y , ωj

qc2 Bj,y , ωj

κ2j = q 2 − ω 2 j /c2 .

(4.8) (4.9) (4.10)

The boundary conditions linking the electromagnetic fields at z = 0 read1 E1,x (x, z)|z=0 = E2,x (x, z)|z=0 ,

(4.11)

B1,y (x, z)|z=0 − B2,y (x, z)|z=0 = µ0 Jx (x) = µ0 σxx E2,x (x, z)|z=0 , (4.12) which assures the continuity of the tangential component of the electric field and the discontinuity of the tangential component of the magnetic field across the interface. We emphasize that the conductivity of graphene enters in the boundary condition only. Note that is the case of metal-dielectric interface, the right-hand-side of Eq. (4.12) is zero (see Chap. 3). Additionally, we further assume that graphene is a truly two-dimensional material2 , whose entire electromagnetic properties are accounted in its frequencydependent conductivity, σ(ω). Letting σ(ω) ≡ σxx = σyy , meaning that graphene’s conductivity is isotropic (which is true for unstrained graphene) and substituting the fields into the boundary conditions (4.11) and (4.12), we arrive to 1 2 σ(ω) + +i =0 , κ1 (q, ω) κ2 (q, ω) ω0

(4.13)

which describes the dispersion relation, ω(q), of graphene TM surface plasmon-polaritons. The reader should note the difference between Eq. (4.13) and Eq. (3.14). Note that Eq. (4.13) is an implicit equation, in the sense that the conductivity depends on the frequency, and κj , given by Eq. (4.10), is a function of both SPP wavenumber, q, and frequency. Hence, despite the simple geometry of the system, the dispersion relation (4.13) does not have an analytical solution and must be solved by numerical means. In addition, it is clear that Eq. (4.13) only has real solutions when the imaginary part of the conductivity is positive and its real part vanishes. On the other hand, if the real part of the conductivity is non-zero, 1 Within

the linear response regime. This holds and gives accurate results in most situations. 2 In this case, the (surface) current density is given by J(r) = J (x, y)δ(z). s

page 69

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

70

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

then, in general, the solutions will be complex. We shall discuss both cases separately in the next paragraphs. Recall that, in the spectral region in which we are interested in this monograph —from the THz to the mid-IR regime— the conductivity of graphene is dominated by a Drude-type term3 σ(ω) = σ0

4i EF , π ~ω + i~γ

(4.14)

provided that EF kB T and EF ~ω (cf. Sec. 2.3.2). Figure 4.2 shows the spectrum of TM graphene surface plasmonpolaritons, obtained from the numerical solution of Eq. (4.13), where we have neglected absorption (that is, γ = 0). Note that, once again, the dispersion curves lie to the right of the light lines in the dielectrics (due to the bound nature of SPPs). Thus, as we have seen in Chapter 3 when we studied SPPs in dielectric-metal interfaces, it is not possible to excite GSPs simply by directly shining electromagnetic radiation onto the structure. Moreover, in this case (γ = 0), for doped graphene, the conductivity is a purely imaginary function of the frequency, so that the wavevector, q, coming out of Eq. (4.13) will be real. Conversely, in the general (and more realistic) case where absorption is present, i.e. for finite γ, the dispersion relation yields a complex-valued wavevector, q = q 0 + iq 00 , whose imaginary part characterizes the attenuation of the SPP, as we shall see further ahead in the text4 . In Fig. 4.3 we present the dispersion curve of TM SPPs in graphene, retrieved from Eq. (4.13) using different values for the damping parameter (γ) entering in the conductivity (4.14). From the figure it is apparent that the GSP dispersion relation is shifted toward higher frequencies with respect to the dispersion curve with Γ = ~γ = 0, and that this effect is larger 3 We want to stress that the use of the full non-homogeneous conductivity of graphene will originate results quantitatively different from those reported in this and the next section. The option for using here Drude’s conductivity relates to the simplicity of the obtained expressions. Qualitatively there are no appreciable changes. 4 Actually, considering a complex wavevector is not the only possibility. One can also consider a complex frequency and follow an alternative interpretation. If γ 6= 0, Eq. (4.13) yields two relations, which link ω and q where, generally speaking, both are complex quantities. One can take either of them as a real independent parameter, then Eq. (4.13) determines entirely the real and imaginary parts of the other. If we take q as independent (real) variable, we shall obtain ω =ω1 + iω2 and the imaginary part, ω2 , is the inverse of the lifetime of SPP eigenmodes (for a certain q). This is relevant to the situation where SPPs are excited by pulsed radiation. On the other hand, if we take ω as independent variable (continuous wave excitation of SPPs), the dispersion relation (4.13) yields a complex-valued eigenvector.

page 70

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

12

12

10

10

Frequency (THz)

Frequency (THz)

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Graphene Surface Plasmons

8 6 4 light (air) TM GSPs

2 0

0

0.4 0.8 1.2 1.6 -1

q (µm )

2

8 6 4 light (air) light (SiO2) TM GSPs

2

2.4

71

0

0

0.4 0.8 1.2 1.6 -1

2

2.4

q (µm )

Figure 4.2: Dispersion relation of TM graphene surface plasmon-polaritons (GSPs) in a dielectric/graphene/dielectric heterostructure, as depicted in Fig. 4.1. Left: free-standing graphene in air; right: air/graphene/SiO2 . Here graphene’s conductivity is assumed to be given by Eq. (4.14) without damping (γ = 0), so that the conductivity only has an imaginary part. We have used the following parameters: EF = 0.45 eV, air = 1 and SiO2 = 3.9.

as Γ increases. The value Γ = 3.7 meV corresponds to a typical damping parameter obtained from transport measurements [Li et al. (2008)], while Γ = 20 meV corresponds to a rather high value. Nevertheless, taking absorption into account only changes the spectrum significantly in the region of low wavevectors, shown in the inset of Fig. 4.3. Looking at this figure at first glance, one might think that it should be possible to excite GSPs directly using free-propagating electromagnetic beams, since the GSPs dispersion curves cross the light lines at some point. However, that is indeed not the case. Here, the usual reasoning fails because the region plotted in the inset of Fig. 4.3 falls within the overdamped regime (ωSP P /γ < 1), in which GSPs (and SPPs in general) cannot be sustained5 . We should stress that although the presence of a non-zero Γ does not significantly alter the aspect of the dispersion curve, it plays a leading role in the attenuation of SPPs, which increases with increasing Γ. Losses are often the main limiting factor in plasmonic-based systems, so that one usually wants a Γ value as small as possible [Yan et al. (2013); Khurgin and Boltasseva (2012)]. 5 In fact, for the higher Γ = 20 meV value, the overdamped regime extends beyond the inset of Fig. 4.3.

page 71

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

72

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

7 GSPs , Γ = 0 meV GSPs , Γ = 3.7 meV GSPs , Γ = 20 meV

Frequency (THz)

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

6 5

1

4

0.8

3

0.6

2

0.4 0.2

1 0

0

0

0.25

0.5

0.75

1

0

0.02

1.25

-1

1.5

0.04

1.75

0.06

2

Re{q} (µm )

Figure 4.3: TM GSPs dispersion curves obtained from Eq. (4.13) using different values for the damping parameter, Γ = ~γ. For comparison, we have also included the dispersion relation with Γ = 0 (orange dot-dashed curve). The dashed lines represent the light dispersion in the cladding dielectrics. The inset shows a closeup of the low-q 0 region (the axis labels are the same as in the main figure). Parameters: 1 = 3 (ion gel), 2 = 4 (SiO2 ) and EF = 0.45 eV.

Albeit by now we have essentially all we need in order to describe SPPs in single-layer graphene, in the end we still must rely on numerical means to solve Eq. (4.13). For pratical matters this does not constitute a problem per se, since any personal laptop will be able to compute the plasmonic spectrum with little effort. It is instructive, however, to analyze a couple of limits and simplifications where it is possible to obtain approximate expressions in closed-form. This will not only allow the reader to gain a deeper understanding of the theoretical framework, but also to build an intuition on the physics governing SPPs in graphene. We start by assuming that the graphene sheet is embedded in a symmetrical dielectric environment ( ≡ 1 = 2 ), which is the degenerate case of the more general situation where the dielectric constants of each media are replaced by their average value, i.e. = (1 + 2 )/2. In this limit, the dispersion relation (4.13) simplifies to σ(ω) p 2 q − ω 2 /c2 = 0 , (4.15) 1+i 2ω0

page 72

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Graphene Surface Plasmons

b2445-mas

73

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

but still needs to be solved numerically. On the other hand, in the non√ retarded regime where q ω/c, Eq. (4.15) reduces to q≈i

2ω0 . σ(ω)

(4.16)

Ignoring absorption, graphene’s conductivity (4.14) becomes σ(ω) = 4iα0 c

EF , ~ω

(4.17)

2

where α = 4πe0 ~c is the fine-structure constant, so that expression (4.16) transforms to r 2α ~ωGSP ≈ EF ~cq , (4.18) √ with the typical ωGSP ∝ q scaling. Furthermore, since for graphene we 1/2 have EF = ~vF kF with kF ∝ ne , then the GSPs’ frequency depends on the electronic density as ωGSP ∝ n1/4 . (4.19) e √ While the plasmon dispersion ωp ∝ q is inherent to all two-dimensional electronic systems [Stern (1967)], the behaviour portrayed in Eq. (4.19) is exclusive of graphene and has been confirmed by several experiments [Ju et al. (2011); Yan et al. (2013)]. We now take one step further in our analysis by including absorption. This is particularly important, since it will allow us to define the GSPs propagation length. Inserting Drude’s full expression (4.14) for the conductivity into Eq. (4.15), we obtain ~ 1 ω 2 + iγω . (4.20) κ(q, ω) = 2αc EF From Eq. (4.20), we can quantify the degree of confinement of the electromagnetic fields of GSPs in the dielectrics using the penetration depth, defined as 2α EF 1 = ~c ζGSP = . (4.21) (r)|z=ζ(x) + O ζ 2 , (8.226) ρ2D = ω ∂x2 ∂x ∂x∂z ∂x2 ∂z up to first order in ζ; recall that here we are interested in the ky = 0 case only —trapped modes in the groove. The ky 6= 0 case would describe localized modes guided along the groove with finite momentum along y ˆ. This expansion allow us to make analytical progress in the calculations, but it is not essential, since we can workout the full expression for the divergence of the current and use numerical quadrature to evaluate the integrals. The first term in Eq. (8.226) represents the field in flat graphene, whereas the second and third terms are associated with the groove’s slope and curvature, respectively. Therefore, the last two terms probe the structure of the groove. 23 In general, we should also include a term of the form −σ [ˆ > ˆ. However, g y · ∇φ (r)] y since we are interested in the simple case of ky = 0, this term gives no contribution.

page 256

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Plasmons in Graphene Nanostructures and in One-dimensional Channels

257

Having introduced the dynamics in the problem via Eq. (8.226), we can use it to rewrite expression (8.222) as (again, up to first order) Z 1 1 ∂ζ 0 = dr0k φ> (r0 )G(r; r0 ) qk + |kx | + i qx + kx 2 2 ∂x0 z0 =ζ(x0 ) Z iσg ∂2ζ ∂ζ 0 0 > 0 2 + drk G(r; r )φ (r ) kx + 2ikx |kx | 0 + |kx | 02 , ω2 0 ∂x ∂x z 0 =ζ(x0 ) (8.227) so that φ> (r0 )G(r; r0 ) is effectively factorized, thereby being a common term with respect to the others. This makes the calculation more compliable. Now, substituting both the potential [cf. Eq. (8.208) for ky = 0] Z dkx > φ (r) = A(kx )eikx x e−|kx |z ; z > ζ(x) , (8.228) 2π and the Green’s function (8.215) explicitly, produces (z > z 0 ) Z Z Z dqx e−|qx |z iqx x ix0 (kx −qx ) dx0 0= dkx A(kx ) e e 2π 2π 2|qx | 1 1 ∂ζ (|qx |−|kx |)ζ(x0 ) ×e |qx | + |kx | + i qx + kx 2 2 ∂x0 2 ∂ζ ∂ ζ +fσ (ω) kx2 + 2ikx |kx | 0 + |kx | 02 , (8.229) ∂x ∂x iσ (ω)

where we have defined the function fσ (ω) = ωg2 0 , and qy vanishes from integrating the delta function δ(qy ) (owing to the fact that we have assumed ky = 0). Now, we introduce the following representations for the terms involving the surface profile function [Maradudin (1986); Farias and Maradudin (1983)]: Z 0 0 dQ eαζ(x ) = 1 + α J(α; Q)eiQx , (8.230) 2π Z 0 ∂ζ αζ(x0 ) dQ e = iQJ(α; Q)eiQx , (8.231) ∂x0 2π Z 0 ∂ 2 ζ αζ(x0 ) dQ 2 e =− Q J(α; Q)eiQx . (8.232) ∂x02 2π to write out the corresponding terms in Eq. (8.229). Doing so and then projecting with e−iqx in the resulting expression (followed by an integration over x), yields, after some lenghty calculations, an integral equation for the potential’s Fourier amplitude, namely Z iσg dkx 1 + 2 + |q| A(q) = A(kx ) J(|q| − |kx |; q − kx ) |kx | ω0 2π iσg (|q| − |kx |) . (8.233) × (2 − 1 ) [1 − sgn(q) sgn(kx )] + ω0

page 257

April 5, 2016

14:13

258

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Moreover, it is interesting to note that for flat graphene, i.e. ζ = 0, we have J(|q| − |kx |; q − kx ) = 0, and thus, in that scenario, we recover the non-retarded condition for the spectrum of graphene surface plasmons: 1 + 2 +

iσg |q| = 0 , ω0

(8.234)

as the reader may check by comparing this result with Eq. (4.13) and taking the electrostatic limit (q ω/c) in that expression. Naturally, the equivalent result for a dielectric-metal interface [i.e. with graphene absent and 2 → 2 (ω)] can be obtained by taking the limit σg → 0 in Eq. (8.233), which gives Z dkx 2 (ω) + 1 A(kx ) J(|q| − |kx |; q − kx ) |kx |[1 − sgn(q) sgn(kx )], A(q) = 2 (ω) − 1 2π (8.235) a result that agrees with the one found in [Maradudin (1986)]. As we show below, the integral equation (8.233) can be transformed into a matrix eigenvalue problem. Assuming that the profile function ζ(x) is even with respect to the x-coordinate, that is, ζ(x) = ζ(−x), the solutions of Laplace’s equation can be classified as either even or odd, φ> (−x, z) = ±φ> (x, z). From the definition (8.228), this implies that A(−p) = ±A(p), which allows us rewrite Eq. (8.233) involving only positive values of q and kx . Taking into to account both types of solutions, that procedure leads to iσg q A(q) = 1 + 2 + ω0 Z iσg ∞ dkx A(kx ) kx (q − kx ) J(q − kx ; q − kx ) ω0 0 2π Z ∞ dkx iσg ± A(kx ) J(q − kx ; q + kx ) kx 2(2 − 1 ) + (q − kx ) , 2π ω0 0 (8.236) with kx , q ≥ 0 and where ± refers to the even/odd eigenvalue problem. Again, for the dielectric-metal interface, this result simplifies considerably. However, for finite σg (ω) the eigenvalue problem has some degree of complexity, since the frequency, ω, appears both at the left- and righ-hand sides of the integral equation (8.236). Because of this, we shall consider here only the specific case in which ≡ 1 = 2 , that is, that of a graphene sheet (with a 1D-groove) encapsulated in a symmetric dielectric environ-

page 258

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Plasmons in Graphene Nanostructures and in One-dimensional Channels

259

ment24 (e.g. free-standing graphene or graphene encapsulated in hBN). This removes the aforementioned complication, allowing us to write Z ∞ dkx 2iω0 A(q) = qA(q) − A(kx ) kx (q − kx ) [J(q − kx ; q − kx ) σg (ω) 2π 0 ± J(q − kx ; q + kx ) ] .

(8.237)

In possession of Eq. (8.237), we now show how to employ a Gauss-Laguerre numerical quadrature to transform the above integral equation into a standard eigenvalue problem. Equation (8.237) contains two quadratures: one in the variable kx and another one in the variable x due to the function J(α; Q) [see Eq. 8.239]. The integral in J(α; Q) can be computed either numerically or analytically for some special profiles, such as the Gaussian one we are considering. However, as already mentioned, the latter approach can only be applied for small values of the ratio A/R. Therefore, we shall proceed in computing the J(α; Q) numerically. 8.5.4

Spectrum of surface plasmon-polaritons in the presence of a Gaussian groove

The spectrum of surface plasmon-polaritons —in the particular case that we have assumed above— is obtained from the solution of the integral equation (8.237). To proceed further we have to specify the profile of the groove. We choose a Gaussian groove defined by [recall Eq. (8.205)] 2

ζ(x) = Ae−x

/R2

,

(8.238)

which is also symmetric with respect to the x-coordinate. Having an explicit form for ζ(x), we can now proceed in the computation of Eq. (8.237). In particular, from the definition of the functions J(α; Q) [Maradudin (1986); Farias and Maradudin (1983)], Z eαζ(x) − 1 , (8.239) J(α; Q) = dxe−iQx α which for an even profile reduces to Z ∞ eαζ(x) − 1 J(α; Q) = 2 dx cos(Qx) . α 0

(8.240)

24 In spite of that, Eq. (8.236) could still be tacked numerically by transforming that integral equation into a homogeneous matrix equation, after which one imposes that the determinant of the resulting matrix must be zero, a condition that yields the eigenfrequencies.

page 259

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

260

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Introducing the following change of variables (transformation to dimensionless variables) Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

u = qR,

v = kx R,

x = x0 R ,

(8.241)

the integral equation (8.237) translates to Z ∞ 1 2iω0 R dv a(v)v(u − v)[Q1 (u, v, A/R) a(u) = ua(u)− σg (ω) 2π 0 ± Q2 (u, v, A/R)] , where the Kernels Q1 (u, v, A/R) and Q2 (u, v, A/R) read Z ∞ (u−v)ζ(x0 ) −1 0 0 e dx cos[(v − u)x ] Q1 (u, v, A/R) = 2 u − v 0 and Z ∞ 0 e(u−v)ζ(x ) − 1 . Q2 (u, v, A/R) = 2 dx0 cos[(u + v)x0 ] u−v 0

(8.242)

(8.243)

(8.244)

The integral equation (8.242) is easily tractable numerically as it can be transformed into an eigenvalue problem. To that end we discretize the integration over the variable v into a finite sum. This procedure has to be judiciously made to account for the improper nature of the integral. Fortunately, our integration kernel Qj (u, v, A/R) behaves as ∼ e−v , for large v (compared to u) and, therefore, the integral of the kernel can be tackled using the Gauss-Laguerre quadrature scheme. In this approach an integral of the form Z ∞ I= dyf (y)e−y , (8.245) 0

is approximated by Z 0

∞

dyf (y)e−y ∼ =

N X

wj f (yj ) ,

(8.246)

j=1

where {wj } are the weights and yj is the j-th zero of the Laguerre polynomial of order N , i.e. satisfying the equation LN (yj ) = 0. The weights are obtained via {yj } . (8.247) {wj } = [(N + 1)LN +1 ({yj })]2 Finally, applying this technique to Eq. (8.242), we obtain N X 2iω0 R a(ui ) ∼ u a(u ) − wj evj Q(ui , vj , A/R) a(vj ) , = i i σg (ω) j=1

(8.248)

page 260

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Plasmons in Graphene Nanostructures and in One-dimensional Channels

261

which is an usual eigenvalue problem that can be solved by any linear algebra numerical package. More explicitly, one has Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

N

X 2iω0 R a(ui ) = Mij a(vj ) , σg (ω) j=1

(8.249)

where the matrix elements Mij stem from Mij = uj δij − wj evj Q(ui , vj , A/R) , where the matrix Q(ui , vj , A/R) is defined as 1 vi (uj − vi )[Q1 (ui , vj , A/R) ± Q2 (ui , vj , A/R)] . 2π (8.250) Once the eigenvalues λi of the eigenvalue problem (8.249) are known, the spectrum of surface plasmon-polaritons, ω = ω(λi ), can be fetched from the numerical solution of Q(ui , vj , A/R) =

λi =

2iω0 R . σg (ω)

(8.251)

Note the similarity of the last result with Eq. (8.48). This is no coincidence, since both methods of solution are, in the end, quite similar, except that in this case we are expanding the potential in plane waves. In the case in which σg (ω) is given by graphene’s Drude conductivity with negligible broadening γ = 0, the previous equation can be solved analytically in order to obtain ω = ω(λi ), which avoids an extra numerical step. We note that is not difficult to generalize the previous paragraphs taking into account the non-local nature of the conductivity of graphene; the equations will be slightly different though. In the problem of the bump at the interface between a metal and a dielectric the electrostatic surface plasmon mode is split into two modes —one even and one odd. The frequency of the even mode softens whereas that of the odd mode stiffs, as can be seen in Fig. 8.22 (left panel) for the first25 two modes. The softening and the hardening the surface plasmon’s spectrum can be interpreted as follows: the groove/bump, to a first approximation, breaks up the system into two disjoint semi-infinite metaldielectric interfaces, each supporting SPP’s of the costumary type observed in a flat metallic interface. To a second approximation the surface plasmons of the two semi-infinite systems interact with each other, leading to 25 We will be order the eigenvalues in decreasing order, i.e. the largest ones being the first ones (cf. Tab. 8.3).

page 261

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

262

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

anti-crossing of the energy levels or, if one prefers, to bonding (even) and anti-bonding (odd) states, if we establish an analogy with the energy levels in molecules. We note that the presence of the groove (or bump for the same matter) renders the concept of a mode with a well defined wavevector along x ˆ meaningless. In fact, these modes correspond to localized electrostatic plasmons in the groove. For graphene, in the right panel of Fig. 8.22 the dependence of the mode λ7 as function of |A/R| (for a groove) is depicted (top panel). There is a clear dependence of the value of λ7 on the ratio |A/R|. Interestingly enough, and contrary to the case of a metal with a Lorentzian bump, the odd and even modes are affected essentially in the same way for graphene deposited onto a Gaussian groove, with no clear dis-

Figure 8.22: Dispersion relation of SPP’s in the electrostatic limit for a metallic Lorentzian bump (left panel), and for corrugated graphene (squares and circles in the right top and bottom panels), with a Gaussian profile. For the metallic case (left panel) the two first modes, ω1 (solid lines) and ω2 (dashed lines) are depicted, which branch up with the parameter A/R in even and odd modes (the frequency is given in units of the plasma frequency). For graphene, two of the eigenvalues, λ7 (top) and λ14 (bottom), are depicted. Although there is a clear dependence of the frequency modes on |A/R|, both the even and the odd modes present the same dependence for the case λ7 , which corresponds to a larger eigenvalue than for the mode λ14 (check Table 8.3). The total number of modes considered is N = 15.

page 262

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Plasmons in Graphene Nanostructures and in One-dimensional Channels

263

tinction between the two cases. On the other hand, for small eigenvalues, as is the case of the mode λ14 (Fig. 8.22 —right bottom panel) the even and odd modes are affected differently upon varying the parameter |A/R|, with the even mode dispersing more with |A/R| than the odd mode. In Fig. 8.23 we depict the profile of the electrostatic potential at the surface of graphene, that is φ[x, ζ(x)]. The modes λ7 , λ8 , λ9 , and λ10 are represented in that figure. The larger the number of the mode the larger is the period of the electrostatic potential, which translates into a smaller degree of confinement of the mode around the groove. Also, smaller values of λi corresponds to more intense fields located near the apex of the groove. This is depicted in the bottom panel of Fig. 8.23 for the mode λ7 , which is the one, from the four represented in the top panel of this figure, that presents the largest degree of confinement and more intense local field. In Fig. 8.24 the density plot of the field Ez (x, z) is depicted for the modes λ8 and λ10 . From a glance at this figure we immediately see the aforementioned behavior of the electric field. If we had kept a finite value of ky we could have plot the dispersion of the modes along the groove for each of the localized modes, a situation describing guided modes in an i 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15

ui 48.03 38.53 31.41 25.62 20.78 16.65 13.13 10.12 7.566 5.425 3.668 2.270 1.216 0.4927 0.09331

λi,+ 48.15 37.71 30.45 28.25 21.78 16.13 10.98 9.507 8.284 5.681 3.868 2.362 1.250 0.5061 0.09481

λi,− 48.15 37.71 30.45 28.25 21.78 16.13 10.98 9.507 8.284 5.681 3.870 2.374 1.248 0.4954 0.09332

Table 8.3: Eigenvalues λi,+ (even modes) and λi,− (odd modes) for N = 15 and A/R = −0.5. The effect of the groove is present in the deviation of the eigenvalues λi from ui .

page 263

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

264

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

indentation covered with graphene, that is, channel plasmons. In table 8.3 we present the numerical eigenvalues λi for both even and odd modes for a particular value of A/R. It is clear from the table that the effect of the groove is largest for the smallest eigenvalues. In Fig. 8.22 we plot the even and odd modes λ7,+ and λ7,− , respectively. It is clear from both this figure and table 8.3 that these modes are affected in the same way and by the same amount by the presence of the groove. Although, as already mentioned, the concept of momentum along the x−direction is rendered meaningless by the presence of the groove, we can still argue that period of the electric potential (or electric field) is controlled by the value of λi . For larger λi there is no difference between the momentum ui and the eigenvalue λi . In this condition we can argue that the system is characterized by a wavelength Λi = 2π/ui . Since ui is large, Λi is small and the system is sensitive to the presence of the groove, leading to well localized modes. As λi decreases Λi increases and the presence groove is essentially invisible to the modes, which leads to poor localization of the modes and to small values of the local electric field. Indeed, we see that for the mode λ14 in Fig. 8.22 the modification of the eigenvalue upon varying |A/R| is, at most, of 0.1. On the contrary, for the mode λ7 the variation is much larger. All this is also clear from Figs. 8.22 and 8.23. We conclude this Chapter showing how to adapt the formalism to a periodic groove, that is, a grating. To that end we recall that: Z 2 d kk A(kk ; ω)eikk ·rk e−kk z . (8.252) φ> (r; ω) = (2π)2 In a periodic landscape the potential must obey the Bloch condition φ> (r+ a; ω) = eiq·a φ> (r; ω), where a is an in-plane vector encoding the period of the grating (for a one-dimensional grating we have a = aˆ x) and q is the Bloch wavevector. If we write the amplitudes A(kk ; ω) as X A(kk ; ω) = A˜G (q; ω)δ(G + q − kk ) , (8.253) G

and introduce it in Eq. (8.252) we obtain X φ> (r; ω) = A˜G (q; ω)ei(G+q)·rk e−|G+q|z G

= eiq·rk

X

A˜G (q; ω)eiG·rk e−|G+q|z ,

(8.254)

G

where G are the reciprocal lattice vectors of the grating and G · a = 2πm, with m an integer. In this latter form φ> (r; ω) obeys the Bloch condition,

page 264

April 8, 2016

11:53

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Plasmons in Graphene Nanostructures and in One-dimensional Channels

265

as required. We can now proceed along the same lines of this Section and derive an eigenvalue problem where the eigenvectors are composed by the amplitudes A˜G (q; ω). This derivation sets the stage for the next chapter, which deals with the excitation of SPP’s in gratings, including retardation effects.

-50

-25

0

25

50

75

Figure 8.23: Profile of the potential at the surface of graphene, that is, φ[x, ζ(x)], for four different modes, in the case of a Gaussian groove (arbitrary units are used). Clearly, the four modes have different degrees of confinement, with the mode labeled λ7 the more confined of the four. In the bottom panel, an intensity plot of the potential, for the mode λ7 , as function of x/R and y/R, is depicted. There is a clear large potential value at the tip of the groove, which translates into a large electric field. Note the different scales in the x− and z−directions, which differ by about an order of magnitude. We have use N = 15 and A/R = −0.4.

page 265

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

266

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

-1.0

-1.0

0

-0.5

-0.5

0

0.5

0.5

Figure 8.24: Density plot of the electric field Ez for λ7 (top) and λ9 (bottom) corresponding to the potential profiles depicted in Fig. 8.23. We have use N = 15 and A/R = −0.5. Note the different scales in the vertical and horizontal axes. Clearly, the λ7 mode is more confined than the λ9 one. The field is normalized to its value at the apex of the groove.

page 266

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Chapter 9

Excitation of Surface Plasmon-Polaritons Using Dielectric Gratings The study of gratings and rough surfaces [Maradudin (2007a)] as methods of exciting surface plasmon-polaritons was quite popular in the eighties in the context of noble-metals plasmonics [Farias and Maradudin (1983)]. The interest in this topic has been kept alive due to the problem of light scattering by rough surfaces at the nanoscale [Maradudin (2007b)]. With the birth of graphene plasmonics came a renewed interest in the problem of grids and gratings based on graphene. In Chapter 7 we have discussed the grid problem, which was the first method used to induce plasmons in graphene-based periodic structures. As expected, the excitation of graphene plasmons by gratings soon followed (see Chapter 1). The advantage of gratings over grids is that the quality of the graphene sheet is not affected by the lithographic process, since graphene keeps its integrity. On the other hand, the fabrication of gratings with high dielectric contrast may present some difficulties. This is specially true for square-wave gratings. If the grating has some profile, as the one discussed in this Chapter, a graphene sheet may follow that profile thus making a natural graphene-based grating. As discussed briefly Chapter 5 a method for inducing surface plasmonpolaritons in graphene is depositing it on a dielectric grating [Gao et al. (2013)]. In that chapter the example of a square wave grating was given. In this chapter we discuss the excitation of surface plasmon-polaritons by a sine-grating, following a method due to Rayleigh [Voronovich (2007)] (for a different method see Appendix J). Our approach is mainly analytical, which is a consequence of the simplicity of the profile used in the calculations. Interesting enough these periodic structures give rise to plasmonic bands [Bludov et al. (2012a)] which is the fundamental reason why surface plasmon-polaritons can be excited via grating coupling. The excitation of SPP’s belonging to different dispersion branches depends, however, on sym-

267

page 267

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

268

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

metry considerations [Yeung et al. (2015)]. Periodic graphene-antidot arrays are another way of inducing SPP’s in graphene [Nikitin et al. (2012b)]. In this problem we discuss the induction of SPP’s by a grating. However the method can also work in reverse. For example, using SNOM coupling we can induce a propagating SPP along a flat graphene portion of a sheet. This SPP will propagate along the sheet until it reaches a region where a grating has been paterned. Upon hitting this region the SPP radiates into space and this radiation can be collected for some purpose. 9.1

Some Basic Definitions and Results

We want to solve the scattering problem of light impinging on a diffraction grating, as represented in Fig. 9.1. It is assumed that both in D+ and D− the dielectric functions 1/2 are homogeneous (they can be frequency dependent however, as in the example considered in Sec. 5.1.1). The regions D+ and D− define the upper and lower half-planes relatively to the curve y = a(x). For a TM wave we have B = (0, 0, Bz ) and E = (Ex , Ey , 0). Maxwell’s equations for the TM wave are ∂x Ey(p) − ∂y Ex(p) = iωBz(p) , Ex(p) = i

(9.1)

vp2 ∂ Bz(p) , ω ∂y

(9.2)

vp2 ∂ Bz(p) , (9.3) ω ∂x where the superscript p defines de region above or below the grating and p vp = c/ rp is the speed of light in the medium p1 . In a region of constant dielectric function the wave equation has the form (assuming T M −polarization) 2 ∂ ∂2 2 (p) + + ω µ (9.4) p Bz = 0 , ∂x2 ∂y 2 Ey(p) = −i

where µ = µ0 µr is the magnetic permeability of the grating’s material, µ0 is the vacuum permeability, and µr is the relative permeability. In the regions D+ and D− , and in the limit y → ±∞, the scattered and transmitted fields are given by the Rayleigh expansions (Bloch representation of the field) Bz(1) =

∞ X

(1)

A1;m ei(xαn +yβm ) ,

m=−∞ 1 In

this chapter p = 0 rp , where rp is the relative permitivity of medium p.

(9.5)

page 268

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Excitation of Surface Plasmon-Polaritons Using Dielectric Gratings

269

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

3D view

2D view

Figure 9.1: Grating geometry and different regions. The grating is covered with graphene. The curve defining the grating is y = a(x). Above the grating we have region D+ with dielectric permittivity 1 , whereas below the curve y = a(x) we have region D− with dielectric permittivity 2 .

and Bz(2) =

∞ X

(2)

A2;m ei(xαn −yβm ) .

(9.6)

m=−∞

The incoming field is given by Binc;z = ei(xk sin θ−yk cos θ) , (9.7) p r r where k = ω/v1 = k0 1 µ1 , where k0 is the wave number in vacuum, and r1 and µr1 are the relative dielectric permittivity and relative magnetic permeability, respectively. The constants αn and βp;m are given by αn = k sin θ − n2π/D = k sin θ − nG , q βn(p) = kp2 − αn2 ,

(9.8) (9.9)

page 269

April 5, 2016

14:13

270

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

(p)

where kp = ω/vp . The form of βn follows from the solution of the wave (p) (p) equation and we must have 0, for respecting the propagating and evanescent nature of the different harmonics. The number αn /k is interpreted as the scattering angle of the Fourier mode n, that is, eixαn = eikx sin θn ,

(9.10)

θn = arcsin(αn /k) .

(9.11)

leading to Whenever the argument of the inverse sine function, in the previous equation, is smaller than one, we have propagating diffracted orders. In fact, (1) αn2 + [βn ]2 = k 2 . The solution of the problem in the regions D+ and D− , that is, above and below the curve y = a(x), respectively, can be transformed into one of a homogeneous boundary condition by transforming from the x, y reference frame to the u, a(u) one. We introduce the change of coordinates y = a(x) + u .

(9.12)

Clearly, the interface is represented by the homogeneous boundary u = 0. 9.2

Tangent and Normal Vectors, and Boundary Conditions

To define the boundary condition in a curved interface we need to find the tangent and normal vectors to that interface. A vector tangent to the curve y = a(x) at point x is given by ˆ + aˆ t=x ˙y ,

(9.13)

ˆ and y ˆ are unit vectors, and a˙ = da(x)/dx. Thus, the unit vector where x tangent to that curve is ˆt = √ 1 (ˆ x + aˆ ˙ y) . 1 + a˙ 2 The normal vector to the same curve reads 1 ˆ=√ ˆ) . n (−aˆ ˙x + y 1 + a˙ 2

(9.14)

(9.15)

ˆ · ˆt = 0. Since the current is tangent to the graphene sheet we Clearly n must have J = σEt = σEtˆt, where σ is the optical conductivity and Et is given by 1 Et = E · ˆt = √ (Ex + aE ˙ y) (9.16) 1 + a˙ 2

page 270

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Excitation of Surface Plasmon-Polaritons Using Dielectric Gratings

271

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

One of the boundary conditions requires the calculation of vector product ˆ: J×n ˆ=√ J×n

σ σ ˆ=√ ˆ. (Ex + aE ˙ y ) ˆt × n (Ex + aE ˙ y) z 1 + a˙ 2 1 + a˙ 2

(9.17)

ˆ = µσJ × n ˆ reads ˆ − Bz− z Thus, the boundary condition Bz+ z Bz+ − Bz− = √

µσ (Ex + aE ˙ y) . 1 + a˙ 2

(9.18)

− The second boundary condition is E+ t = Et , which can be written as

Ex+ + aE ˙ y+ = Ex− + aE ˙ y− . 9.3

(9.19)

A Trivial Example: Recovering Previous Results

When the surface is flat we have a˙ = 0. Then, the boundary conditions reduce to Bz+ − Bz− = µσEx , Ex+

=

Ex−

.

(9.20) (9.21)

The second boundary condition can be written as 1 1 ∂y Bz+ = ∂y Bz− . 1 2

(9.22)

Since the B + and B − behave, generically, as e−q1 y and eq2 y , respectively, we have −

q1 + q2 q1 2 + Bz = Bz− ⇔ Bz− = − B . 1 2 q2 1 z

(9.23)

Then, the first boundary condition reads Bz+ +

q 1 2 + i q1 Bz = µσ ∂y Bz+ = −iµσ B+ , q 2 1 ωµ1 ωµ1 z

(9.24)

which gives the spectrum of the surface plasmon-polaritons in graphene, since we obtain 1 2 σ + + i = 0, q1 q2 ω in agreement with the results of Chap. 4.

(9.25)

page 271

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

272

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

9.4

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

The Fields in D+ and D−

The fields in region D+ are (the harmonic convention e−iωt is used): X (1) (1) Bz+ = ei(α0 x−β0 y) + ei(αn x+βn y) An , (9.26) n

Ex+

1 = ωµ1

(1) (1) β0 ei(α0 x−β0 y)

! X

−

(1) βn(1) ei(αn x+βn y) An

,

(9.27)

n

and Ey+

1 = ωµ1

α0 e

(1)

!

i(α0 x−β0 y)

+

X

αn e

(1) i(αn x+βn y)

An

.

(9.28)

n

The fields in region D− are Bz− =

X

(2)

ei(αn x−βn

y)

Cn ,

(9.29)

n

Ex− =

1 X (2) i(αn x−βn(2) y) β e Cn , ωµ2 n n

(9.30)

(2) 1 X αn ei(αn x−βn y) Cn . ωµ2 n

(9.31)

and Ey− =

(p)

Recall that the constants αn and βn are given by αn = k sin θ − n2π/D = k sin θ − nG , q βn(p) = kp2 − αn2 , kp > αn , q βn(p) = i αn2 − kp2 , kp < αn ,

(9.32) (9.33) (9.34)

where kp = ω/vp and p = 1, 2; also we have k1 ≡ k. In what follows, we need the Fourier transforms X a˙ = a˙ p eiGpx , (9.35) p

X 1 √ = Kp eiGpx , 1 + a˙ 2 p X a˙ √ = Rp eiGpx , 1 + a˙ 2 p

(9.36) (9.37)

page 272

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Excitation of Surface Plasmon-Polaritons Using Dielectric Gratings

273

where a˙ p , Kp , and Rp have the generic definition Z 1 D −iGpx Cp = e c(x)dx . (9.38) D 0 When a˙ 1 we have Rp = a˙ p and Kp = δp,0 , which is the case for shallow gratings. If we now introduce the change of variables y = u + a(x), the boundary conditions are applied at u = 0. Then we replace y by u + a(x) in the fields and put u = 0 when we consider the boundary conditions. We also define X (1) (1) eiβn a(x) = Lj;n eiGjx , (9.39) j

e

(1) −iβ0 a(x)

=

X

(1)

(9.40)

(2)

(9.41)

Lj;0 eiGjx ,

j (2)

e−iβn

a(x)

=

X

Lj;n eiGjx ,

j

where L(κ) m;n =

1 D

D

Z

e−iGmx e(−1)

κ+1

(κ) iβn a(x)

dx ,

(9.42)

0

with κ = 1, 2 and Z 1 D −iGpx −iβ0(1) a(x) dx . (9.43) = e e D 0 After a lengthy calculation, the boundary condition (9.18) reads X (2) X (1) σ X (1) (2) Lk;0 + Ln+k;n An − Ln+k;n Cn = Kk−j βn(2) Ln+j;n Cn ω 2 n n n,j X (2) + Rk−j αn Ln+j;n Cn , (9.44) (1) Lp;0

n,j

and the boundary condition (9.19) reads X X 2 (1) (1) (1) β0 Lk;0 + α0 a˙ k−j Lj;0 − βn(1) Ln+k;n An 1 n j X X X (1) (2) (2) + a˙ k−j αn Ln+j;n An = βn(2) Ln+k;n Cn + a˙ k−j αn Ln+j;n Cn . n,j

n

n,j

(9.45) We can use Eqs. (9.44) and (9.45) to compute the intensity of the reflect orders.

page 273

April 5, 2016

14:13

274

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

9.4.1

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Reflectance and transmittance efficiencies

In the end we want to compute the amount of reflected, transmitted, and absorbed radiation. To that end we have to defined the different electromagnetic fluxes. The pointing vector S = E × B∗ /µ is given by ˆ Ey Bz∗ − y ˆ Ex Bz∗ . S=x

(9.46)

From Maxwell’s equations we have Ex = i

v2 ∂y Bz . ω

(9.47)

Thus for a mode m we have v 2 (1) (9.48) Sinc = − 1 β0 , ω v2 (9.49) Srefl = 1 βn(1) |Am |2 , ω v2 Stran = − 2 βn(2) |Cm |2 (9.50) ω for the incident, reflected, and transmitted pointing vector, respectively. Thus the reflectance and transmittance efficiencies are (1)

Rn =

βn

(1)

β0

|Am |2 ,

(2)

Tn =

(9.51) (2)

v22 βn

1 βn

v12 β0

2 β0

|Cm |2 = (1)

(1)

|Cm |2 ,

respectively. Naturally, the absorbance is defined as A = 1 − where n extends over the propagating orders only. 9.4.2

(9.52) P

n (Rn + Tn ),

Particular limits for the transmittance and the reflectance

As a rather simple limit, we want to obtain from Eqs. (9.44) and (9.45) the transmittance and the reflectance of a flat graphene sheet in vacuum, and the same quantities for an interface composed of two flat dielectrics. For these two cases we have a(x) = 0 which implies: a(x) ˙ = 0, Rp = 0, Kp = δp,0 , and Lp = δp,0 . In this case, Eqs. (9.44) and (9.45) reduce to σ (2) δk,0 + A−k − C−k = β C−k , (9.53) ω2 1 (2) (1) β (1) δk,0 − β−k A−k = β−k C−k . (9.54) 2

page 274

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Excitation of Surface Plasmon-Polaritons Using Dielectric Gratings

275

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

The last two equations imply that only A0 and C0 are non-zero. Then, σ (2) 1 + A0 − C0 = β C0 , (9.55) ω2 0 (2)

1 − A0 =

1 β0

(1)

2 β0

C0 ,

(9.56)

from which we obtain (2)

2=

1+

1 β0

(1)

2 β0

σ (2) + β ω2 0

! C0 .

(9.57)

In the particular limit 1 = 2 , C0 reduces to 2 , (9.58) C0 = 2 + σ cos θ/(1 v1 ) which is the transmittance amplitude through graphene at an incident angle θ. The transmittance follows from T0 = |C0 |2 . Another particular limit is σ = 0. In this case we have (1)

C0 =

22 β0 (1)

(2)

,

(9.59)

2 β 0 + 1 β0

from which follows A0 = −1 + C0 =

(1)

(2)

(1)

(2)

2 β0 − 1 β0

2 β0 + 1 β0 p p 2 /1 cos θ − 1 − 1 sin2 θ/2 p = p , 2 /1 cos θ + 1 − 1 sin2 θ/2

(9.60)

which reproduces the well known result from elementary optics for the reflectance amplitude at the interface between two dielectrics. 9.5

A Non-Trivial Example: A Grating with a Sine-Profile

Let us now consider a non-trivial example, where the expressions for Rp , Kp , and Lp are not expressed in terms of simple numbers, as in the previous example. We assume a profile of the form a(x) = h sin(2πx/D) ,

(9.61)

a˙ = 2πh/D cos(2πx/D) .

(9.62)

from which follows In the regime 2πh/D 1, we have Rp ≈ a˙ p and Kp ≈ δp,0 , with πh (δm,1 + δm,−1 ) . a˙ p = D

(9.63)

page 275

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

276

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

In this case, Eqs. (9.44) and (9.45) simplify to

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

N X

fa (n + k; n)An +

n=−N N X

N X

(1)

fc (n + k; n)Cn = Lk;0 ,

(9.64)

n=−N

ga (n + k; n)An +

n=−N

N X

(1)

gc (n + k; n)Cn = Lk;0

n=−N

+

α0 πh (1) (1) (L + Lk+1;0 ) , β0 D k−1;0

(9.65)

where the functions fa (n + k; n), fc (n + k; n), ga (n + k; n), and gc (n + k; n) read (1)

fa (n + k; n) = −Ln+k;n , σ (2) ~cβn(2) Ln+k;n fc (n + k; n) = 1 + ω2 c~ πh σ (2) (2) ~cαn (Ln+k−1;n + Ln+k+1;n ) , + D ω2 c~ (1)

ga (n + k; n) =

βn

(1)

(1) β0

Ln+k;n −

πh αn (1) (1) (L + Ln+k+1;n ) , D β0 n+k−1;n

(9.66)

(9.67) (9.68)

(2)

gc (n + k; n) =

πh 1 αn (2) 1 βn (2) (2) L + (L + Ln+k+1;n ) . 2 β (1) n+k;n D 2 β (1) n+k−1;n 0 0 (9.69)

We also have the following definitions (1) L(1) m;n = Jm (βn h) ,

(9.70)

(1) Lm;0

=

(1) Jm (−β0 h) ,

(9.71)

=

Jm (−βn(2) h) ,

(9.72)

L(2) m;n

where Jm (x) is the regular Bessel function at the origin. It is convenient for numerical purposes to write p (1) ~cβ0 = r1 ~ω cos θ , (9.73) p r ~cαn = 1 ~ω sin θ − 2πn~c/D , (9.74) q p ~cβn(p) = rp (~ω)2 − ( r1 ~ω sin θ − 2πn~c/D)2 , (9.75) and (2)

σ (2) 4 EF ~cβn βn = α r , ω2 2 ~ω ~γ − i~ω

(9.76)

where r1/2 are the relative dielectric permittivities, EF is the Fermi energy, and α is the fine structure constant. In Fig. 9.2 we represent the efficien-

page 276

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Excitation of Surface Plasmon-Polaritons Using Dielectric Gratings

b2445-mas

277

Figure 9.2: Dependence of the reflectance, transmittance efficiencies, and absorbance as function of frequency for different depth of the grooves for a sinegrating. The parameters are D = 10 µm, ~γ = 2.6 meV, EF =0.45 eV, 1 = 1, 2 = 11, and h = D/25 (circles), h = D/15 (squares), and h = D/10 (triangles).

cies R0 and T0 , top and central panels, respectively, and the absorbance, A = 1 − R0 − T0 , as function of the energy of the incoming photon, for different values of the ratio h/D. When h/D 1 we recover the properties of a flat graphene sheet. In Fig. 9.3 we compare results from the Rayleigh procedure, described in this chapter, with those produced by the extinction theorem (dashed curves) [Ferreira and Peres (2012)]. We see that the agreement is excellent. In the figure, results for several angles of incidence θ are given for h/D = 0.1. The resonance seen in Figs. 9.2 and 9.3 around 10 meV is due to the excitation of a surface-plasmon-polariton of energy s 4α 2π EF c~ = 11 meV . (9.77) ~ω ≈ r1 + r2 D It should now be clear that the technique described above is suitable for the excitation of SPP’s. A different approach to the same problem was considered in [Slipchenko et al. (2013b)]. We note that we have not included the effect of the grating profile, which also acts as a gate, in the

page 277

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

278

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Figure 9.3: Reflectance and absorbance of graphene on a silicon sine-grating. Left: Dependence of the reflectance on the angle of incidence. We compare the Rayleigh method (solid circles) with the results from the extinction theorem [Ferreira and Peres (2012)] (solid lines); the parameters are D = 10 µm, ~γ = 2.6 meV, EF =0.45 eV, 1 = 1, 2 = 11, h = D/10. The arrow indicates the direction of growth of the incident angle θ for the several curves. Right: Absorbance for the same parameters as before but different γ values. The prominent peak see in the absorbance curves is the fingerprint of the excitation of an SPP.

conductivity of the system. This effect will induce an additional periodicity into the problem [Ochiai (2015)] which can be tackled by methods similar to those explained above by [Peres et al. (2012)]. An interesting variation of the problem we have considered here was proposed in [Ferreira and Peres (2012)], where a periodic meta-material grating was covered with graphene. In this work it was show that it is possible to obtain 100% of light absorption (see also [Thongrattanasiri et al. (2012a)]) in graphene due to the excitation of surface plasmon-polaritons. The tuning parameter was (maybe as expected) the amplitude h of the grating profile. It was also found (and this maybe less obvious) that the dependence of the absorption on h is non-monotonous. Interesting enough, the corrugation needed to achieve total absorption is not very large: h ∼ 10 − 100 nm, and decreases as the Fermi energy increases. These findings are summarized in Fig. 9.4. It should be appreciate that central to the mechanism of total absorption

page 278

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Excitation of Surface Plasmon-Polaritons Using Dielectric Gratings

b2445-mas

279

Figure 9.4: Dependence of the absorption at resonance (that is, at the frequency ωspp of the surface plasmon-polariton) on the corrugation height for different graphene Fermi energies, EF . The fast change in the absorbance as EF varies from 0.07 to 0.08 eV results from a suppression of interband transitions in graphene as 2EF & ~ωspp . In this calculation, both the inter- and intra-band conductivity have been included.

is the negative value of the dielectric function of the meta-material in the spectral region of interest (see also Fig. 5.2, where a similar effect has been explored). Indeed, we can imagine that by changing (ω), for example, by considering a meta-material with an appropriate plasma frequency, the resonant frequencies ωspp can be controlled within a broad range of values, thus tailoring the hybrid structure for a desired spectral region. An interesting variation of the above problem is that of a square-profile grating [Peres et al. (2013)] (see also [Sheng et al. (1982)]). This problem is rather pathological due to the infinite derivative of the profile at the transition from the tooth to the trenches. However, the problem can still be solved exactly by considering a Kronig-Penney model in the grating zone. This method was applied in Sec. 5.1.1 to the solution of graphene on a Gallium-Arsenide substrate with a square grating in between, and the technical details can be found in [Peres et al. (2013)]. As expected, this configuration is quite efficient in exciting surface plasmon-polaritons

page 279

April 5, 2016

14:13

280

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

on graphene. The efficiency of absorption is a function of the depth of the trenches, as in the case of Fig. 9.4 albeit with a different behavior.

page 280

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Chapter 10

Excitation of Plasmons by an Emitting Dipole

The problem of the emission of an excited dye (or quantum dot) over a graphene sheet has been studied both theoretically [Gómez-Santos and Stauber (2011); Koppens et al. (2011)] and experimentally [Kasry et al. (2012); Gaudreau et al. (2013)]. The case of Förster resonant energy transfer (FRET) between two dyes in the presence of graphene has also been considered [Biehs and Agarwal (2013)]. In this chapter we show that a dye can, in principle, de-excite via the excitation of plasmons in graphene. This possibility has its fingerprint in a resonance in the effective dielectric function of the system, or in the dispersion of the life-time of the excited state of the dye with the distance to the graphene sheet. We first formulate the problem in the electrostatic approximation and use Fermi’s golden rule, following [Swathi and Sebastian (2009)]. We show that this approach corresponds to a decaying pathway associated with the induction of particle-hole excitations in graphene. We end the chapter with an exact calculation of the total decaying rate of the dye in the presence of graphene, where the fingerprint of plasmon excitation becomes manifest. We show that the decaying rate of an emitter in the presence of graphene differs substantially from the free space decaying rate, a manifestation of the Purcell effect. This effect has been demonstrated in a variety of physical systems, such as radiating molecules near a metallic-dielectric interface, Rydberg atoms in an optical cavity, and nuclear transitions in small metallic particles, the latter example being the basis of the work of Purcell [Purcell (1995)]. A decaying emitter can couple to surface plasmons when the distance to the metallic interface (which can be doped graphene) is smaller than the emission wavelength (but much larger than typical atomic distances), the reason being that the dipole field contains large in-plane wavevectors, associated with evanescent modes, that do not propagate in the far field but can couple to the SPP’s at

281

page 281

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

282

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

the surface of the conductor [Toropov and Shubina (2015)]. For distances much smaller than the emission wavelength, the emitter couples to the conductor by inducing either inter-band or intra-band absorption. For neutral graphene only the inter-band transitions pathway exists. This latter case is discussed in the appendix section M.2. 10.1

Statement of the Problem and a Bit of Electrostatics

Let us consider a point-like dipole embedded, at a distance z > 0, in a dielectric medium of permittivity 1 above a doped graphene sheet (EF > 0). This dipole represents a quantum emitter (such as a dye). The sheet rests on a dielectric of permittivity 2 (located at z < 0). We want to derive the explicit boundary conditions obeyed by the field (or the potential for that matter) at the graphene plane (z = 0). We define s as the in-plane (z = 0) position vector, as shown in Fig. 10.1. We want to compute the rate at 3D view

side view

graphene

Figure 10.1: An emitting dipole (e.g. a dye), characterized by a dipole moment µ, over a graphene sheet. Above the graphene the dielectric constant is 1 and below it is 2 . The vector r can be written as r = s − zˆ uz , and s an in-plane vector. At the right we have a side view of the geometry under consideration together with the image dipole in medium 2.

which the dye decays to the ground state via an energy transfer to electronic particle-hole excitations in graphene, that is, we want to compute the non-radiative decaying rate of the dye. We further assume that graphene is doped with electrons and the energy between the excited state and the ground state of the dye, ~ω, is smaller than 2EF . In this case, there are no electronic inter-band excitations in graphene; all excitation processes are

page 282

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Excitation of Plasmons by an Emitting Dipole

b2445-mas

283

intra-band particle-hole excitations. The rate of excitation of intra-band electronic processes is given by Fermi’s golden rule (see Sec. 2.3.1 for the definitions of the different quantities) 1 2π X X = gs gv |hψk+q,+ |V |ψk,+ i|2 F (k, q)δ(Ek+q,+ − Ek,+ − ~ω) , τ ~ q k

(10.1) where gs and gv are the spin and valley degeneracies, respectively, F (k, q) is a combination of Fermi distribution functions (see Appendix M): F (k, q) = f (vF ~k)[1 − f (vF ~|k + q|)] ,

(10.2)

taking into account the empty and occupied electronic states, and V represents the dipole potential. The next step is to compute the potential felt by the electrons due to the dipole at position z. This is not as simple as it may sound because of the existence of two different dielectrics. Indeed, we have to compute the image potential created by the real dipole. Let us do this in two steps. First we consider the case where graphene is absent and later we introduce graphene into the problem. In the first case, the boundary conditions are the continuity of the potential and of the component perpendicular to the interface of the electric displacement vector D at z = 0. Following the method of images, we assume that there is a image dipole at z < 0 with dipole moment µ0 (see Fig. 10.2). The original dipole is located at z = h and the image dipole at z = −h. The potential of the side view

Figure 10.2: Position vectors r and r0 of the point R = (x, y, z) relative to the dipoles. The vector s has coordinates (x, y) and ˆ z = uˆz .

page 283

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

284

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

original dipole reads 1 µ·r , (10.3) 4π0 1 r3 and that of the image dipole reads 1 µ0 · r , (10.4) Vi = 4π0 1 r3 where r = (x, y, z − h) and r0 = (x, y, z + h) (see Fig. 10.2). At z > 0 the total potential reads V1 = V +AVi and at z < 0 we have V2 = BV , where A and B are to be determined from the boundary conditions. We assume that µ0 = (µz , −µx , −µy ) and check whether this choice allows the determination of A and B uniquely. The z−component of the electric field is determined from the derivative of the potential in order to z. The condition V1 = V2 at z = 0 implies A + B = 1 and the condition 1 Ez,1 = 2 Ez,2 implies 1 (1 + A) = 2 B. Solving these two equations we obtain 2 − 1 A= , (10.5) 2 + 1 21 B= . (10.6) 2 + 1 Then, the potential felt by the electrons in graphene would be 2 1 µ·r V2 = BV = , (10.7) 2 + 1 4π0 r3 with z = 0. This is true for neutral graphene. However, the electrons in doped graphene change the second boundary condition. Indeed, the correct boundary condition is given by Eq. (K.1). Furthermore, due to the presence of the dipole, the electronic charge is not homogeneous, becoming a function of the vector s. As shown in Appendix K, and ignoring diffusion, the correct boundary condition is

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

V =

1 Ez1 (z = 0, q) − 2 Ez2 (z = 0, q) = σD (ω)q · E(z = 0, q)/ω ,

(10.8)

where, due to the dot product of E(q) with q, only the component of the field parallel to the graphene plane enters in the right-hand-side of the boundary condition. Note that the boundary condition (10.8) is written in a mixed representation, where we have kept the spatial dependence along the z−direction but have Fourier transformed the x- and y-coordinates of the fields. We can relate the field in-plane, Ek (q), to the potential in the following way: Ek (z, s) = −∇s φ(z, s), where φ(z, s) is the electrostatic potential. Introducing the Fourier representation of the field and of the potential we obtain Ek (q) = −iqφ(z, q), which leads to 0 1

∂ ∂ φ(0+ , q)−0 2 φ(0− , q) = iσD (ω)q 2 φ(0, q)/ω ≡ λφ(0, q) , (10.9) ∂z ∂z

page 284

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Excitation of Plasmons by an Emitting Dipole

b2445-mas

285

where λ = iσD (ω)q 2 /ω. Thus, we need to determine the Fourier transform of the potential (see Appendix L). For a dipole µa , at z = h, and for z < h we obtain µa q Va = · −i − u ˆz e−q(h−z) . (10.10) 20 1 q For a dipole µb , at z = −h, and for z > −h we obtain µb q Vb = · −i + u ˆz e−q(h+z) . (10.11) 20 2 q To determine the potential (in Fourier space) felt by the dipole we again employ the method of images. In the region 0 < z < h the total potential is a sum of the real dipole plus the image dipole, that is V+ (z) = Va + Vb ,

(10.12)

and for z < 0, the potential is due to a third dipole located at z = h, that is, q µc ˆz e−q(h−z) . · −i − u (10.13) V− (z) = 20 1 q It follows from the boundary conditions that V+ (0) = V− (0) and ∂ ∂ 0 1 V+ (0+ ) − 0 2 V− (0− ) = λV− (0) . (10.14) ∂z ∂z We choose to write µa = (µax , µay , µaz ), µb = (−µbx , −µby , µbz ), and µc = (µcx , µcy , µcz ). Introducing these in the boundary conditions we obtain µbz µc µa + z = z, 2 1 1

(10.15)

and −

1 b µ + 2 z

2 λ + 1 q0 1

µcz = µaz .

(10.16)

Solving the last two equations for µbz and µcz we obtain 2 2 − 1 + λ/(0 q) 1 2 + 1 + λ/(0 q) 21 , µcz = µaz 2 + 1 + λ/(0 q)

µbz = µaz

(10.17) (10.18)

which is the generalization of the results (10.5) and (10.6). Identical equations hold for the other components of the dipole moments, µbx/y and µcx/y . Finally, the potential (in Fourier space) felt by the electrons in graphene is V− (0) =

µa · (−iq/q − u ˆz ) −qh e . 0 [2 + 1 + λ/(0 q)]

(10.19)

page 285

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

286

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

We are now in position of computing the matrix element of the potential entering in Fermi’s golden rule. We can show (see Appendix L) that the matrix element is given by1 1 hψk+q,+ |V |ψk,+ i = −e [1 + ei(θk −θk+q ) ]V− (0) . (10.20) 2A It is clear from the above expression that 1 |hψk+q,+ |V |ψk,+ i|2 ∝ |2 + 1 + λ/(0 q)|2 1 = (10.21) 00 02 /(ω )2 , [1 + 2 − qσD /(ω0 )]2 + q 2 σD 0 0 where the conductivity has been separated in its real, σD , and imaginary, 00 σD , parts. The previous denominator has a resonance when the frequency obeys the condition 00 1 + 2 − qσD /(ω0 ) = 0 ,

(10.22)

which is nothing but the equation for the spectrum of graphene surface plasmon-polaritons in the electrostatic limit [see Eq. (4.16)]. Thus, at least in principle, the decay of a quantum emitter (a dye, a quantum dot, etc.) may excite SPP’s in graphene. A note on the results (10.17) and (10.18) is in order. Let us consider, for simplicity, the result for (10.18) in vacuum. In this case we obtain 2 . (10.23) µcz = µaz 2 + λ/(0 q) We now show that the factor multiplying µaz is nothing but the transmission amplitude of a plane wave through graphene in vacuum. In fact, that proportionally factor can be written as 2 tp = . (10.24) 2 + iσD q/(0 ω) On the other hand, from the results of Appendix N, the transmission amplitude for a p−polarized wave reads 2 tp = . (10.25) 2 + παf (ω) cos θ 1 In Eq. (10.20) we are using the spinors representing the electronic motion in graphene in the form: 1 1 χα = √ , iθ 2 αe q

and not as written in Eq. (2.49). The two representations are equivalent as they differ from an overall multiplicative phase. What representation to use is a matter of convenience.

page 286

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Excitation of Plasmons by an Emitting Dipole

287

p Since σD = σ0 f (ω) and cos θ = kz /k = c k 2 − q 2 /ω, the two results coincide when qc/ω 1, that is, in the electrostatic limit (in this case we have cos θ → icq/ω). This result brings about an interesting connection between the boundary conditions in electrostatics at the interface of two dielectrics and the transmittance and the reflectance amplitudes of the same interface. It should therefore come as no surprise to learn that the electromagnetic fields of a dipole at an interface can be expressed in terms of these amplitudes (more on this in Sec. 10.3). 10.2

Calculation of the Non-Radiative Transition Rate: Particle-Hole Excitations Pathway

We now compute the non-radiative transition-rate of a quantum emitter via the particle-hole excitations pathway. We will see that within the model of the previous section the calculation of 1/τ cannot account for the presence of the SPP’s. That is because we are assuming that the only possible excitation induced in graphene is the creation of particle-hole pairs. From Appendix M we have [see Eq. (M.15)] 2 2 Z 2π e2 2πµz + πµk 2kF +Ω dq q 3 e−2qz 1 p =2 G(q) . τ ~ 20 (2π)4 ~vF |(q, ω)|2 q 2 − Ω2 Ω

(10.26)

From Fig. M.1 we see that the integral extends only over the regions 1A and 2A of Fig. 2.5. However, plasmons, as long-lived excitations, exist in region 1B (see Fig. 4.5). Nevertheless, the presence of the plasmons can still be felt rather indirectly. The idea is simple: the tail of the spectral function associated with the presence of the plasmons “leaks” from region 1B into region 1A, this is possible because of damping effects. This leaking, however, is appreciable only at frequencies and momenta where the dispersion is close to the line ω = vF q (see Fig. 4.5) and therefore has no significant impact on the results computed in this section (the impact is higher if the dielectric constant of the substrate is large; see the right panel of Fig. 4.5). In technical terms, we say that the SPPs are, in this case, excited off-shell. Thus the calculation presented in this section refers to the decay pathway associated with Ohmic losses. As noted in Appendix M, the integral over q cannot be performed analytically. Therefore we present below the result of a numerical calculation of 1/τ . For simplicity, we assume that graphene is in vacuum and compare the non-radiative decaying rate with the radiative decaying rate of an

page 287

April 5, 2016

14:13

288

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

isolated dipole, given by [Novotny and Hecht (2014); Zettili (2009)]

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

1 τvac

=

ω 3 |µ|2 . 3π0 ~c3

(10.27)

τvac , τ

(10.28)

We then define the ratio Φ(z, ω) =

which allows to compare the two decaying rates. Next, we introduce the change of variables q/Ω = x. This allows to write the decaying rate as 2 2 Z dx x3 e−2xΩz 2π e2 ω 3 2πµz + πµk 2kF /Ω+1 1 √ G(xΩ) , (10.29) =2 τ ~ 20 (2π)4 ~vF4 |(x, ω)|2 x2 − 1 1 and allows to rewrite Φ(z, ω) as Φ(z, ω) = 6αg

µ2z + µ2k /2 c3 J(z, ω) , |µ|2 vF3

where αg = e2 /(4π0 ~vF ) ≈ 2.3 and Z 2EF /(~ω)+1 dx x3 e−2xΩz √ J(z, ω) = G(xΩ) , |(x, ω)|2 x2 − 1 1

(10.30)

(10.31)

where 1 1 = 00 /(v )]2 + x2 σ 02 /(v )2 . |(x, ω)|2 [2 − xσD F 0 F 0 D

(10.32)

For σD we use the value of the longitudinal non-homogeneous conductivity σxx (ω, q) derived in Appendix C. In Fig. 10.3 we plot both Φ(z, ω), for three different values of z, and 1/|(q, ω)|2 , for two different values of x, corresponding to the extremes of the integration interval in Φ(z, ω). Whenever Φ(z, ω) grows the non-radiative decaying rate is enhanced. We see an enhancement of Φ(z, ω) at low frequencies. The effect of increasing z is to suppress the effect of the non-radiative energy transfer, as can be seen in the left panel of Fig. 10.3, by comparing the different curves. This is due to the exponential in the integral, which depends both on z and ω. In the right panel of Fig. 10.3 we see that 1/|(q, ω)|2 has no resonance in the integration interval. We should note that, by construction, our model cannot be extended to frequencies higher that 2EF , since in this case, inter-band transitions start to play a role, an effect we have not included in the model (its inclusion is, however, straightforward and does not change the conclusions).

page 288

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Excitation of Plasmons by an Emitting Dipole

289

Figure 10.3: Non-radiative decaying rate of a dipole, as measured by the function Φ(z, ω) (left panel), for different values of z, z = 7, 10, 15 nm. Right panel: Inverse of the absolute value of the dielectric function for different values of x, x = 1 and x = 1 + 2EF /(~ω). The parameters are EF = 0.3 eV and ~γ = 4 meV.

10.3

Calculation of the Total Transition Rate: Full Electromagnetic Calculation

As we have seen, the decaying rate of a quantum emitter is influenced by the environment. It is possible to compute this effect using a full electromagnetic theory. What we need to know is the full electromagnetic field in the presence of the environment. This can be determined using dyadic Green’s functions [Novotny and Hecht (2014)]. Here we consider a doped graphene sheet in vacuum with a quantum emitter located at distance z above graphene. To determine the fields, we need to know the reflectance amplitudes of a plane wave through graphene. These coefficients are derived in Appendix N and read παfL (ω, q)sz , 2 + παfL (ω, q)sz παfT (ω, q) rs = − , 2sz + παfT (ω, q)

rp =

(10.33) (10.34)

√ for p− and s−polarizations, respectively, and sz = 1 − s2 . Taking into account intra-band transitions only, the functions fT (ω, q) and fL (ω, q) read

page 289

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

290

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

(see Appendix C) 1 1 8EF fL (ω, q) = π ~γ − i~ω β 2 (ω, q) fT (ω, q) =

8EF 1 1 π ~γ − i~ω β 2 (ω, q)

−1 + p

1

!

, (10.35) 1 − β 2 (ω, q) p −1 − 1 − β 2 (ω, q) , (10.36)

where β(ω, q) is defined as β(ω, q) =

i~vF q , Γ − i~ω

(10.37)

and Γ = ~γ. It can be shown [Novotny and Hecht (2014)] that the rate of decay of the dipole, when compared with the decaying rate in vacuum is given by (see Appendix P) Z µ2x + µ2y 3 ∞ 1/τg τvac s 2 2iωzsz /c = = 1+ ds< (r − s r )e s z p 1/τvac τg µ2 4 0 sz Z s3 µ2 3 ∞ rp e2iωzsz /c (10.38) ds< + z2 µ 2 0 sz where 1/τg is the decaying rate of the quantum emitter in the presence 2 of graphene; √ τvac /τg is called the Purcell factor . For s > 1 √ the ratio we have 1 − s2 = i s2 − 1. In general, decaying of a quantum emitter can occur through several channels, but in our case only three are active: radiative decay, particle-hole excitations in graphene, and excitation of surface plasmon-polaritons propagating at the surface of graphene. From Eq. (10.38) we see the existence of two regimes. In the first the emission is controlled by propagating waves, corresponding to 0 < s < 1; in interval 1 < s < ∞ the emission is by evanescent waves, which can excite surface plasmon-polaritons. The result of the calculation of the ratio τvac /τg is given in Fig. 10.4. As in the case of Fig. 10.3, an increase of the distance z leads to a reduction of the decaying rate (and therefore to an increase of τg ). This leads to a similar behaviour of τvac /τg and τvac /τ , as can be seen by comparing the left panels of Figs. 10.3 and 10.4. However, in Fig. 10.3 the mechanism of excitation of surface plasmon-polaritons is not present (although the dielectric function does have a pole at the plasmon dispersion the momentum is off-shell). 2 The Purcell effect refers to the change of the decaying rate of an emitter due to the proximity of a system that can support both losses (as either metal or graphene) and/or surface modes (as, for example, a metal, graphene, and hBN).

page 290

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Excitation of Plasmons by an Emitting Dipole

b2445-mas

291

Figure 10.4: Radiative and non-radiative decaying rate of a dipole, as measured by the ratio τvac /τg (Purcell factor), for three different values of z = 7, 10, 15 nm. The parameters are EF = 0.3 eV, ~γ = 4 meV, and µx = µy = µz = 1. The right panel is a zoom-in (in log-scale) of the low frequency behavior of the data in the left panel. The broad bump in the data in the left panel is due to the excitation of surface-plasmon-polaritons, as argued in Table 10.1.

We can also show numerically that the largest contribution to the integral τvac /τg comes from evanescent waves in the TM-channel (p−polarization). In fact, we can approximate the ratio τvac /τg by Z µ2x + µ2y 3 ∞ τvac s(s2 − 1) −2ωz√s2 −1/c √ ds=m[r ] e ≈ 1+ p τg µ2 4 1 s2 − 1 Z √ µ2 3 ∞ s3 2 + z2 e−2ωz s −1/c , ds=m[rp ] √ 2 µ 2 1 s −1 Z 2 2 √ 3 µz + µk /2 ∞ s3 −2ωz s2 −1/c √ ≈ 1+ ds=m[r ] e (10.39) p 2 µ2 s2 − 1 1 where =m[rp ], in the limit β(ω, q) → 0, reads √ 2αEF ~γ s2 − 1 √ =m[rp ] = , (10.40) (~γ)2 + (~ω − 2EF α s2 − 1)2 and has a resonance at the surface plasmon-polariton energy. Indeed, we see that when s = q/k 1 (where q is the in-plane momentum) we have a resonance at the energy p ~ω − 2EF αq/k = 0 ⇔ ~ω = 2EF αq/(ω/c) ⇔ ~ω = 2EF α~cq , (10.41)

page 291

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

292

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

which agrees with the result of Eq. (4.16). We note that the result (10.39) is rather similar to the that derived from the Fermi’s golden rule (10.31) for the non-radiative rate of decay. On the other hand it is, clear from Fig. 10.4 that the peak of the broad bump is dispersing as function of z. We can show that this dispersion is due to the excitation of surface plasmons. We assume that the distance z introduces a momentum of the order of qSP P ∝ 1/z. In this case, the ratio of energy of two maxima has to coincide with the ratio of the square root of qSP P . This analysis is done in Table 10.1 and confirms the above statement. p z (nm) ωz /EF ω7 /ωz z/7 p z=7 ω7 /EF = 1.01 ω7 /ω7 = 1 p 7/7 = 1.00 z = 10 ω10 /EF = 0.86 ω7 /ω10 = 1.17 p10/7 = 1.20 z = 15 ω15 /EF = 0.71 ω7 /ω15 = 1.42 15/7 = 1.46 Table 10.1: Analysis of the dispersion,p as function of z, of the bump seen in the curves of Fig. 10.4. We note that the zi /7, with zi = 7, 10, 15 was computed assuming that the electrostatic limit for ωSP P is valid.

10.4

Purcell Effect in Hyperbolic Materials: Few Results

In this section we note that tunable strong light-matter interaction can be obtained by depositing graphene on a hyperbolic material, as is the case of hexagonal Boron Nitride (hBN) [see also Sec. 4.5]. The surface phononpolaritons of hBN [Dai et al. (2014)] can couple to the surface plasmonpolaritons on graphene giving rise to tunable surface phonon-polaritons which in turn can interact to a quantum emitter thus altering its decaying rate [Kumar et al. (2015)]. However, although the presence of graphene can lead to tunable phonon-polaritons, hBN alone can have a strong effect on the Purcell factor of a quantum emitter. Following [Kumar et al. (2015)], we have computed the Purcell factor for a quantum emitter in the presence of a 50 nm thick hBN crystal, considering that only the µz component of the dipole moment is finite. The results are presented in Fig. 10.5 and are identical to those reported in [Kumar et al. (2015)]. In this figure we see a dramatic enhancement of the Purcell factor, by several orders of magnitude (the effect is more pronounced for smaller distances to the hBN crystal), when the quantum emitter is located in the proximity of hBN, in the spectral range where the system presents type II hyperbolic behavior.

page 292

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Excitation of Plasmons by an Emitting Dipole

b2445-mas

293

Figure 10.5: Purcell factor of a quantum emitter in the presence of finite thickness (50 nm) hBN crystal. We took µx = µy = 0 and µz = 1. The spectral range scanned in between the vertical dashed lines is that where the system possesses type II hyperbolic behavior. The dielectric function used for hBN is defined in 4.5 and the crystal is standing on air.

As discussed in Sec. 4.5, in this spectral range the system supports surface phonon-polaritons, which can be excited by the proximity of a quantum emitter. That is, the emitter can decay via the excitation of surface waves in the hBN waveguide. We then see that this type of polaritons is an alternative (to plasmons) for controlling light-matter interactions at the nanoscale.

page 293

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

May 2, 2013 14:6 BC: 8831 - Probability and Statistical Theory

This page intentionally left blank

PST˙ws

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Chapter 11

Concluding Remarks

The field of plasmonics is growing, as it can be seen from the data-plot in a recent editorial in Nature Photonics [Editorial (2012)]. In that article it is shown that the number of publications in plasmonics has been growing steadily over the last twenty years. Broadly speaking, we can divide the field of plasmonics according to the nature of the surface-plasmon resonances. Whenever these resonances occur in localized nano-particles we talk about localized surface plasmon-polaritons [Willets and Duyne (2007); Pelton and Bryant (2013); Klimov (2014)]. When they occur at metal/dielectric surfaces one usually denotes them as (propagating) surface plasmon-polaritons [Sarid and Challener (2010)]. In both cases, these plasmonic resonances have wavelengths below the diffraction limit [Armstrong (2012)] and exhibit intense electric fields. For propagating surface plasmon-polaritons we are generally interested in the case of propagation along a thin metal film. Since 2004 the thinnest conductive film available has been a graphene sheet. It is natural to inquire whether graphene can support propagating surface plasmon-polaritons [Low and Avouris (2014)] (which can be excited by different methods; see Chapter 5 and [Bludov et al. (2013); Zhang et al. (2014)]). Indeed, the combination of graphene and plasmonics opened a new avenue to this exciting field. This recent branch of nanophotonics is nowadays known as graphene (nano)plasmonics. For example, graphene plasmons can be used to engineer nanoscale infrared light sources [Manjavacas et al. (2014)], and intrinsic plasmons on graphene have already been used for enhancing photodetection [Kim et al. (2014); Koppens et al. (2014)]. Graphene, however, is not the only two-dimensional material available these days [Castro Neto and Novoselov (2011); Novoselov and Castro Neto (2012)]. Many others, as dichalcogenides (MX2 ), hexagonal boron 295

page 295

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

296

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

nitride (hBN), phosphorene [Low et al. (2014b)], silicene, some oxides, and graphene multilayers [Low et al. (2014a); Wu et al. (2014b)], are waiting in line to be explored from the point of view of their electronic properties and light-matter interactions [Kim et al. (2014); Koppens et al. (2014)]. Indeed, a new class of materials, dubbed “van der Waals heterostructures” [Geim and Grigorieva (2013)], were conjectured to unleash a number of both new fundamental physics and new applications unforeseen until recently. On one hand, these new heterostructures [Kretinin et al. (2014)] can be made of two-dimensional materials (or, for that matter, of few layers of those materials); on the other hand, can be combined with more traditional materials, like noble metals [Yamaguchi et al. (2014); Chaves et al. (2014); Moriya et al. (2015)]. This opens a multitude of possibilities for light-matter interactions where plasmonics will certainly play a key role. Since graphene is intrinsically a surface, the coupling of surface plasmons to surface polar phonons of the underlying substrate, for instance hBN, is an interesting prospect, leading to hybrid surface phonon-plasmon polaritons [Luxmoore et al. (2014); Brar et al. (2014)], which appear as multiple dispersion branches. Furthermore, it has been shown that plasmons in graphene encapsulated in hBN possess very low damping [Woessner et al. (2015)]. Thus, this type of van der Waals heterostructure emerges as a plasmonic medium with high uniformity. As the field matures, low losses in plasmons propagation can be translated into long propagation lengths, which might open new routes for photonic/plasmonic-based communications and data transfer. On another topic, graphene-dichalcogenides van der Waals heterostructures, coupled to noble metals plasmonics, seem to work better as a chemical sensor than the same system in the absence of the heterostructure [Zeng et al. (2015)] (see also [Kravets et al. (2014)]); in this case, the plasmonic medium is the noble metal and not graphene, the latter acting as an intermediate for enhancing light-matter interactions. Also worth noting is the interaction of surface plasmons with grain boundaries in CVD-grown graphene. It has been shown that the reflection of plasmons at grain boundaries in graphene presents an anomalous scattering phase (different from π) [Fei et al. (2013); Nikitin et al. (2014)] (see also [Sánchez-Gil and Maradudin (1999); Polanco et al. (2013)] for calculations of SPPs scattering amplitudes in traditional plasmonics). Strongly related to the field of surface plasmon-polaritons is the emerging field of surface phonon-polaritons in van der Waals heterostructures, hBN and hBN/graphene structures being the most studied. Hexagonal Boron Nitride is a hyperbolic material, that is, the in-plane and the out-

page 296

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Concluding Remarks

9in x 6in

b2445-mas

297

of-plane dielectric constants have different signs [Jacob (2014); Dai et al. (2014); Caldwell et al. (2014); Kumar et al. (2015)]. As a consequence, hBN presents two Reststrahlen bands where free radiation cannot propagate. Within these bands the system behaves like a conventional metal (as concerns radiation propagation). The existence of these Reststrahlen bands allows the propagation of surface phonon-polaritons in hBN. When graphene is deposited on hBN, an additional coupling between the surface phonon-polaritons in hBN and the surface plasmon-polaritons in graphene becomes possible, giving rise to tunable plasmon-phonon-polaritons [Dai et al. (2015)]. These results are opening a new field in van der Waals heterostructures. Additionally, with the simple stacking of layered materials, a new degree of freedom enters in the game: the relative rotation of the lattices associated with different layers [Mishchenko et al. (2014)]. This rotation, say between a graphene layer on a boron nitride buffer layer, creates an external potential that splits the graphene bands, leading to the emergence of further plasmonic branches (dubbed spectrum reconstruction). The new avenue opened by this additional degree of freedom has not yet been fully explored [Tomadin et al. (2014)]. Another interesting line of research is that of plasmonics in graphene nano-structures [Christensen et al. (2014); Cox and de Abajo (2014); Nene et al. (2014); Wang et al. (2015); Yeung et al. (2014); Zhu et al. (2014)] or even in nanoparticles coated with graphene [Christensen et al. (2015a)] which may also exhibit non-linear optical response [Peres et al. (2014); Cox and de Abajo (2015)]. In fact, the non-linear optical response of graphene has recently been used to excite surface plasmons in this material [Constant et al. (2015)]. Graphene’s plasmonic response can also be put to good use for non-linear optics [Gullans et al. (2013)], and graphene itself is able to exhibit non-linear GSPs, as predicted by a recent work [Gorbach (2013)], and highly confined TE waves [Bludov et al. (2014)]. On a related topic, we can consider the combination of metallic nanoparticles, acting as a plasmonic material, with graphene. It has recently been shown that gold nano-disks can interact strongly with graphene, generating locally hot carriers which can be probed by femtosecond pump-probe measurements [Gilbertson et al. (2015)]. In this book we have only covered some aspects related to graphene plasmonics [Politano and Chiarello (2014); Low and Avouris (2014); Grigorenko et al. (2012); Xiao et al. (2016)]. We started by reviewing the basic proper-

page 297

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

298

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

ties of SPPs sustained at dielectric-metal interfaces, setting the stage for the discussion of SPPs in doped graphene. We then derived the dispersion relation of SPP in graphene, both in single-layer graphene and in double-layer graphene. We have seen that even for these simple geometries, the spectrum needs to be obtained by numerical means. From the corresponding solutions, it was clear that GSP-excitation is not feasible by simply striking light directly on graphene, since the dispersion curve always lies to the right of the light line. Therefore, in Chapter 5 we reviewed the most popular methods to couple electromagnetic radiation to GSPs (see also [Torre et al. (2015)] for a full-electrical plasmon detection method). Another interesting idea has been put forward in [Liu et al. (2015a)]. The excitation methods described in Chapter 5 cannot distinguish left from right propagation of plasmons. However, by putting graphene on a magneto-optical substrate, its dispersion relation becomes asymmetric in the forward and backward directions, thus allowing unidirectional excitation [Liu et al. (2015a)]. Motivated by a recent experiment reporting the excitation of GSPs using a metallic antenna [Alonso-González et al. (2014)], in Chapter 6 we have conducted a theoretical study of a similar system consisting of an infinitely long and highly conducting metal stripe placed on top of a graphene layer. In Chapter 7 we developed a general theoretical framework for describing the excitation of GSPs in systems where the graphene’s conductivity is periodically modulated. In particular, we have applied our analytical model to the case of a periodic array of graphene ribbons, since this setup has been extensively studied experimentally. We then confronted our theoretical results against the experimental data [Ju et al. (2011)], having observed a good agreement between theory and experiment (see also [Velizhanin (2015)]). In a recent experiment [Sorger et al. (2015)], GSPs’ excitation in graphene stripes grown in silicon carbide has been achieved, and the same model that was used in Chapter 7 was applied to the description of the experimental data. In Chapter 8 the case of a single graphene ribbon was considered in the electrostatic limit. The approach used was then applied to graphene disks and rings. The case of a groove was also discussed. If the groove is periodically repeated we achieve a diffraction grating, a problem that can be analyzed semi-analytically. In Chapter 9 an extension of Chapter 7 was presented, which consisted of an approach to deal with graphene on periodically corrugated surfaces, that is diffraction gratings. These can be made of either a dielectric or a metamaterial, as in the case discussed at the end of that Chapter. It is worth mentioning that graphene resting on a grating can be a source of THz radiation [Zhan et al. (2014)], when a

page 298

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Concluding Remarks

9in x 6in

b2445-mas

299

beam of electrons moves over its surface, a problem that we have analysed at the end of Chapter 5 . Finally, in Chapter 10 we discussed the excitation of SPP’s by an emitting dipole. We have shown that the decaying rate of a dipole is intimately tied to the excitation of SPP’s on graphene, a manifestation of the Purcell effect.

page 299

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

May 2, 2013 14:6 BC: 8831 - Probability and Statistical Theory

This page intentionally left blank

PST˙ws

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Appendix A

Derivation of the Susceptibility of Graphene (written with André Chaves)

In this Appendix we compute the electronic susceptibility of graphene. This quantity is defined by Eq. (2.75), which we now write with a slightly different, more convenient, notation1 : X Z d2 k nF (αEk ) − nF (α0 Ek+q ) χ(q, ω) = 4 Fαα0 (q, k) , (A.1) 4π 2 ω + αEk − α0 Ek+q + iε 0 α,α =±

where ε = 0+ , Fαα0 (q, k) =

1 2

1 + αα0

k2 + k · q k|k + q|

,

(A.2)

and h i−1 nF (E) = eβ(E−EF ) + 1 ,

(A.3)

where β = 1/(kB T ), with T the temperature and kB the Boltzmann constant. From here on we treat the case of zero temperature only. First, we P 0 write the susceptibility as χ(q, ω) = αα0 χαα (q, ω). Next, we separate the susceptibility into doped, χD (q, ω), and undoped, χU (q, ω), parts: χ(q, ω) = χD (q, ω) + χU (q, ω) .

(A.4)

By undoped part we mean the expression of χ(q, ω) that appears in the limit EF = 0, which is also present for EF 6= 0. The doped part is given by the remaining terms. A.1

Undoped Susceptibility

The term χU is the susceptibility when EF = 0 and is given by: −+ χU (q, ω) = χ+− U (q, ω) + χU (q, ω) .

(A.5)

It is convenient to determine both the imaginary and real parts separately. 1 In

what follows we choose vF = ~ = 1, which simplifies the calculations. 301

page 301

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

302

b2445-mas

An Introduction to Graphene Plasmonics

A.1.1

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

9in x 6in

The imaginary part of the undoped susceptibility

The imaginary part of χ+− U is null, because the argument of the δ−function is always positive, and the imaginary part of χ−+ is given by: U Z kdkdθ δ(ω − k − |k + q|)F−+ (q, k), (A.6) =mχU (q, ω) = −π π2 where we have used the Sokhotski-Plemelj formula. First we perform the integral over θ and we obtain: Z ω 1 2|ω − k| =mχU (q, ω) = −2 kdk p 2 2 q+ω 2π 2 4k q − (ω 2 − 2kω − q 2 )2 2k 2 + ω 2 − 2kω − q 2 × 1− , q>ω (A.7) 2k(ω − k) Z q+ω 2 2|ω − k| 1 kdk p =mχU (q, ω) = −2 2 q 2 − (ω 2 − 2kω − q 2 )2 2π ω−q 4k 2 2k 2 + ω 2 − 2kω − q 2 × 1− , qω

−1 π

q+ω 2

Z

ω−q 2

q 2 − ω 2 + 4kω − 4k 2 dk p , q ω −1

π

p

ω2 − q2

Z

q+ω 2

dk

p q 2 − ω 2 + 4kω − 4k 2 , q < (A.10) ω

ω−q 2

and finally =mχU (q, ω) = 0,

q>ω q2 =mχU (q, ω) = − p , 4 ω2 − q2 Let us now compute the real part of χU .

q 2kF , it follows s 2 2 π ω − 2k q 2k − ω 2k − ω F F F + arcsin . p 1− =mχ2D = + q q q 4π ω 2 − q 2 2 (A.43) After some trigonometric manipulations we can write s 2 2 q 2k − ω 2k − ω ω − 2k F F F π − arccos . p =mχ2D = + 1− q q q 4π ω 2 − q 2 (A.44) For q > ω and 2kF > ω + q we obtain Z kF p 1 =mχ2D = p dk (ω − 2k)2 − q 2 , (A.45) 2 2 ω+q π q −ω 2 which after integration, gives s 2 2 2k − ω 2k − ω q 2k − ω F F F . p − 1 − arccosh =mχ2D = q q q 4π q 2 − ω 2 (A.46) In all other cases =mχ2D is zero.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Derivation of the Susceptibility of Graphene

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

A.2.5

b2445-mas

307

Real Part of χ1D and χ2D

The real part of χ1D and χ2D is given by the Cauchy principal value of the expressions (A.28) and (A.29), that is Z 2π Z kF 2k 2 + kω + kq cos θ 1 1 dk 2 dθ kF the lower limit of the integral in k is zero, if Ω < kF the lower limit of the integral is kF − Ω. Then we can write Z kF Z 2π 1 I(ω, q) = kdk dψ[1 + cos(θk+q − θk )]δ[g(ψ)] vF ~ max(kF −Ω,0) 0 Z kF Z 2π 1 k + q cos ψ δ[g(ψ)] , kdk = dψ 1 + vF ~ max(kF −Ω,0) k+Ω 0 (M.6) p

with g(ψ) = k 2 + q 2 + 2kq cos ψ − k − Ω. Simplifying the δ−function, we write (after some algebra) p 1 (2k + Ω)2 − q 2 k + q cos ψ p δ[g(ψ)] = 1+ [δ(ψ − ψ0 ) + δ(ψ + ψ0 )] , k+Ω k q 2 − Ω2 (M.7) where ψ0 follows from g(ψ0 ) = 0. The integral in ψ is now elementary, and we obtain p Z kF (2k + Ω)2 − q 2 2 p dk Θ(q − Ω) , (M.8) I(ω, q) = vF ~ max(kF −Ω,0) q 2 − Ω2 where Θ(x) is the step function. A further constraint is imposed by the square root in the numerator: k > (q − Ω)/2 and since 0 < k < kF we determine the domain of q available for excitation of particle-hole pairs as Ω < q < 2kF + Ω ,

(M.9)

page 362

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Non-Radiative Decaying Rate: Electrostatic Calculation

b2445-mas

363

as shown in the right panel of Fig. M.1. Then, the integral I(ω, q) reads Z kF p 1 2 p dk (2k + Ω)2 − q 2 . I(ω, q) = (M.10) 2 2 vF ~ q − Ω max[kF −Ω,(q−Ω)/2] We now make the transformation of variable 2k + Ω = x followed by the transformation x = q cosh φ. The integral becomes elementary and we obtain q2 1 p I(ω, q) = v F ~ q 2 − Ω2 1 1 1 φ− − φ+ + sinh(2φ+ ) − sinh(2φ− ) 2 2 2 q2 1 p G(q) , (M.11) ≡ v F ~ q 2 − Ω2 where 2kF + Ω , (M.12) q max(2kF − Ω, q) . (M.13) φ− = arccosh q Finally, the decay rate reads Z (µ2z + µ2k cos2 θ) 1 q 2 e−2qz 1 2π e2 1 p =2 dq G(q) . (M.14) τ ~ 20 (2π)4 |(q, ω)|2 v F ~ q 2 − Ω2 φ+ = arccosh

Integrating over the angle θ we obtain 2 2 Z 2π e2 2πµz + πµk 2kF +Ω 1 dq q 3 e−2qz p G(q) . =2 τ ~ 20 (2π)4 ~vF |(q, ω)|2 q 2 − Ω2 Ω

(M.15)

The integral in q cannot be done analytically. We note that the integral vanishes for kF = 0, which is a consequence of the fact that only intraband transitions were considered. M.2

A Detour: Neutral Graphene

We now take a detour of our main line —plasmons in graphene— and show, following [Swathi and Sebastian (2009)], that neutral graphene also plays a role in the non-radiative decay rate of a quantum emitter, although it does not support plasmons. This role happens because graphene has no energy-gap and, therefore, particle-hole excitations from the valence band to the conduction band can take place at arbitrary low energies. As in the

page 363

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

364

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

previous section the quantity to be computed is the non-radiative decay rate, which for this case takes the form 1 2π X X = gs gv |hψk+q,+ |V |ψk,− i|2 δ(Ek+q,+ − Ek,− − ~ω) . (M.16) τ ~ q k

Note the differences between Eq. (10.1) and Eq. (M.16). We consider the case of graphene in vacuum. Following the same steps as in the previous section, we are faced with the calculation of an integral of the form [see Eq. (M.5)] Z ∞ Z 2π 1 kdk dψ[1 − cos(θk+q − θk )]δ(|k + q| + k − Ω) . I(ω, q) = vF ~ 0 0 (M.17) Following the same procedure as in the previous section, the integrand in Eq. (M.17) can be transformed into to p 1 q 2 − (Ω − 2k)2 p [1 − cos(θk+q − θk )]δ[g(ψ)] = [δ(ψ − ψ0 ) + δ(ψ + ψ0 )] , k Ω2 − q 2 (M.18) where g(ψ) = |k + q| + k − Ω and ψ0 follows from g(ψ0 ) = 0. The following conditions have to be enforced: Ω > q and q 2 > (Ω − 2k)2 , from which follows that (Ω − q)/2 < k < (Ω + q)/2. The integral in ψ becomes elementary, and the integral over k transforms into Z (Ω+q)/2 p 1 2 p dk q 2 − (Ω − 2k)2 . (M.19) I(ω, q) = vF ~ Ω2 − q 2 (Ω−q)/2 Introducing the change of variables Ω − 2k = x, followed by x = q sin θ, we obtain I(ω, q) =

q2 π p . 2vF ~ Ω2 − q 2

Thus, the expression for the decaying rate becomes Z Ω π 2 e2 q 3 e−2qz 1 2 2 p = 2 (µ + µ /2) dq . k τ 20 ~(2π)3 vF ~ z Ω2 − q 2 0

(M.20)

(M.21)

Let us now compute the integral over q in an approximate way. We introduce the change a variables q = xΩ. This leads to Z 1 Z Ω q 3 e−2qz x3 e−2xΩz dq p = Ω3 dx √ . (M.22) 1 − x2 Ω2 − q 2 0 0

page 364

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Non-Radiative Decaying Rate: Electrostatic Calculation

b2445-mas

365

In the limit Ωz 1, the integral over x is dominated by values of x 1. Then, we approximate the square root by one, following Z 1 Z ∞ 3 1 x3 e−2xΩz dx √ dxx3 e−2xΩz = . (M.23) Ω3 ≈ Ω3 2 8Ω z 4 1−x 0 0 Finally, the decaying rate reads 1 3˜ µ2 λ π 2 e2 3 1 2 2 = α , = 2 (µ + µ /2) z k τ 20 ~(2π)3 ~ 8ω z 4 64π0 ~ z 4

(M.24)

where λ is the wavelength of the radiation. Recalling the form of the decaying rate of a dipole in vacuum, Eq. (10.27), we obtain 32 µ ˜2 τvac =α 9 3 2 τ 2 π µ

4 λ , z

(M.25)

where µ ˜2 = µ2z + µ2k /2. In conclusion, the non-radiative decaying rate decreases with a z −4 dependence in the distance of the quantum emitter to graphene [Swathi and Sebastian (2009)].

page 365

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

May 2, 2013 14:6 BC: 8831 - Probability and Statistical Theory

This page intentionally left blank

PST˙ws

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Appendix N

Reflection Amplitude of an Electromagnetic Wave due to a Graphene Interface In this Appendix we derive the transmittance and reflectance amplitudes for T M (p−polarized) and T E (s−polarized) waves, when electromagnetic radiation impinges on graphene resting on a dielectric. First we consider the simple case of free standing graphene. Later we generalize to graphene clad by two different dielectrics.

N.1

The Simple Case of Free Standing Graphene

In this section we solve a very simple problem as a warm up exercise to the next section. The geometry of the problem is given in Fig. N.1. Let us first work out the scattering amplitudes for the p−polarized wave. We define the electric field to the left of graphene as E< = Ei + Et and to the

Figure N.1: Left: Geometry of the scattering problem for a p−polarized wave (the magnetic field is perpendicular to the plane of the drawing). Right: Geometry of the scattering problem for a s−polarized wave (the electric field is perpendicular to the plane of the drawing). 367

page 367

April 5, 2016

14:13

368

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

right as E> = Et . In terms of coordinates we have Ei = Ei (− sin θ, cos θ)ei(ki ·r−ωt) , Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

i(kr ·r−ωt)

Er = Er (− sin θ, − cos θ)e Et = Et (− sin θ, cos θ)e

i(kt ·r−ωt)

(N.1) ,

,

(N.2) (N.3)

where the wavevectors are defined as ki = k(cos θ, sin θ) ,

(N.4)

kr = k(− cos θ, sin θ) ,

(N.5)

kf = k(cos θ, sin θ) ,

(N.6)

where k is the wave number of the impinging radiation. The boundary conditions imply that the component of the field parallel to the interface must be continuous. This condition gives E>,k = E,k . The magnetic field is determined by Maxwell’s equation. Once this is known, the boundary condition reduces to k(Ei + Er − Et ) = ωµ0 σL (ω, q)Et cos θ .

(N.8)

Combining the two boundary conditions we obtain 2 Et , = Ei 2 + παfL (ω, q) cos θ παfL (ω, q) cos θ rp = 1 − tp = , 2 + παfL (ω, q) cos θ tp =

(N.9) (N.10)

where we have written σL (ω, q) = σ0 fL (ω, q), with σ0 = πe2 /(2h) and α the fine structure constant. For the s−polarized geometry, the boundary conditions are Ei,y + Er,y = Et,y , where the subscript y denotes the component of the electric field perpendicular to the plane of the drawing in Fig. N.1. The boundary condition for the magnetic field reads k cos θ(Ei,y − Er,y − Et,y ) = ωµ0 σT (ω, q)Et,y .

(N.11)

Solving the boundary conditions, we obtain Et,y 2 cos θ = , Ei,y 2 cos θ + παfT (ω, q) παfT (ω, q) rs = ts − 1 = − , 2 cos θ + παfT (ω, q) ts =

(N.12) (N.13)

page 368

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Reflection Amplitude of an Electromagnetic Wave due to a Graphene Interface

369

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

p where σT (ω, q) = σ0 fT (ω, q). We note that cos θ = kz,i /k = k 2 − kx2 /k. Thus, if the plane of incidence is rotate around the z−axis, we have cos θ = q q √ 2 2 2 2 2 k − kx − ky /k ≡ k − kρ /k ≡ 1 − s2 . For the Drude model, and neglecting the momentum dependence of fL/T (ω, q), rp and rs have the explicit forms rp =

2EF α cos θ , 2EF α cos θ + γ − iω

(N.14)

2EF α . 2EF α + cos θ(γ − iω)

(N.15)

and rs = −

For neutral graphene we take fL/T (ω) = 1. N.2

Reflection and Transmission Amplitudes: Fresnel Coefficients in the General Case

We start by computing the Fresnel coefficients for an interface containing a graphene sheet, as represented in Fig. N.2. We consider a planar interface

Figure N.2: Geometry of an incoming field, with general polarization, at a graphene interface, clad between two different dielectric media of relative permittivity 1 and 2 . The electric field has s− and p−components. The magnetic field is not shown.

page 369

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

370

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

at z = 0 between two media. Medium 1, z > 0, has a dielectric constant 1 , while medium 2 has dielectric constant 2 . We assume that there is a source of electromagnetic field in region 1. In each region the electric field can be written in general as Z Z d2 k dω i(k·rk −ωt) , (N.16) E(r, t) = 2 E(ω, k, z)e 2π (2π) where |k| = k, with k an in-plane two-dimensional vector. In a medium with relative dielectric constant n and relative permeability µn , the wave equation of the electric field E in the absence of source currents reads ∇ × ∇ × E + µn µ0 n 0

∂2E =0 ∂t2

(N.17)

Using the fact that ∇ × ∇× = ∇ · ∇ · −∇2 and the fact that if there are no free charges, we have ∇ · D = n 0 ∇ · E = 0, we obtain − ∇2 E(r) + µn µ0 n 0

∂2E = 0, ∂t2

which in terms of the Fourier components becomes ∂2 ω2 2 − 2 + k E(ω, k, z) − 2 E(ω, k, z) = 0. ∂z cn

(N.18)

(N.19)

The previous equation implies that E(ω, k, z) = E(ω, k, z). The general solution of the previous differential equation is given by E(ω, k, z) = E+ (ω, k)eikz,n z + E− (ω, k)e−ikz,n z , where p kz,n = sgn(ω) kn2 − k 2 + isgn(ω),

(N.20) √ and we have introduced the notation kn = ω/cn , and cn = 1/ n µn 0 µ0 . For kn2 > k 2 , the solutions correspond to propagating waves, while for kn2 < k 2 the solutions correspond to evanescent waves with p kz,n = i k 2 − kn2 . (N.21) The solution E+ (ω, k) corresponds to a wave propagating in the +z direction, while E− (ω, k) propagates in the −z direction. The condition ∇·E = 0 still has to be enforced. This is automatically satisfied if we write the field in terms of the polarization vectors: ± ± ± E± (ω, k) = Es,n (ω, k)e± s,n + Ep,n (ω, k)ep,n ,

(N.22)

page 370

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Reflection Amplitude of an Electromagnetic Wave due to a Graphene Interface

371

where we have introduced the polarization vectors (see Fig. P.1) e± (N.23) s,n = ek × ez , k kz,n e± ez ∓ ek , (N.24) p,n = kn kn where ek = (kx , ky , 0) /k and ez is the unit vector along the z direction. These two polarization vectors correspond to s− (transverse electric, TE) and p− (transverse magnetic, TM) polarizations of the electric field. For concreteness, in a coordinate system such that (kx , ky ) = 0, kk , the polarization vectors are given by e± (N.25) s,n = (1, 0, 0) , kz,n k . (N.26) , e± p,n = 0, ∓ kn kn The magnetic field strength follows from H = (iµω)−1 ∇ × E and is written as r r 0 n 0 n ± ± ± ± ± H (ω, k) = −Es,n (ω, k)ep,n + E (ω, k)es,n . (N.27) µ0 µn µ0 µn p,n From this we see the justification of the names TE and TM. For the s/TE polarization, the electric field is transverse to the incidence plane (which is spanned by the vectors ek and ez ), while for the p/TM polarizations it is H that is perpendicular to the plane of incidence. For the situation where we have isotropy and no Hall conductivity in the interface, both polarizations are decoupled from each other. Thus, in the following, we analyze then separately. Assuming that the 2D material, located at the interface, is isotropic, we want to study the situation where we have an incident electric field from − + +z, E− 1 , a reflected wave E1 , and a transmitted wave E2 . We write the TE and TM components of the electric field electric as ±(T E) ±(T E) E1/2 = E1/2 (1, 0, 0) , (N.28) ±(T M ) ±(T M ) E1/2 = E1/2 0, ∓kz,1/2 , k /k1/2 , (N.29) where we are assuming that kx = 0, for simplicity. The choice of signs in the polarization vectors obeys the condition that ∇ · E = 0 (for later use, it is good to have this in mind). Furthermore, recall that the in-plane momentum k reads k = (0, ky ) = (0, k), since kx = 0. With this convention, the magnetic field strength r components read respectively 0 1 ±(T E) ±(T E) E1/2 0, ±kz,1/2 , −k /k1/2 , (N.30) H1/2 = µ0 µ1 r 0 1 ±(T E) ±(T M ) H1/2 = E (1, 0, 0) . (N.31) µ0 µ1 1/2

page 371

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

372

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Let us analyse each component separately.

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

N.2.1

TE (transverse electric) / s−components

With the results (N.28) and (N.30) in mind, let us discuss the scattering of a transverse electric wave by a graphene sheet embeded in two different dielectrics. We assume the electric field is coming from +z. Therefore, we write −(T E)

E1

+(T E) E1 −(T E) E2 +(T E) E2

(T E)

= Ei = =

(1, 0, 0) ,

(N.32)

(T E) rs Ei (1, 0, 0) , (T E) ts Ei (1, 0, 0) ,

(N.33) (N.34)

= (0, 0, 0) ,

(N.35)

where rs and ts are the reflection and transmission amplitudes, respectively. The boundary condition (see Chap. 2) ˆ × (E1 − E2 ) = 0, n

(N.36)

implies that Esi + Esr = Est , Esi ,

(N.37) Esr ,

Est

are the incident, and where the notation has been simplified, and reflected, and transmitted amplitudes of the electric field, respectively, for and s−polarized electric field. The boundary condition (see Chap. 2) ˆ × (H1 − H2 ) = Jf,2D , n

(N.38)

implies kz2 t kz1 x Esi − Esr − E = µ0 ωJf,2D . (N.39) µ1 µ2 s We introduce the conductivity tensor, such that Jf,2D = σT ·E2D . Therefore we have two boundary conditions Esi + Esr = Est ,

(N.40)

and kz2 t kz1 Esi − Esr − E = µ0 ωσT Est . µ1 µ2 s Solving for Esr and Est we obtain: Esr µ2 kz1 − µ1 kz2 − µ1 µ2 µ0 ωσT = , Esi µ2 kz1 + µ1 kz2 + µ1 µ2 µ0 ωσT Et 2µ2 kz1 ts = si = , Es µ2 kz1 + µ1 kz2 + µ1 µ2 µ0 ωσT

rs =

(N.41)

(N.42) (N.43)

page 372

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Reflection Amplitude of an Electromagnetic Wave due to a Graphene Interface

373

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

where σT is the transverse conductivity (see Appendix C). It is easy to see that ts = 1 + rs .

(N.44)

We can show that these last three results reduce to the case discussed in Sec. N.1 when 1 = 2 = 0 . N.2.2

TM (transverse magnetic) / p−components

With the results (N.29) and (N.31) in mind, let us discuss the scattering of a transverse magnetic wave by a graphene sheet embeded in two different dielectrics. The magnetic field strength is transverse and is given by r 1 0 i Epi , 0, 0 , (N.45) Hp = µ1 µ0 r 1 0 Epr , 0, 0 , (N.46) Hrp = µ1 µ0 r 2 0 Htp = Ept , 0, 0 . (N.47) µ2 µ0 The boundary condition ˆ × (E1 − E2 ) = 0 , n

(N.48)

tells us that kz1 i kz1 r kz2 t Ep − Ep = E k1 k1 k2 p ckz1 ckz2 ckz1 Ei − √ Er = √ E t , (N.49) ⇔ √ 1 µ1 ω p 1 µ1 ω p 2 µ2 ω p

i r t Epy + Epy = Epy ⇔

while the boundary condition ˆ × (H1 − H2 ) = Jf,2D , n

(N.50)

tells us that r r r 1 0 i 1 0 r 2 0 t kz2 t ckz2 y Ep + Ep − E = Jf,2D = σL E = σL √ Et , µ1 µ0 µ1 µ0 µ2 µ0 p k2 p 2 µ2 ω p (N.51) where σL is the longitudinal conductivity (see Appendix C). Therefore, solving the two following conditions kz1 kz1 kz2 Ei − √ Er = √ Et , √ 1 µ1 p 1 µ1 p 2 µ2 p

(N.52)

page 373

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

374

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

and

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

r

1 i E + µ1 p

r

1 r E − µ1 p

r

2 t σL kz2 Ep = Et √ µ2 ω0 2 µ2 p

(N.53)

for Epr and Ept we obtain: rp =

Epr kz1 2 − kz2 1 + kz1 kz2 σL /(0 ω) = Epi kz1 2 + kz2 1 + kz1 kz2 σL /(0 ω)

2 /kz2 − 1 /kz1 + σL /(0 ω) , 2 /kz2 + 1 /kz1 + σL /(0 ω) r Ept 2kz1 2 1 µ2 tp = i = Ep kz1 2 + kz2 1 + kz1 kz2 σL /(0 ω) µ1 2 r 22 /kz2 1 µ2 = . 2 /kz2 + 1 /kz1 + σL /(0 ω) µ1 2 =

The coefficients obey the following relation: r kz1 2 µ2 tp = (1 − rp ) . kz2 1 µ1

(N.54)

(N.55)

(N.56)

We can show that these last three results reduce to the case discussed in Sec. N.1 when 1 = 2 = 0 . It is also possible to generalize the above expressions for the reflection and transmission amplitudes to the case where a magnetic field perpendicular to the graphene plane is present [Kort-Kamp et al. (2015)]. This is important in the discussion of the effect of a magnetic field in the Purcell factor.

page 374

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Appendix O

Green’s Functions of a Rope with Two Different Mass Densities Subject to a Point-Like Excitation (written with Bruno Amorim) It is perhaps surprising to find a problem of mechanics in a book about plasmonics. However, this appendix in meant as a prelude to the next one. Here we discuss a problem that is quite similar to the calculation of the Green’s functions of a radiating dipole in the presence of an interface, but without the complexity of matrix Green’s functions. The study of this appendix may facilitate the reading of the following one. O.1

The Homogeneous Rope

Let us consider a uniform rope under stress, which we describe by tbe Lagrangian density 1 1 2 (O.1) L = ρφ˙ 2 − Y (∂x φ) , 2 2 where φ(x, t) is the height profile of the rope, ρ is the mass density, Y is the tension of the rope, φ˙ = ∂φ/∂t p and ∂x φ = ∂φ/∂x. The waves propagate with a velocity given by c = Y /ρ. The equation of motion for the height field is given by ρφ¨ = Y ∂x2 φ.

(O.2)

We now want to consider the response of the rope to an external perturbation. O.1.1

Response to a localized force

Let us subject the rope to an external force at x = 0 and t = 0, F (x, t) = f δ(x)δ(t), such that the Lagrangian density reads L=

1 ˙2 1 2 ρφ − Y (∂x φ) − φF, 2 2 375

(O.3)

page 375

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

376

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

and the equation of motion become

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

ρφ¨ = Y ∂x2 φ + f δ (x) δ(t) .

(O.4)

We want to obtain φ as a function of f . Performing a Fourier transform of the equation of motion and using the definition Z dωdk ikx −iωt e , (O.5) φ(x, t) = 2 φ(k, ω)e (2π) we obtain 1 f, −ρω 2 + Y k 2

(O.6)

eikx e−iωt . (2π) −ρω 2 + Y k 2

(O.7)

dt0 dx0 G(x − x0 ; t − t0 )F (x0 , t0 ),

(O.8)

φ(k, ω) = which implies Z φ(x, t) = f

dωdk

2

This allows to write Z

t

φ(x, t) = −∞

where we have defined the Green’s function for the rope by Z dωdk eikx e−iωt G(x; t) = . 2 (2π) −ρω 2 + Y k 2

(O.9)

To obtain a retarded response we perform the usual replacement ω → ω + i0+ . It is useful for later use to invert the Fourier transform in space, thus obtaining Z Z eikx 1 eikx dk dk G(x; ω) = = . 2π −ρω 2 + Y k 2 Y 2π (k − ω/c − i0+ ) (k + ω/c + i0+ ) (O.10) For x > 0 we can close the contour in the upper half plane, collecting the contribution from the pole at k = ω/c + i0+ and obtaining (for x > 0) G(x; ω) = i

eiωx/c . 2Y ω/c

(O.11)

For x < 0 we can close the contour in the lower half plane, collecting the contribution from the pole at k = −ω/c − i0+ and obtaining Z dk eikx e−iωx/c G(x; ω) = = i . x < 0. (O.12) 2π −ρω 2 + Y k 2 2Y ω/c

page 376

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Green’s Functions in the Rope Problem

b2445-mas

377

Writing both cases in a unified way we have

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

G(x; ω) = i

eiω|x|/c . 2Y ω/c

(O.13)

Finally, the height field is given by φ(x, ω) = G(x; ω)f.

(O.14)

Notice that integrating the equation of motion Eq. (O.4), around x = 0 we would obtain the condition Y ∂x φ(0+ ) − Y ∂x φ(0− ) = −f.

(O.15)

Therefore the Green’s function should obey such discontinuity condition: Y ∂x G(x = 0+ ) − Y ∂x G(x = 0− ) = −1.

(O.16)

Indeed, we can check that Eq. (O.13) satisfies the previous condition 1 ∂ G(x; ω) = − (O.17) lim+ x→0 ∂x 2Y ∂ 1 lim G(x; ω) = . (O.18) 2Y x→0− ∂x O.2

The Inhomogeneous Rope

Let us suppose now that we have an inhomogeneous rope such that for x > 0 it has a mass density ρ1 and tension Y1 and for x < 0 it has a mass density ρ2 and tension Y2 . The Lagrangian density describing this situation is given by 1 1 2 x > 0, (O.19) L = ρ1 φ˙ 2 − Y1 (∂x φ) , 2 2 1 1 2 L = ρ2 φ˙ 2 − Y2 (∂x φ) , x < 0. (O.20) 2 2 Having two different tension values in the two different parts of the rope is perhaps a bit artificial. O.2.1

Reflection and transmition coefficients

We now want to discuss the scattering of an incoming wave at the interface between the two different pieces of a rope (in terms of the electric field problem of the next appendix, this corresponds to the scattering at the interface between two different dielectrics). Let us assume we have an incoming wave from x → ∞ φi e−iωt e−iωx/c1 ,

(O.21)

page 377

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

378

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

p where ci = Yi /ρi , with i = 1, 2, refers to the speed of the wave in the medium i. The solution everywhere is of the form φ(x > 0, t) = φi e−iωt e−iωx/c1 + rφi e−iωt e+iωx/c1 , φ(x < 0, t) = tφi e

−iωt −iωx/c2

e

,

(O.22) (O.23)

where r and t are the reflection and transmission coefficients, which need to be determined. At x = 0 we have the following boundary conditions apply: φ(0+ ) = φ(0− ) , +

(O.24) −

Y1 ∂x φ(0 ) = Y2 ∂x φ(0 ) ,

(O.25)

which translate into 1 + r = t,

(O.26)

−Y1 k1 + Y1 k1 r = −Y2 k2 t , (O.27) p and where we have defined ki = ρi /Yi ω for i = 1, 2. Solving this set of equations we obtain Y1 k1 − Y2 k2 , Y1 k1 + Y2 k2 2Y1 k1 t= . Y1 k1 + Y2 k2

r=

(O.28) (O.29)

These coefficients will emerge again in what follows. O.2.2

Response to an external force in the inhomogeneous regime

Low let us apply an external force at x = x0 > 0 of the form F = f δ (x − x0 ) (in the electromagnetic problem of the following appendix, a radiating dipole plays the role of the force in this mechanical problem). Then, the equations of motion become ρ1 φ¨ = Y1 ∂x2 φ + f δ(x − x0 ), x > 0 , ρ2 φ¨ = Y2 ∂x2 φ, x < 0 .

(O.30) (O.31)

Integrating the first equations from x0 − to x0 + an taking the limit → 0 we obtain the boundary condition at x = x0 : − Y1 ∂x φ(x+ 0 ) − Y1 ∂x φ(x0 ) + f = 0

(O.32)

page 378

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Green’s Functions in the Rope Problem

379

Therefore we now have four boundary conditions (two at x = 0 and other two at x = x0 ) Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

φ(0+ ) − φ(0− ) = 0 , +

−

(O.33)

Y1 ∂x φ(0 ) − Y2 ∂x φ(0 ) = 0 ,

(O.34)

− φ(x+ 0 ) − φ(x0 ) − Y1 ∂x φ(x+ 0 ) − Y1 ∂x φ(x0 )

= 0,

(O.35)

= −f .

(O.36)

We write the solution in the whole space as −iωt ik1 x φ(x0 < x, t) = φ> e , I e

φ(0 < x < x0 , t) = φ(x < 0, t) =

−iωt ik1 x −iωt −ik1 x φ> e + φ< e , II e II e < −iωt −ik2 x φIII e e ,

(O.37) (O.38) (O.39)

φ> I,II

where k1/2 = ω/c1/2 , and represents the amplitude of the waves that are propagating towards x → ∞ and φ< II,III the amplitudes of the waves that are propagating towards x → −∞. With this choice for the fields, the boundary conditions become < < φ> II + φII − φIII = 0 , < < Y1 k1 φ> II − k1 φII − Y2 −k2 φIII = 0 , > < −i2k1 x0 φ> = 0, I − φII + φII e > > < −i2k1 x0 φI − φII − φII e = −e−ik1 x0 f /(iY1 k1 ) .

(O.40) (O.41) (O.42) (O.43)

It is easy to solve this system of equations obtaining if ik1 x0 Y1 k1 − Y2 k2 if −ik1 x0 e + e , (O.44) φ> I = 2Y1 k1 2Y1 k1 Y1 k1 + Y2 k2 if ik1 x0 Y1 k1 − Y2 k2 e , (O.45) φ> II = 2Y1 k1 Y1 k1 + Y2 k2 if ik1 x0 φ< e , (O.46) II = 2Y1 k1 2Y1 k1 if ik1 x0 e . (O.47) φ< III = 2Y1 k1 Y1 k1 + Y2 k2 In the above expressions we recognize the presence of the reflection and transmission coefficients that we have obtained in the previous section. The full solution to φ is therefore given by if −ik1 x0 ik1 x if ik1 x0 ik1 x φI (x0 < x) = e e +r e e , (O.48) 2Y1 k1 2Y1 k1 if ik1 x0 −ik1 x if ik1 x0 ik1 x φII (0 < x < x0 ) = e e +r e e , (O.49) 2Y1 k1 2Y1 k1 if ik1 x0 −ik2 x φIII (x < 0) = t e e , (O.50) 2Y1 k1

page 379

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

380

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

The solution can be recast in the appealing form [cf. P.70-P.72] φI (x0 < x) = Gi> (x, x0 ; ω) + Gr (x, x0 ; ω) f φII (0 < x < x0 ) = Gi< (x, x0 ; ω) + Gr (x, x0 ; ω) f φ

III

t

(x < 0) = G (x, x0 ; ω)f

(O.51) (O.52) (O.53)

where we have introduced the Green’s functions i e−ik1 x0 eik1 x , 2Y1 k1 i Gi< (x, x0 ; ω) = eik1 x0 e−ik1 x , 2Y1 k1 i Gr (x, x0 ; ω) = r eik1 x0 eik1 x , 2Y1 k1 i Gt (x, x0 ; ω) = t eik1 x0 e−ik2 x . 2Y1 k1 Gi> (x, x0 ; ω) =

(O.54) (O.55) (O.56) (O.57)

We recognize that the Green’s functions Gi> (x, x0 ; ω) and Gi< (x, x0 ; ω) are actually just the Green’s function of a homogeneous rope characterized by ρ1 and Y1 : Gi> (x, x0 ; ω) = Gi< (x, x0 ; ω) = i

eiki |x−x0 | . 2Y1 k1

(O.58)

Since the Green’s functions represent the response to an external stimulus, Eqs. (O.51)-(O.53) have the following physical interpretation: the external force f at x = x0 emits a primary wave in both directions along the x axis with amplitude Gi≷ (x, x0 ; ω) f . The wave that goes towards x → −∞ is reflected and transmitted at the interface x = 0. The amplitude of the reflected wave is obtained by multiplying the primary wave by the reflection coefficient r. The reflected wave seems to be emitted from the position x = −x0 . The amplitude of the transmitted wave is obtained by multiplying the amplitude of the primary wave by the transmission coefficient t. The transmitted wave seems to be emitted from position x = k1 x0 /k2 . The last result is a consequence of the change of the material properties of the rope as we pass through x = 0. These results can be applied to other kinds of waves, provided we know the form of the Green’s functions and the form of the reflection and transmission coefficients, as we shall see in the following appendix. For future use, we note that the physical quantities introduce in this appendix relate to those of the next one by the following

page 380

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

Green’s Functions in the Rope Problem

b2445-mas

381

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

mapping: φ → E, 1 Y → , µµ0 ρ → 0 ,

(O.59)

f → iωjf (ω) ,

(O.62)

G(x, x0 ; ω) → µµ0 G(r, r0 ; ω) ,

(O.60) (O.61) (O.63)

where E is the electric field, µµ0 and 0 are the magnetic permeability and the dielectric permittivity of the medium, respectively, ω is the frequency of the emitting dipole, jf (ω) is the current associated with the emitting dipole, and G(r, r0 ; ω) is the matrix Green’s function. The reason why we have a matrix Green’s function for the radiating dipole problem is due to the vectorial nature of the electric field.

page 381

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

May 2, 2013 14:6 BC: 8831 - Probability and Statistical Theory

This page intentionally left blank

PST˙ws

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Appendix P

Derivation of the Transition Rate of a Quantum Emitter Near an Interface (written with Bruno Amorim) Here consider the problem of deriving Eq. (10.38). The final expression needs the general results of Appendix N, as they define the reflectance amplitudes for the s− and p−polarizations. We will see that the problem of determining the transition rate of a dipole can be cast in terms of matrix Green’s functions (also termed dyadic Green’s functions). The reader may want to read first Appendix O, which is meant as prelude to this one. Using first order perturbation theory, we can prove[Novotny and Hecht (2014)] that the lifetime of a two-level system is given by

2ω 2 µµ0 ∗ 1 = µge · =mG (r0 , r0 ; ω) · µge , τ ~

(P.1)

where µ is the relative permeability, µ0 is the vacuum permeability, G (r0 , r0 ; ω) is the electromagnetic Green’s function at the position of the ˆ |ei ≡ (µx , µy , µz ) is the dipole operator matrix element dipole, µTge = hg| d (and T stands for the transpose operation), ω = e − g , is the frequency of the emitting dipole, g and e are the energies of the ground and excited states, respectively, and r0 is the position of the dipole. The goal is to compute 1/τ for a dipole near a flat interface covered with graphene. This is a rather long Appendix, but its study will pay off, since the reader will be, in the end, equipped with all the tools needed to tackle more complex problems. A note on notation is in order: d2 k stands for a 2D in-plane integration, whereas d3 k stands for a 3D integration. We √ also use n = for the refractive index of the medium where the dipole is embedded. When used as a subindex, n refers to the medium with relative dielectric constant n . 383

page 383

April 5, 2016

14:13

384

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

P.1

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Polarization Vectors and Green’s Functions

The aim of this section is to define the polarization vectors, depicted in Fig. P.1, to write the electric and magnetic fields in terms of these vectors, and, finally, to obtain the free space Green’s function and the Green’s functions in the presense of an interface in terms of the polarization vectors.

Figure P.1: Definition of the polarization vectors in the interface problem. These ± are: e± s,n = (1, 0, 0) and ep,n = (0, ∓kz,n /kn , k/kn ). Note that k is the absolute value of the in-plane momentum and should not be confused with kn = ω/vn , with vn the velocity in medium n.

P.1.1

Definition of s− and p−polarization vectors and angular spectrum representation

For the sake of completeness, here we repeat the beginning of Sec. N.2. Any electric field can be written in general form Z Z dω d2 k i(k·rk −ωt) E(r, t) = , (P.2) 2 E(ω, k, z)e 2π (2π) where |k| = k, with k an in-plane two-dimensional vector. In a medium with relative dielectric constant n and relative permeability µn , the wave

page 384

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Derivation of the Transition Rate of a Quantum Emitter Near an Interface

385

equation of the electric field E in the absence of source currents reads

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

∇ × ∇ × E + µn µ0 n 0

∂2E =0 ∂t2

(P.3)

Using the fact that ∇ × ∇× = ∇ · ∇ · −∇2 and the fact that if there are no free charges, we have ∇ · D = n 0 ∇ · E = 0, we obtain ∂2E = 0, ∂t2 which in terms of the Fourier components becomes ω2 ∂2 − 2 + k 2 E(ω, k, z) − 2 E(ω, k, z) = 0. ∂z cn − ∇2 E(r) + µn µ0 n 0

(P.4)

(P.5)

The previous equation implies that E(ω, k, z) = E(ω, k, z). The general solution of the previous differential equation is given by E(ω, k, z) = E+ (ω, k)eikz,n z + E− (ω, k)e−ikz,n z , where p kz,n = sgn(ω) kn2 − k 2 + isgn(ω),

(P.6) √ and we have introduced the notation kn = ω/cn , and cn = 1/ n µn 0 µ0 . For kn2 > k 2 , the solutions correspond to propagating waves, while for kn2 < k 2 the solutions correspond to evanescent waves with p (P.7) kz,n = i k 2 − kn2 . The solution E+ (ω, k) corresponds to a wave propagating in the +z direction, while E− (ω, k) propagates in the −z direction. The condition ∇·E = 0 still has to be enforced. This is automatically satisfied if we write the field in terms of the polarization vectors: ± ± ± E± (ω, k) = Es,n (ω, k)e± s,n + Ep,n (ω, k)ep,n ,

(P.8)

where we have introduced the polarization vectors (see Fig. P.1) e± s,n = ek × ez , k kz,n e± ez ∓ ek , p,n = kn kn

(P.9) (P.10)

where ek = (kx , ky , 0) /k and ez is the unit vector along the z direction. These two polarization vectors correspond to s− (transverse electric, TE) and p− (transverse magnetic, TM) polarizations of the electric field. For

page 385

April 5, 2016

14:13

386

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

concreteness, in a coordinate system such that (kx , ky ) = 0, kk , the polarization vectors are given by e± s,n = (1, 0, 0) , kz,n k ± ep,n = 0, ∓ , . kn kn

(P.11) (P.12)

The magnetic field strength follows from H = (iµω)−1 ∇ × E and is written as r r 0 n 0 n ± ± ± H± (ω, k) = −Es,n (ω, k)e± + E (ω, k)e . p,n s,n µ0 µn µ0 µn p,n (P.13) From this we see the justification of the names TE and TM. For the s/TE polarization, the electric field is transverse to the incidence plane (which is spanned by the vectors ek and ez ), while for the p/TM polarizations it is H that is perpendicular to the plane of incidence. For the situation where we have isotropy and no Hall conductivity in the interface, both polarizations are decoupled from each other. Thus, in the following, we analyze then separately. P.1.2

The free space Green’s function

In the presence of a free source current Jf in a medium with dielectric constant n and permeability µn , the wave equation of the electric field E reads ∂Jf ∂2E = −µn µ0 . ∂t2 ∂t The electric field can be written in terms of the source current as Z Z ∂Jf 0 0 E(t, r) = dt0 d3 r0 G(t, r; t0 , r0 ) · −µn µ0 (t , r ) , ∂t ∇ × ∇ × E + µn µ0 n 0

(P.14)

(P.15)

where G(r, t; r0 , t0 ) is the electric field dyadic Green’s function, defined by the following equation 1 ∂2G = Idδ(r)δ(t) , (P.16) c2 ∂t2 where Id is the 3 × 3 identity matrix. If we have translational invariance, G(t, r; t0 , r0 ) = G(t − t0 , r − r0 ) and performing a Fourier transform in space and time, we obtain ∇ · ∇ · G − ∇2 G +

E(ω, k) = iµn µ0 ωG(ω, k) · Jf (ω, k),

(P.17)

page 386

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Derivation of the Transition Rate of a Quantum Emitter Near an Interface

387

and

k 2 − kn2 δij − ki kj Gjk (ω, k) = δik .

(P.18)

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

10

Isotropy imposes that Gij must be of the form Gij = aδij + bki kj . Using this form, the previous equation can be easily inverted and we obtain 1 ki kj . (P.19) Gij (ω, k) = δij − 2 2 kn k − kn2 Note that Gij (ω, k) has longitudinal a component that will disappear when we perform below the Fourier transform to real-space in the kz coordinate. At will soon be clear the final result is purely transverse. Performing and inverse Fourier transform Z in the z coordinate we obtain dkz Gij (ω, kk , z) = Gij (ω, k)eikz z 2π Z dkz ki kj eikz z = δij − 2 2 2π kn kz + kk2 − kn2 . Z ki kj eiqz z dkz δij − 2 (P.20) = 2π kn (kz − kz,n ) (kz + kz,n ) q The definition of kz,n = kn2 − kk2 is such that =mkz,n > 0. Therefore, for z > 0, the integration can be deformed into the upper complex half-space and collecting the pole at kz,n . The obtained result is eikz,n z c2 Gij (ω, kk , z) = i δij − 2 ki kj . (P.21) ω kz →kz,n 2kz,n In a coordinate system such that (kx , ky ) = 0, kk we obtain 1 1 2 k2 kz,n k k k k ki kj − kk2z,n 1 − k2k − kk2z,n = 2 = δij − 2 k n n n n 2 kn kk kz →kz,n k2 k k k k − kk2z,n 1 − kz,n − kk2z,n 2 2 kn n n n 0 1 i k h kz,n kk = 0 · 1 0 0 + − kz,n · .(P.22) 0 − n kn kn kk 0 k n

Comparing with Eqs. (P.11) and (P.12), we recognize that 1 k k qz2 + + + − kk2z,n = e+ 2 k s,n ⊗ es,n + ep,n ⊗ ep,n . n n 2 kk kk kz,n − k2 k2 n

(P.23)

n

is because R · G(k) · RT = G(R · k), where R is a rotation matrix, if G(k) has the given form. 10 This

page 387

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

388

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

For z < 0, the integral in Eq. (P.20) can be performed by deforming the contour into the lower half-plane and collecting the contribution at −kz,n . Therefore, the Green’s function can be written as i ± ± ± G0 (ω, kk ) = e±ikz,n z e± (P.24) s,n ⊗ es,n + ep,n ⊗ ep,n , 2kz,n where ⊗ represents a dyadic or tensor product and the + sign is valid for z > 0 and the − sign for z < 0. Note that in the derivation we have assumed that the emitting dipole is located at z = 0. It is also instructive to express the local electric field in terms of the real-space Green’s functions. Let us now see the connection between the electric field of a dipole d with the free space Green’s function. If we have a free dipole described by the polarization Pf (r, t) = d(t)δ (r − r0 ) ,

(P.25)

then we have a free current11 ∂d(t) δ (r − r0 ) , (P.26) ∂t and the electric field generated by the dipole is, from Eq. (P.15), given by Z ∂ 2 d(t0 ) E(r, t) = −µµ0 dt0 G(r, r0 ; t, t0 ) · . (P.27) ∂t02 or, after making a Fourier transform in time, by Jf (r, t) =

E(r, ω) = µµ0 ω 2 G(r, r0 ; ω) · d(ω).

(P.28)

This result will be used ahead. P.1.3

Green’s functions for problems with flat interfaces I

Eq. (P.24) is very useful as allows one to naturally interpret results in terms of emitted waves with s− and p−polarization. For example, suppose we wave a dipole, d, located at z = z0 . The electric field emitted by the dipole is given by E0 (ω, k) = µn µ0 ω 2 G0 (ω, k) · d(ω, k) ± i = e±ikz,n (z−z0 ) e± s,n es,n · d(ω, k) 2kz,n ± i + e±ikz,n (z−z0 ) e± (P.29) p,n ep,n · d(ω, k) , 2kz,n and we have an emitted electric field in the ±z direction and s-polarization with amplitude i 0,± Es,n (ω, k) = e± · d(ω, k), (P.30) 2kz,n s,n 11 In

frequency space the current density reads Jf (r, t) = −iωdδ (r − r0 ) ≡ jδ (r − r0 ).

page 388

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Derivation of the Transition Rate of a Quantum Emitter Near an Interface

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

and an electric field with p-polarization with amplitude i 0,± Ep,n (ω, k) = e± · d(ω, k). 2kz,n p,n

389

(P.31)

If we have an interface located at z = 0, the field emitted in the −z direction will be reflected at the interface. At the interface the emitted electric field is given by 0,− 0,− ikz,1 z0 − ep,1 . Es,n (ω, k)eikz,1 z0 e− s,1 + Ep,n (ω, k)e

(P.32)

Since we already have the field decomposed in s− and p−polarizations, the reflected wave can be written in terms of Fresnel coefficients. The reflected field at the interface is simply given by (s)

(p)

0,− 0,− ikz,1 z0 − r2←1 Es,n (ω, k)eikz,1 z0 e− ep,1 . s,1 + r2←1 Ep,n (ω, k)e

(P.33)

Therefore the total electric field for z0 > z > 0 is given by 0,− 0,− ikz,1 (z0 −z) − E(z, z0 , k, ω) = Es,n (ω, k)eikz,1 (z0 −z) e− ep,1 s,1 + Ep,n (ω, k)e (s)

0,− + r2←1 Es,n (ω, k)eikz,1 (z+z0 ) e− s,1 (p)

0,− + r2←1 Ep,n (ω, k)eikz,1 (z+z0 ) e− p,1 µ1 µ0 ω 2 n −ikz,1 (z−z0 ) − e es,1 ⊗ e− =i s,1 2kz,1 o − + e−ikz,1 (z−z0 ) e− p,1 ⊗ ep,1 · d µ1 µ0 ω02 n (s) ikz,1 (z0 +z) + r2←1 e es,1 ⊗ e− +i s,1 2kz,1 o (p) − + r2←1 eikz,1 (z0 +z) e+ p,1 ⊗ ep,1 · d ,

(P.34)

where in the second equality we have used Eqs. (P.30) and (P.31). For z > z0 , the total electric field is given by o µ1 µ0 ω02 n ikz,1 (z−z0 ) + ikz,1 (z−z0 ) + E(z, z0 , k, ω) = i e es,1 ⊗ e+ ep,1 ⊗ e+ s,1 + e p,1 · d 2kz,1 µ1 µ0 ω02 n (s) ikz,1 (z0 +z) + r2←1 e es,1 ⊗ e− +i s,1 2kz,1 o (p) − + r2←1 eikz,1 (z0 +z) e+ (P.35) p,1 ⊗ ep,1 · d. For z < 0, we have a transmitted electric field that is given by (s)

−(s) ikz,1 z0 −ikz,2 z − e e es,2

E(z, z0 , k, ω) = t(12) E0

−(p) ikz,1 z0 −ikz,2 z − e e ep,2

+ E0

µ1 µ0 ω02 n (s) ikz,1 z0 −ikz,2 z − e es,2 ⊗ e− t2←1 e s,1 2kz,1 o (p) − + t2←1 eikz,1 z0 e−ikz,2 z e− p,2 ⊗ ep,1 · d ,

=i

(P.36)

page 389

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

390

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

where in the second equality we have used Eqs. (P.30) and (P.31). Note that for the transmitted field both the polarization vectors of the media 1 and 2 appear. The previous equations must be read from right to left. Thus, in the case of Eq. (P.36) the dipole vector contracts, for example, with the polarization vector e− p,1 to give the amplitude of the incident field at the interface, via Eq. (P.31). The final result comes proportional to the polarization vector e− p,2 which gives the polarization of the transmitted field in medium 2. In summary, we can write E(z, z0 , k, ω) = µ1 µ0 ω 2 G(z, z0 , k, ω0 ) · d,

(P.37)

where the Green’s function is written for z > 0 as G(z, z0 , k, ω0 ) = G0 (z, z0 , k, ω0 ) + Gr (z, z0 , k, ω0 ),

(P.38)

with i n (s) ikz,1 z0 ikz,1 z + r e e es,1 ⊗ e− s,1 2kz,1 2←1 o (p) − + r2←1 eikz,1 z0 eikz,1 z e+ p,1 ⊗ ep,1 ·

(P.39)

G(z, z0 , k, ω0 ) = Gt (z, z0 , k, ω0 ) i n (s) ikz,1 z0 −ikz,2 z − = t e e es,2 ⊗ e− s,1 2kz,1 2←1 o (p) − + t2←1 eikz,1 z0 e−ikz,2 z e− p,2 ⊗ ep,1 .

(P.40)

Gr (z, z0 , k, ω0 ) =

and for z < 0

This concludes the relation between the matrix Green’s function and the polarization vectors, with the former being written in terms of the latter. We end this section by noting that in the Weyl gauge the electromagnetic field scalar potential is set to zero, φ = 0, and E = −∂A/∂t. Therefore, we have that E = iωA ,

(P.41)

A(ω, k) = µn µ0 G(ω, k) · Jf (ω, k),

(P.42)

and Eq. (P.17) becomes

therefore G coincides with the Green’s function for the vector potential A in the Weyl gauge.

page 390

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Derivation of the Transition Rate of a Quantum Emitter Near an Interface

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

P.2

page 391

391

Dipole Decaying Rate

To compute Eq. (P.1) we need the Green’s function in real space at the position of dipole. For a dipole close to an interface, at position r0 = (0, 0, z0 ), we have Z d2 k r 0 G (r0 , r0 ; ω) = G (r0 , r0 ; ω) + 2 Gs (z0 , z0 ; ω; k) (2π) Z d2 k r + (P.43) 2 Gp (z0 , z0 ; ω; k) , (2π) where G0 (r0 , r0 ; ω) is the free Green’s function in real space, Grs (z0 , z0 ; ω; k) is given by Eq. (P.84), and Grp (z0 , z0 ; ω; k) is given by Eq. (P.92). Once G (r0 , r0 ; ω) is determined we known how to compute Eq. (P.1). For having an explicit matrix form for the Green’s functions we need to write the tensor product of the polarization vectors explicitly. This is done in Sec. P.3. Once is possession of these results, we progress by performing the angular integration implicit in d2 k, obtaining Z Z 100 rs iei2z0 kz1 d2 k r (P.44) dkρ kρ 0 1 0 , 2 Gs (z0 , z0 ; ω; k) = 4π 2kz1 (2π) 000 and Z Z fρ 0 0 2 i2kz1 z0 rp d k r ie 0 fρ 0 , (P.45) dkρ kρ 2 Gp (z0 , z0 ; ω; k) = 4π 2kz1 (2π) 0 0 2fz1 where kρ2 kρ2 =1+ 2 , fρ = −1 + (P.46) 2 (n1 ω/c) k1 2 2 kz1 kz1 fz1 = 1 − = 1 − , (P.47) (n1 ω/c)2 k12 √ where n1 = 1 is the refractive index of medium 1. Using the these results for determining G (r0 , r0 ; ω) and replacing it in Eq. P.1 we obtain !# " Z ∞ µ2x + µ2y kρ2 γ 3c iei2kz1 z0 = 1+ √ =m dkρ kρ rs + rp −1 + 2 2 γ01 2 µ1 1 ω µ (n1 ω/c) 2kz1 0 Z ∞ 2 3c 2µ2z kz1 iei2kz1 z0 + √ =m dkρ kρ rp 1 − , (P.48) 2 2 2 µ1 1 ω µ (n1 ω/c) 2kz1 0 where γ = 1/τ and γ01 is the dipole decaying rate if the whole space was embedded with the dielectric medium 1, which reads √ √ ω 3 µ2 µ1 1 2ω 2 µ1 µ0 µ1 1 ω 2 γ01 = µ = µ1 µ0 . (P.49) ~ 6πc 3π~ c

April 8, 2016

11:53

An Introduction to Graphene Plasmonics

392

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

√ Now we define k1 √ = µ1 1 ω/c, and perform a change of coordinates kρ = k1 s, and kz1 = k1 1 − s2 + i0+ , thus obtaining Z ∞ i2k1 z0 √1−s2 s γ 3 µ2x + µ2y 2 √ =m ds = 1+ r −1 + s ie p γ01 4 µ2 1 − s2 0 Z ∞ √ 3 µ2x + µ2y s i2k1 z0 1−s2 √ + =m ds r ie s 4 µ2 1 − s2 0 Z ∞ 3 2 √ 3µ s 2 + z2 =m ds √ rp iei2kz1 z0 1−s , 2 2µ 1−s 0 (P.50) a result that agrees with Eq. (10.38). P.3

Explicit Form of the Tensor Product of the Polarization Vectors

For converting the Green’s functions, written in terms of a tensor product of the polarization vectors, in a matrix form, we need to make the tensor product explicit. This is done below. We recall that the polarization vectors are given by Eqs. (P.9) and (P.10). Then we have ky2 −kx ky 0 1 ± −kx ky kx2 0 , (P.51) e± s,n ⊗ es,n = 2 k 0 0 0 2 2 2 2 /k 2 −kx kz1 kx kz1 /k kx ky kz1 1 + 2 2 e+ (P.52) /k 2 −ky kz1 , kx ky kz1 /k 2 ky2 kz1 p,1 ⊗ ep,1 = 2 k1 −kx kz1 −ky kz1 k2 2 2 2 2 /k 2 kx kz1 kx kz1 /k kx ky kz1 1 − 2 2 e− (P.53) kx ky kz1 /k 2 ky2 kz1 /k 2 ky kz1 , p,1 ⊗ ep,1 = 2 k1 2 kx kz1 ky kz1 k 2 2 /k 2 −kx ky kz1 /k 2 −kx kz1 −kx2 kz1 1 − 2 2 (P.54) e+ −kx ky kz1 /k 2 −ky2 kz1 /k 2 −ky kz1 , p,1 ⊗ ep,1 = 2 k1 2 kx kz1 ky kz1 k and kx2 kz1 kz2 /k 2 kx ky kz1 kz2 /k 2 kx kz2 1 = kx ky kz1 kz2 /k 2 ky2 kz1 kz2 /k 2 ky kz2 . k1 k2 kx kz1 ky kz1 k2

− e− p,2 ⊗ ep,1

(P.55)

page 392

April 8, 2016

11:53

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Derivation of the Transition Rate of a Quantum Emitter Near an Interface

393

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

The expressions given above enter the Green’s functions of the flat interface problem. Other combinations of the tensor product of the polarization vectors can be computed in similar form. P.4

The Free Green’s Function in Real Space

Using Eq. (P.19), the Green’s function in real space is obtained from (note that in this section k is a 3D vector) Z c2 1 dωd3 k Gij (r, t) = δij − 2 2 ki kj 2 eik·r e−iωt (P.56) (2π)4 n ω k − n2 ω 2 /c2 Z dωd3 k c2 1 = δij + 2 2 ∂i ∂j 2 eik·r e−iωt (P.57) (2π)4 n ω k − n2 ω 2 /c2 √ where n = is the refractive index of the medium where the dipole is embedded. Making a Fourier transform back to real space, we obtain Z 1 d3 k ik·r 3 k 2 − n2 ω 2 /c2 e (2π) Z π Z ∞ 1 k 2 eikr cos θ dθ sin θ = dk 4π 2 0 (k − nω/c − i0+ ) (k + nω/c + i0+ ) 0 Z ∞ 1 dk keikr = 2πr −∞ 2πi (k − nω/c − i0+ ) (k + nω/c + i0+ ) einωr/c . (P.58) 4πr Where the prescription ω → ω + i0+ is imposed because we are interested in a retarded response function. Therefore, we obtain =

F IF FF Gij (r, ω) = GN ij (r, ω) + Gij (r, ω) + Gij (r, ω)

(P.59)

with einωr/c c2 h xi xj i δij − 3 2 , (P.60) 3 2 2 4πr n ω r xi xj i einωr/c c h δ − 3 GIF (r, ω) = i , (P.61) ij ij 4πr2 nω r2 einωr/c h xi xj i F GF δij − 2 . (P.62) ij (r, ω) = 4πr r Note that r should be interpreted as |r − r0 |. From these, the contribution to the total decaying rate coming from G0 (r0 , r0 ; ω), and leading to the free space decaying rate, can be computed. Some care must be exercised since there are cancelling divergences when r → r0 . With this section, we have all we need to compute the Purcell factor. F GN ij (r, ω) = −

page 393

April 5, 2016

14:13

394

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

P.5

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Green’s Function for Problems With Flat Interfaces II

For the sake of completeness, here we re-derive the same results obtained above using a more traditional approach [Novotny and Hecht (2014)], where everything is expressed in terms matrix Green’s functions right from the start, with no reference to polarization vectors (see also [Johansson (2011)]). P.5.1

The free space Green’s function revisited

Combing Eqs. (P.23) and (P.24) it is possible to write the free space Green’s function as a 3×3 matrix. It will also be useful to split the free Green’s function in s− and p−components. Let us choose k = (kx , ky ) = (0, kρ ), we then obtain the matrix Green’s function (or dyadic Green’s function) 1 0 0 ik |z| kρ2 i kρ kz z 0 1 − n2 ω2 /c2 ∓ n2 ω2 /c2 G(ω, ky = kρ , z) = , (P.63) e 2kz kz2 kρ kz 0 ∓ n2 ω2 /c2 1 − n2 ω2 /c2 √ where the − sign is for z > 0, while the + sign is for z < 0, where n = is the refractive index of the medium where the dipole is embedded. We now split the Green’s function in s− and p−components, such that Gij (ω, ky = kρ , z) = Gsij (ω, ky = kρ , z) + Gpij (ω, ky = kρ , z), (P.64) where (specializing in the z > 0 case) ikz |z| 1 0 0 ie 0 0 0 Gs (ω, ky = kρ , z) = (P.65) 2kz 000 0 0 0 ikz |z| ie k2 k k (P.66) Gp (ω, ky = kρ , z) = 0 1 − n2 ωρ 2 − nρ2 ωz2 . 2kz kz2 kρ kz 0 − n2 ω2 1 − n2 ω2 We can recover the the Green’s function for general (kx , ky ) by applying the rotation matrix sin θ cos θ 0 R = − cos θ sin θ 0 , (P.67) 0 0 1 such that R · (0, kρ ) = kρ (cos θ, sin θ). We have (omitting the exponential pre-factors in the rotation of the matrices, but reintroducing them in the final expression): 2 100 ky −kx ky 0 ikz |z| ie −kx ky kx2 0 , Gs (ω, k, z) = R · 0 0 0 · Rt = (P.68) 2kz kρ2 000 0 0 0

page 394

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Derivation of the Transition Rate of a Quantum Emitter Near an Interface

395

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

and 0 0 0 kρ2 kρ kz · Rt Gp (ω, k, z) = R · 2 0 1 − n2 ω2 /c2 − n2 ω2 /c 2 k k kz 1 − n2 ω2z/c2 0 − n2 ωρ2 /c 2 2 kρ2 kρ2 kx kx ky kx kz 1 − 1 − − 2 kρ2 (nω/c)2 (nω/c)2 (nω/c)2 kρ2 ieikz |z| kx ky kρ2 kρ2 kx ky kz = (P.69) . 1 − (nω/c)2 − (nω/c) 2 kρ2 1 − (nω/c)2 2kz kρ2 kz2 ky kz kx kz − (nω/c)2 − (nω/c)2 1 − (nω/c)2 P.5.2

Electric field from a dipole in terms of Green’s functions

We want to determine the form of the electromagnetic field generated by a dipole (at position z = z0 ) close to an interface (at position z = 0). Following Eq. (P.28), we write the electric field as [cf. Eqs. (O.51)- (O.53)] EI (z0 < z) = (iωµ1 µ0 ) Gi> (z, z0 ; ω; k) + Gr (z, z0 ; ω; k)] · j EII (0 < z < z0 ) = (iωµ1 µ0 ) Gi< (z, z0 ; ω; k) III

E

+ Gr (z, z0 ; ω; k)] · j (z < 0) = (iωµ1 µ0 ) Gt (z, z0 ; ω; k) · j

(P.70) (P.71) (P.72)

where j = −iωd is the current density in frequency space generated by the dipole (recall Sec. P.1.2). The reason for the preceding expressions for the fields can be intuitively obtained from Fig. P.2. For example, EI (z0 < z)

Figure P.2: Three regions of the scattering problem (I, II, and III) and corresponding Green’s functions: Gt and Gr are the transmitted and reflected Green’s functions, respectively, G< is the contribution that propagates downwards from the dipole (represented by an arrow), and G> is the contribution that propagates upwards, from the same source. The dipole is located at z = z0 .

page 395

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

396

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

refer to the field above the dipole. Then, it is composed from the contribution of the Green’s function that propagates in the forward direction, Gi> (z, z0 ; ω; k), plus the Green’s functions that has been reflected at the interface, Gr (z, z0 ; ω; k). The same reasoning applies to the other spatial regions. We recall that the Green’s function is the response to a point-like source. As such, it can be loosely understood as a field. This allows to write the Green’s functions entering in the three previous equations as follows: P.5.3

Green’s functions: s−component

For the s−component, the three previous equations translate into: r EIs (z0 < z) = (iωµ1 µ0 ) Gi> s (z, z0 ; ω; k) + Gs (z, z0 ; ω; k) · j , i< r EII s (0 < z < z0 ) = (iωµ1 µ0 ) Gs (z, z0 ; ω; k) + Gs (z, z0 ; ω; k) · j , t EIII s (z < 0) = (iωµ1 µ0 ) Gs (z, z0 ; ω; k) · j .

(P.73) (P.74) (P.75)

The s−component of the free Green’s function is given by [remember that k = (0, ky ) = (0, kρ )] ikz1 |z| 1 0 0 ie 0 0 0 . (P.76) G0s (z; ω; kρ ) = 2kz1 000 From Eq. (P.76) we can easily write the different Green’s functions appearing in Eqs. (P.73), (P.74), and (P.75) as 100 i 0 0 0 eikz1 (z−z0 ) , Gi> (P.77) s (z, z0 ; ω; kρ ) = 2kz1 000 10 i Gi< (z, z ; ω; k ) = 00 0 ρ s 2kz1 00

0 0 e−ikz1 (z−z0 ) , 0

10 i 0 0 Grs (z, z0 ; ω; kρ ) = rs 2kz1 00 10 i t Gs (z, z0 ; ω; kρ ) = tp 00 2kz1 00

(P.78)

0 0 eikz1 (z+z0 ) , 0

(P.79)

0 0 e−ikz2 z eikz1 z0 . 0

(P.80)

page 396

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Derivation of the Transition Rate of a Quantum Emitter Near an Interface

397

The origin of the phase in the exponentials of the Green’s functions can be understood as follows. Take, for example, the Green’s function (P.77): since z > z0 , the propagation from z0 to z picks up a phase kz1 (z − z0 ). By the same reasoning, the phase pick up by the Green’s function (P.80) is kz1 z0 + kz2 |z| = kz1 z0 − kz2 z, since z < 0. The simplicity of the matrix structure is a consequence of the polarization of the field, which is transverse, being in the graphene plane. To obtain the Green’s function for general k = (kx , ky ) we just need to apply the rotation matrix

sin θ cos θ 0 R = − cos θ sin θ 0 , 0 0 1

(P.81)

and we obtain: ky2 −kx ky i> Gs (z, z0 ; ω; k) = −kx ky kx2 2kz1 kρ2 0 0

0 0 eikz1 (z−z0 ) , 0

(P.82)

0 0 e−ikz1 (z−z0 ) , 0

(P.83)

ky2 −kx ky 0 i −kx ky kx2 0 eikz1 (z+z0 ) , Grs (z, z0 ; ω; k) = rs 2kz1 kρ2 0 0 0

(P.84)

i

ky2 −kx ky i< Gs (z, z0 ; ω; k) = −kx ky kx2 2kz1 kρ2 0 0

i

ky2 −kx ky t Gs (z, z0 ; ω; k) = ts −kx ky kx2 2kz1 kρ2 0 0

i

where kρ =

q

0 0 e−ikz2 z eikz1 z0 , 0

(P.85)

kx2 + ky2 . Notice how the boundary conditions at z = z0 and

z = 0 are satisfied by the Green’s functions. At z = z0 , Gr (z, z0 ; ω; k) and its derivatives are continuous, while the Green’s functions Gi≶ (z, z0 ; ω; k) satisfies the boundary conditions imposed by the current at z = z0 . At z = 0, we have the Fresnel coefficients rs and ts that enforce the boundary conditions due to the change of medium.

page 397

April 5, 2016

14:13

398

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

P.5.4

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

An Introduction to Graphene Plasmonics

Green’s functions: p−component

As for the p−component, we can write the electric field in the whole space as r EIp (z0 < z) = (iωµ1 µ0 ) Gi> j, p (z, z0 ; ω; k) + Gp (z, z0 ; ω; k) · (P.86) i< II r Ep (0 < z < z0 ) = (iωµ1 µ0 ) Gp (z, z0 ; ω; k) + Gp (z, z0 ; ω; k) · (P.87) j, t III Ep (z < 0) = (iωµ1 µ0 ) Gp (z, z0 ; ω; k) · j . (P.88) The p−component of the free space Green’s function is given by [k = (0, kρ )] 0 0 ikz |z−z0 | 0 ie 2 0 G0p (z, z0 ; ω; kρ ) = kz1 − sgn(z − z0 )kρ kz1 . 2kz k12 0 − sgn(z − z0 )kρ kz1 kρ2 (P.89) Contrary to the s−polarization, it is not immediately obvious how to write from G0p the different Green’s functions. This happens because the polarization vectors are not contained in the graphene plane. For k = (0, ky ) = (0, kρ ) the results are (See Sec. P.5.5) 0 0 0 i 2 0 kz1 Gi> (P.90) −kρ kz1 eikz1 (z−z0 ) , p (z, z0 ; ω; kρ ) = 2kz1 k12 0 −kρ kz1 kρ2 0 0 0 2 0 kz1 Gi< kρ kz1 e−ikz1 (z−z0 ) , p (z, z0 ; ω; kρ ) = 2kz1 k12 0 kρ kz1 kρ2

(P.91)

0 0 0 2 0 −kz1 Grp (z, z0 ; ω; kρ ) = rp −kρ kz1 eikz1 (z+z0 ) , 2kz1 k12 0 kρ kz1 kρ2

(P.92)

0 0 0 i 0 kz1 kz2 kρ kz2 e−ikz2 z+ikz1 z0 . Gtp (z, z0 ; ω; kρ ) = tp 2kz1 k1 k2 0 kρ kz1 kρ2

(P.93)

i

i

To obtain the Green’s function for general k = (kx , ky ) we just need to apply the rotation matrix Eq. (P.81). We obtain (note that upon rotation the length of kρ does not change) 2 2 2 2 kx kz1 /kρ kx ky kz1 /kρ2 −kx kz1 i 2 2 kx ky kz1 Gi> /kρ2 −ky kz1 eikz1 (z−z0 ) , /kρ2 ky2 kz1 p (z, z0 ; ω; k) = 2kz1 k12 −kx kz1 −ky kz1 kρ2 (P.94)

page 398

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Derivation of the Transition Rate of a Quantum Emitter Near an Interface

399

2 2 kx2 kz1 /kρ2 kx ky kz1 /kρ2 kx kz1 i 2 2 kx ky kz1 Gi< /kρ2 ky2 kz1 /kρ2 ky kz1 e−ikz1 (z−z0 ) , p (z, z0 ; ω; k) = 2kz1 k12 kx kz1 ky kz1 kρ2 (P.95) 2 2 −kx2 kz1 /kρ2 −kx ky kz1 /kρ2 −kx kz1 i r 2 2 2 2 −kx ky kz1 /kρ −ky kz1 /kρ2 −ky kz1 Gp (z, z0 ; ω; k) = rp 2kz1 k12 kx kz1 ky kz1 kρ2

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

×eikz1 (z+z0 ) , (P.96) 2 2 2 kx kz1 kz2 /kρ kx ky kz1 kz2 /kρ kx kz2 i kx ky kz1 kz2 /kρ2 ky2 kz1 kz2 /kρ2 ky kz2 Gtp (z, z0 ; ω; k) = tp 2kz1 k1 k2 kx kz1 ky kz1 kρ2 ×e−ikz2 z+ikz1 z0 . P.5.5

(P.97)

Derivation of the matrix structure of the Green’s functions for the p−polarization component in the interface problem

For convenience we rewrite here the p−component of the free Green’s function: G0p (z; z0 ; ω; ky = kρ ) 0 0 0 ieikz1 |z−z0 | 2 = 0 kz1 − sgn(z − z0 )kρ kz1 . 2kz1 k12 0 − sgn(z − z0 )kρ kz1 kρ2

(P.98)

If follows that the Green’s functions that emanate from z0 are simply given by 0 0 ikz1 (z−z0 ) 0 ie 2 0 kz1 Gi> (P.99) −kρ kz1 , p (z; z0 ; ω; ky = kρ ) = 2kz1 k12 0 −kρ kz1 kρ2 and 0 0 ikz1 (z0 −z) 0 ie 2 0 kz1 Gi< kρ kz1 . p (z; z0 ; ω; ky = kρ ) = 2kz1 k12 0 kρ kz1 kρ2

(P.100)

It is the latter Green’s function that gives rise to the reflected and transmitted Green’s functions. To derive the reflected and transmitted Green’s functions one route is to start by writing the electric field in the three

page 399

April 5, 2016

14:13

400

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

regions (see Fig. N.2) as

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

0

EIp (z0 < z) = Epi> eikz1 z −kz1 /k1 kρ /k1 0 i< ikz1 z + rp Ep e −kz1 /k1 kρ /k1 0 i< −ikz1 z EII kz1 /k1 p (0 < z < z0 ) = Ep e

(P.101)

kρ /k1

0

+ rp Epi< eikz1 z −kz1 /k1 kρ /k1 0 i< −ikz2 z EIII kz2 /k2 p (z < 0) = tp Es e kρ /k2

(P.102)

(P.103)

where Epi< is the amplitude of the primary field at z = z0 . We can connect the Green’s function Gi< p (z; z0 ; ω; ky ) with 0 Epi< e−ikz1 z kz1 /k1 (P.104) kρ /k1 using Eq. (P.28). Clearly we must have 0 Epi< kz1 /k1 = µµ0 ω 2 eikz1 z0 Gi< (P.105) p (z0 ; z0 ; ω; ky ) · d . kρ /k1 This allow us to write the reflected Green’s function as follows 1 0 0 0 0 rp Epi< eikz1 z −kz1 /k1 = rp Epi< eikz1 z 0 −1 0 kz1 /k1 = kρ /k1 0 0 1 kρ /k1 0 0 0 µµ0 ω 2 rp eikz1 (z+z0 ) 0 −1 0 Gi< (P.106) p (z0 ; z0 ; ω; ky ) · d , 0 0 1 which implies that 0 0 0 Grp (z; z0 ; ω; ky ) = rp eikz1 (z+z0 ) 0 −1 0 Gi< p (z0 ; z0 ; ω; ky ) , (P.107) 0 0 1

page 400

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Derivation of the Transition Rate of a Quantum Emitter Near an Interface

401

which upon matrix multiplication yields Eq. (P.92) The transmitted Green’s function is built is a similar manner. First we write 0 0 0 0 0 k1 tp Esi< e−ikz2 z kz2 /k2 = tp Esi< e−ikz2 z 0 kz2 /kz1 0 kz1 /k1 k2 kρ /k1 0 0 1 kρ /k2 0 0 0 k1 = µµ0 ω 2 eikz1 z0 tp e−ikz2 z 0 kz2 /kz1 0 Gi< p (z0 ; z0 ; ω; ky ) · d . (P.108) k2 0 0 1 From the latter result it follows 0 0 k 1 Gtp (z; z0 ; ω; ky ) = eikz1 z0 tp e−ikz2 z 0 kz2 /kz1 k2 0 0

0 0 Gi< p (z0 ; z0 ; ω; ky ) , 1 (P.109) which upon matrix multiplication yields Eq. (P.93). The same technique could have been used to construct the s−polarized Green’s function, although in this case this is not strictly necessary.

page 401

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

May 2, 2013 14:6 BC: 8831 - Probability and Statistical Theory

This page intentionally left blank

PST˙ws

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Bibliography

Abedinpour, S. H., Vignale, G., Principi, A., Polini, M., Tse, W.-K., and MacDonald, A. H. (2011). Drude weight, plasmon dispersion, and ac conductivity in doped graphene sheets, Phys. Rev. B 84, p. 045429. Abergel, D., Apalkov, V., Berashevich, J., Ziegler, K., and Chakrabort, T. (2010). Properties of graphene: a theoretical perspective, Advances in Physics 59, pp. 261–482. Ablowitz, M. J. and Fokas, A. S. (1997). Complex Variables (Cambridge University Press, New York). Abramowitz, M. and Stegun, I. A. (1965). Handbook of Mathematical Functions: with Formulas, Graphs, and Mathematical Tables (Dover, New York). Aćimović, S. S., Ortega, M. A., Sanz, V., Berthelot, J., Garcia-Cordero, J. L., Renger, J., Maerkl, S. J., Kreuzer, M. P., and Quidant, R. (2014). Lspr chip for parallel, rapid, and sensitive detection of cancer markers in serum, Nano Lett. 14, pp. 2636–2641. Alonso-González, P., Nikitin, A. Y., Golmar, F., Centeno, A., Pesquera, A., Vélez, S., Chen, J., Navickaite, G., Koppens, F., Zurutuza, A., Casanova, F., Hueso, L. E., and Hillenbrand, R. (2014). Controlling graphene plasmons with resonant metal antennas and spatial conductivity patterns, Science 344. Amorim, B., Schiefele, J., Sols, F., and Guinea, F. (2012). Coulomb drag in graphene/boron nitride heterostructures: Effect of virtual phonon exchange, Phys. Rev. B 86, p. 125448. Anker, J. N., Hall, W. P., Lyandres, O., Shah, N. C., Zhao, J., and Duyn, R. P. V. (2008). Biosensing with plasmonic nanosensors, Nature Materials 7, pp. 442 – 453. Archambault, A., Teperik, T. V., Marquier, F., and Greffet, J. J. (2009). Surface plasmon fourier optics, Phys. Rev. B 79, p. 195414. Arfken, G. B., Weber, H. J., and Harris, F. E. (2012). Mathematical Methods for Physicists, 7th edn. (Academic Press). Armstrong, S. (2012). Plasmonics: Diffraction-free surface waves, Nature Photonics 6, p. 720. Ashcroft, N. W. and Mermin, N. D. (1976). Solid State Physics, 1st edn. (Saunders 403

page 403

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

404

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

College, New York). Atwater, H. A. (2007). The promise of plasmonics, Scientific American 4, pp. 1–5. Aversa, C. and Sipe, J. E. (1995). Nonlinear optical susceptibilities of semiconductors: Results with a length-gauge analysis, Phys. Rev. B 52, pp. 14636– 14645. Balandin, A. A., Ghosh, S., Bao, W., Calizo, I., Teweldebrhan, D., Miao, F., and Lau, C. N. (2008). Superior thermal conductivity of single-layer graphene, Nano Lett. 8, pp. 902–907. Bao, Q., Zhang, H., Wang, B., Ni, Z., Lim, C. H. Y. X., Wang, Y., Tang, D. Y., and Loh, K. P. (2011). Broadband graphene polarizer, Nature Photonics 5, pp. 411–415. Barnes, W. L. (2006). Surface plasmon-polariton length scales: a route to subwavelength optics, J. Opt. A: Pure Appl. Opt. 8, p. S87. Barnes, W. L., Dereux, A., and Ebbesen, T. W. (2003). Surface plasmon subwavelength optics, Nature 424, pp. 824–830. Baskin, I., Ashkinadze, B. M., Cohen, E., and Pfeiffer, L. N. (2011). Imaging of magnetoplasmons excited in a two-dimensional electron gas, Phys. Rev. B 84, p. 041305. Bass, F. G. and Yakovenko, V. M. (1965). Theory of radiation from a charge passing through an electrically inhomogeneous medium, Sov. Phys. Usp. 8, p. 420. Beletskii, N. N. and Bludov, Y. V. (2005). Edge magnetoplasmons in a finite array of two-dimensional electron gas strips, Telecommunications and Radio Engineering 63, pp. 405–417. Berini, P. and Leon, I. D. (2012). Surface plasmon-polariton amplifiers and lasers, Nature Photonics 6, pp. 16–24. Biehs, S.-A. and Agarwal, G. S. (2013). Large enhancement of förster resonance energy transfer on graphene platforms, ppl. Phys. Lett. 103, p. 243112. Billings, L. (2013). Exotic optics: Metamaterial world, Nature 500, pp. 138–140. Blount, E. I. (1962). Formalisms of band theory, in F. Seitz and D. Turnbull (eds.), Solid state physics, Vol. 13 (Academic Press), pp. 839–839. Bludov, Y. V., Ferreira, A., Peres, N. M. R., and Vasilevskiy, M. I. (2013). A primer on surface plasmon-polaritons in graphene, Int. J. Mod. Phys. B 27, p. 1341001. Bludov, Y. V., Peres, N. M. R., and Vasilevskiy, M. I. (2012a). Graphene-based polaritonic crystal, Phys. Rev. B 85, p. 245409. Bludov, Y. V., Smirnova, D. A., Kivshar, Y. S., Peres, N. M. R., and Vasilevskiy, M. I. (2014). Nonlinear te-polarized surface polaritons on graphene, Phys. Rev. B 89, p. 035406. Bludov, Y. V., Vasilevskiy, M. I., and Peres, N. M. R. (2010). Mechanism for graphene-based optoelectronic switches by tuning surface plasmonpolaritons in monolayer graphene, EPL 92, p. 68001. Bludov, Y. V., Vasilevskiy, M. I., and Peres, N. M. R. (2012b). Tunable graphenebased polarizer, Journal of Appl. Phys. 112, 8, p. 084320. Bolotin, K., Sikes, K., Jiang, Z., Klima, M., Fudenberg, G., Hone, J., Kim, P.,

page 404

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Bibliography

9in x 6in

b2445-mas

405

and Stormer, H. (2008). Ultrahigh electron mobility in suspended graphene, Solid State Communications 146, pp. 51–355. Boriskina, S. V., Ghasemi, H., and Chen, G. (2013). Plasmonic materials for energy: From physics to applications, Materials Today 16, pp. 375–386. Bracewell, R. N. (1999). The Fourier Transform & Its Applications, 3rd edn. (McGraw-Hill, New York). Brar, V. W., Jang, M. S., Sherrott, M., Kim, S., Lopez, J. J., Kim, L. B., Choi, M., and Atwater, H. (2014). Hybrid surface-phonon-plasmon polariton modes in graphene/monolayer h-bn heterostructures, Nano Lett. 14, pp. 3876–3880. Brar, V. W., Jang, M. S., Sherrott, M., Lopez, J. J., and Atwater, H. A. (2013). Highly confined tunable mid-infrared plasmonics in graphene nanoresonators, Nano Lett. 13, pp. 2541–2547. Brolo, A. G. (2012). Plasmonics for future biosensors, Nature Photonics 6, pp. 709–713. Cai, X., Sushkov, A. B., Jadidi, M. M., Nyakiti, L. O., Myers-Ward, R. L., Gaskill, D. K., Murphy, T. E., Fuhrer, M. S., and Drew, H. D. (2015). Plasmon-enhanced terahertz photodetection in graphene, Nano Lett. 15, pp. 4295–4302. Cai, Y.-J., Li, M., Ren, X.-F., Zou, C.-L., Xiong, X., Lei, H.-L., Liu, B.-H., Guo, G.-P., and Guo, G.-C. (2014). High-visibility on-chip quantum interference of single surface plasmons, Phys. Rev. Appl. 2, p. 014004. Caldwell, J. D., Kretinin, A. V., Chen, Y., Giannini, V., Fogler, M. M., Francescato, Y., Ellis, C. T., Tischler, J. G., Woods, C. R., Giles, A. J., Hong, M., Watanabe, K., Taniguchi, T., Maier, S. A., and Novoselov, K. S. (2014). Sub-diffractional volume-confined polaritons in the natural hyperbolic material hexagonal boron nitride, Nature Communications 5, pp. 1–9. Carbotte, J. P., LeBlanc, J. P. F., and Nicol, E. J. (2012). Emergence of plasmaronic structure in the near-field optical response of graphene, Phys. Rev. B 85, p. 201411(R). Castro Neto, A. H., Guinea, F., Peres, N. M. R., Novoselov, K. S., and Geim, A. K. (2009). The electronic properties of graphene, Rev. Mod. Phys. 81. Castro Neto, A. H. and Novoselov, K. (2011). New directions in science and technology: two-dimensional crystals, Reports on Progress in Physics 74, p. 082501. Chaikin, P. M. and Lubensky, T. C. (2000). Principles of Condensed Matter Physics (Cambridge University Press, Cambridge). Chang, D. E., Sørensen, A. S., Hemmer, P. R., and Lukin, M. D. (2006). Quantum optics with surface plasmons, Phys. Rev. Lett. 97, p. 053002. Chaves, F. A., Jiménez, D., Cummings, A. W., and Roche, S. (2014). Physical model of the contact resistivity of metal-graphene junctions, Journal of Appl. Phys. 115, p. 164513. Chen, J., Badioli, M., Alonso-González, P., Thongrattanasiri, S., Huth, F., Osmond, J., Spasenović, M., Centeno, A., Pesquera, A., Godignon, P., Elorza, A. Z., Camara, N., de Abajo, F. J. G., Hillenbrand, R., and Koppens, F. H. L. (2012). Optical nano-imaging of gate-tunable graphene plasmons, Nature 487, pp. 77–81.

page 405

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

406

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Chen, P.-Y. and Alù, A. (2011). Atomically thin surface cloak using graphene monolayers, ACS Nano 5, pp. 5855 – 5863. Chen, Z., Berciaud, S., Nuckolls, C., Heinz, T. F., and Brus, L. E. (2010). Energy transfer from individual semiconductor nanocrystals to graphene, ACS Nano 4, pp. 2964–2968. Cheng, H., Chen, S., Yu, P., Duan, X., Xie, B., and Tian, J. (2013). Dynamically tunable plasmonically induced transparency in periodically patterned graphene nanostrips, Appl. Phys. Lett. 103, p. 203112. Cheng, J., Wang, W. L., Mosallaei, H., and Kaxiras, E. (2014). Surface plasmon engineering in graphene functionalized with organic molecules: A multiscale theoretical investigation, Nano Lett. 14, pp. 50 – 56. Chiu, K. W. and Quinn, J. J. (1974). Plasma oscillations of a two-dimensional electron gas in a strong magnetic field, Phys. Rev. B 9, pp. 4724–4732. Christensen, J., Manjavacas, A., Thongrattanasiri, S., Koppens, F. H. L., and de Abajo, F. J. G. (2012). Graphene plasmon waveguiding and hybridization in individual and paired nanoribbons, ACS Nano 6, 1, pp. 431–440. Christensen, T., Jauho, A.-P., Wubs, M., and Mortensen, N. A. (2015a). Localized plasmons in graphene-coated nanospheres, Phys. Rev. B 91, p. 125414. Christensen, T., Wang, W., Jauho, A.-P., Wubs, M., and Mortensen, N. A. (2014). Classical and quantum plasmonics in graphene nanodisks: the role of edge states, Phys. Rev. B 90, p. 241414(R). Christensen, T., Yan, W., Jauho, A.-P., Wubs, M., and Mortensen, N. A. (2015b). Kerr nonlinearity and plasmonic bistability in graphene nanoribbons, Phys. Rev. B 92, 121407(R). Constant, T. J., Hornett, S. M., Chang, D. E., and Hendry, E. (2015). All-optical generation of surface plasmons in graphene, Nat. Phys. 11, p. 1. Cox, J. D. and de Abajo, F. J. G. (2014). Electrically tunable nonlinear plasmonics in graphene nanoislands, Nature Communications 5, 5725. Cox, J. D. and de Abajo, F. J. G. (2015). Plasmon-enhanced nonlinear wave mixing in nanostructured graphene, ACS Photonics 2, pp. 306–312. Cox, J. D., Singh, M. R., Gumbs, G., Anton, M. A., and Carreno, F. (2012). Dipole-dipole interaction between a quantum dot and a graphene nanodisk, Phys. Rev. B 86, p. 125452. Crassee, I., Orlita, M., Potemski, M., Walter, A. L., Ostler, M., Seyller, T., Gaponenko, I., Chen, J., and Kuzmenko, A. B. (2012). Intrinsic terahertz plasmons and magnetoplasmons in large scale monolayer graphene, Nano Lett. 12, pp. 2470–2474. Crozier, K. B., Zhu, W., Wang, D., Lin, S., Best, M. D., and Camden, J. P. (2014). Plasmonics for surface enhanced raman scattering: Nanoantennas for single molecules, IEEE Journal of Selected Topics in Quantum Electronics 20. Dai, S., Fei, Z., Ma, Q., Rodin, A. S., Wagner, M., McLeod, A. S., Liu, M. K., Gannett, W., Regan, W., Watanabe, K., Taniguchi, T., Thiemens, M., Dominguez, G., Castro Neto, A. H., Zettl, A., Keilmann, F., Jarillo-Herrero, P., Fogler, M. M., and Basov, D. N. (2014). Tunable phonon polaritons in atomically thin van der waals crystals of boron nitride, Science 343, pp. 1125–1129.

page 406

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Bibliography

9in x 6in

b2445-mas

407

Dai, S., Ma, Q., Zhu, S.-E., Liu, M. K., Andersen, T., Fei, Z., Goldflam, M., Wagner, M., Watanabe, K., Taniguchi, T., Thiemens, M., Keilmann, F., Janssen, G. C. A. M., Jarillo-Herrero, P., Fogler, M. M., and Basov, D. N. (2015). Graphene on hexagonal boron nitride as an agile hyperbolic metamaterial, Nature Nanotechnology 10, pp. 682–686. Danos, M. (1955). Čerenkov radiation from extended electron beams, J. Appl. Phys. 26, p. 2. Das, A. K. (1974). The linear response of a one-dimensional electron gas, Solid State Communications 15, pp. 475–477. Das, A. K. (1975). The relaxation-time approximation in the rpa dielectric formulation, J. Phys. F: Met. Phys. 5, p. 2035. de Abajo, F. J. G. (2014). Graphene plasmonics: Challenges and opportunities, ACS Photonics 1, 135-152. Di Martino, G., Sonnefraud, Y., Tame, M. S., Kéna-Cohen, S., Dieleman, F., Ozdemir, S. K., Kim, M. S., and Maier, S. A. (2014). Observation of quantum interference in the plasmonic hong-ou-mandel effect, Phys. Rev. Appl. 1, p. 034004. Dionne, J. A. and Atwater, H. A. (2012). Plasmonics: Metal-worthy methods and materials in nanophotonics, MRS Bulletin 37, pp. 717–724. Dionne, J. A., Sweatlock, L. A., Atwater, H. A., and Polman, A. (2005). Planar metal plasmon waveguides: frequency-dependent dispersion, propagation, localization, and loss beyond the free electron model, Phys. Rev. B 72, p. 075405. Dressel, M. and Grüner, G. (2002). Electrodynamics of Solids: Optical Properties of Electrons in Matter, 1st edn. (Cambridge University Press, Cambridge). Drude, P. (1909). Zur elektronentheorie der metalle, Annalen der Physik 306, pp. 566–613. Duffy, D. G. (2015). Green’s Functions with Applications, 2nd edn. (CRC Press, Boca Raton). Ebbesen, T. W., Genet, C., and Bozhevolnyi, S. I. (2008). Surface plasmon circuitry, Nature 61, pp. 44–50. Ebbesen, T. W., Lezec, H. J., Ghaemi, H. F., Thio, T., and Wolff, P. A. (1998). Extraordinary optical transmission through sub-wavelength hole arrays, Nature 391, pp. 667–669. Editorial (2012). Surface plasmon resurrection, Nature Photonics 6, p. 707. Ehrenreich, H. and Cohen, M. H. (1959). Self-consistent field approach to the many-electron problem, Phys. Rev. 115, p. 786. Enoch, S. and Bonod, N. (2012). Plasmonics: From Basics to Advanced Topics (Springer Series in Optical Sciences, New York). Fakonas, J. S., Lee, H., Kelaita, Y. A., and Atwater, H. A. (2014). Two-plasmon quantum interference, Nature Photonics 8, pp. 317–320. Falkovsky, L. A. (2008). Optical properties of graphene, Journal of Physics: Conference Series 129, p. 012004. Falkovsky, L. A. and Varlamov, A. A. (2007). Space-time dispersion of graphene conductivity, Eur. Phys. J. B 56, pp. 281–284. Fallahi, A. and Perruisseau-Carrier, J. (2012). Design of tunable biperiodic

page 407

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

408

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

graphene metasurfaces, Phys. Rev. B 86, p. 195408. Fang, Z., Liu, Z., Wang, Y., Ajayan, P. M., Nordlander, P., and Halas, N. J. (2012a). Graphene-antenna sandwich photodetector, Nano Lett. 12, pp. 3808–3813. Fang, Z., Thongrattanasiri, S., Schlather, A., Liu, Z., Ma, L., Wang, Y., Ajayan, P. M., Nordlander, P., Halas, N. J., and de Abajo, F. J. G. (2013). Gated tunability and hybridization of localized plasmons in nanostructured graphene, ACS Nano 7, pp. 2388–2395. Fang, Z., Wang, Y., Liu, Z., Schlather, A., Ajayan, P. M., Koppens, F. H. L., Nordlander, P., and Halas, N. J. (2012b). Plasmon-induced doping of graphene, ACS Nano 6, pp. 10222–10228. Fang, Z., Wang, Y., Schlather, A. E., Liu, Z., Ajayan, P. M., de Abajo, F. J. G., Nordlander, P., Zhu, X., and Halas, N. J. (2014). Active tunable absorption enhancement with graphene nanodisk arrays, Nano Lett. 14, pp. 299–304. Fano, U. (1941). The theory of anomalous diffraction gratings and of quasistationary waves on metallic surfaces (sommerfeld’s waves), J. Opt. Soc. Am. 31, pp. 213–222. Farhat, M., Guenneau, S., and Bağcı, H. (2011). Exciting graphene surface plasmon polaritons through light and sound interplay, Phys. Rev. Lett. 111, p. 237404. Farias, G. A. and Maradudin, A. A. (1983). Surface plasmons on a randomly rough surface, Phys. Rev. B 28, pp. 5675–5687. Fedorych, O. M., Moreau, S., Potemski, M., Studenikin, S. A., Saku, T., and Hirayama, Y. (2009). Microwave magnetoplasmon absorption by a 2deg stripe, Int. J. Mod. Phys. B 23, pp. 2698–2702. Fei, Z., Andreev, G. O., Bao, W., Zhang, L. M., McLeod, A. S., Wang, C., Stewart, M. K., Zhao, Z., Dominguez, G., Thiemens, M., Fogler, M. M., Tauber, M. J., Castro Neto, A. H., Lau, C. N., Keilmann, F., and Basov, D. N. (2011). Infrared nanoscopy of dirac plasmons at the graphene–sio2 interface, Nano Lett. 11, pp. 4701–4705. Fei, Z., Iwinski, E. G., Ni, G. X., Zhang, L. M., Bao, W., Rodin, A. S., Lee, Y., Wagner, M., Liu, M. K., Dai, S., Goldflam, M. D., Thiemens, M., Keilmann, F., Lau, C. N., Castro Neto, A. H., Fogler, M. M., and Basov, D. N. (2015). Tunneling plasmonics in bilayer graphene, Nano Lett. 15, pp. 4973–4978. Fei, Z., Rodin, A. S., Andreev, G. O., Bao, W., McLeod, A. S., Wagner, M., Zhang, L. M., Zhao, Z., Thiemens, M., Dominguez, G., Fogler, M. M., Castro Neto, A. H., Lau, C. N., Keilmann, F., and Basov, D. N. (2012). Gate-tuning of graphene plasmons revealed by infrared nano-imaging, Nature 487, pp. 82–85. Fei, Z., Rodin, A. S., Gannett, W., Dai, S., Regan, W., Wagner, M., Liu, M. K., McLeod, A. S., Dominguez, G., Thiemens, M., Castro Neto, A. H., Keilmann, F., Zettl, A., Hillenbrand, R., Fogler, M. M., and Basov, D. N. (2013). Electronic and plasmonic phenomena at graphene grain boundaries, Nature Nanotechnology 8, pp. 821 –825. Ferreira, A. and Peres, N. M. R. (2012). Complete light absorption in graphenemetamaterial corrugated structures, Phys. Rev. B 86, p. 205401.

page 408

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Bibliography

9in x 6in

b2445-mas

409

Ferreira, A., Peres, N. M. R., and Castro Neto , A. H. (2012). Confined magnetooptical waves in graphene, Phys. Rev. B 85, p. 205426. Ferreira, A., Viana-Gomes, J., Bludov, Y. V., Pereira, V. M., Peres, N. M. R., and Castro Neto, A. H. (2011). Faraday effect in graphene enclosed in an optical cavity and the equation of motion method for the study of magneto-optical transport in solids, Phys. Rev. B 84, p. 235410. Fetter, A. L. (1986). Magnetoplasmons in a two-dimensional electron fluid: Disk geometry, Phys. Rev. B 33, pp. 5221–5227. Fetter, A. L. and Walecka, J. D. (2003). Quantum Theory of Many-Particle Systems (Dover, New York). Fischetti, M. V., Neumayer, D. A., and Cartier, E. A. (2001). Effective electron mobility in si inversion layers in metal–oxide–semiconductor systems with a high-κ insulator: The role of remote phonon scattering, Journal of Appl. Phys. 90, 9, pp. 4587–4608. Flensberg, K., Hu, B. Y.-K., Jauho, A.-P., and Kinaret, J. M. (1995). Linearresponse theory of coulomb drag in coupled electron systems, Phys. Rev. B 52, pp. 14761–14774. Fox, M. (2010). Optical Properties of Solids (Oxford University Press, New York). Fratini, S. and Guinea, F. (2008). Substrate-limited electron dynamics in graphene, Phys. Rev. B 77, p. 195415. Freitag, M., Low, T., Zhu, W., Yan, H., Xia, F., and Avouris, P. (2013). Photocurrent in graphene harnessed by tunable intrinsic plasmons, Nature Communications 4, 1951. Fuchs, R. and Kliewer, K. L. (1965). Optical modes of vibration in an ionic crystal slab, Phys. Rev. 140, pp. A2076–A2088. Gao, W., Shi, G., Jin, Z., Shu, J., Zhang, Q., Vajtai, R., Ajayan, P. M., Kono, J., and Xu, Q. (2013). Excitation and active control of propagating surface plasmon polaritons in graphene, Nano Lett. 13, pp. 3698–3702. Garcia, M. A. (2011). Surface plasmons in metallic nanoparticles: fundamentals and applications, J. Phys. D: Appl. Phys. 44, p. 283001. Garcia de Abajo, F. J. and Manjavacas, A. (2015). Plasmonics in atomically thin materials, Faraday Discuss. 178, pp. 87–107. Gaudreau, L., Tielrooij, K. J., Prawiroatmodjo, G. E. D. K., Osmond, J., de Abajo, F. J. G., and Koppens, F. H. L. (2013). Universal distance-scaling of nonradiative energy transfer to graphene, Nano Lett. 13, pp. 2030–2035. Geim, A. K. (2009). Graphene: Status and prospects, Science 324, pp. 1530– 1534. Geim, A. K. (2012). Graphene prehistory, Physica Scripta 2012, p. 014003. Geim, A. K. and Grigorieva, I. V. (2013). Van der waals heterostructures, Nature 499, pp. 419 – 425. Gilbertson, A. M., Francescato, Y., Roschuk, T., Shautsova, V., Chen, Y., Sidiropoulos, T. P. H., Hong, M., Giannini, V., Maier, S. A., Cohen, L. F., and Oulton, R. F. (2015). Plasmon-induced optical anisotropy in hybrid graphene–metal nanoparticle systems, Nano Lett. 15, pp. 3458–3464. Gómez-Santos, G. and Stauber, T. (2011). Fluorescence quenching in graphene: a fundamental ruler and evidence for transverse plasmons, Phys. Rev. B

page 409

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

410

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

84, p. 165438. Goerbig, M. O. (2011). Electronic properties of graphene in a strong magnetic field, Rev. Mod. Phys. 83, pp. 1193–1243. Goldflam, M. D., Ni, G.-X., Post, K. W., Fei, Z., Yeo, Y., Tan, J. Y., Rodin, A. S., Chapler, B. C., Ozyilmaz, B., Castro Neto, A. H., Fogler, M. M., and Basov, D. N. (2015). Tuning and persistent switching of graphene plasmons on a ferroelectric substrate, Nano Lett. 15, pp. 4859–4864. Gong, S., Hu, M., Zhong, R., Chen, X., Zhang, P., Zhao, T., and Liu, S. (2014). Electron beam excitation of surface plasmon polaritons, Opt. Express 22, pp. 19252–19261. Gorbach, A. V. (2013). Nonlinear graphene plasmonics: Amplitude equation for surface plasmons, Phys. Rev. A 87, p. 013830. Gorbachev, R. V., Geim, A. K., Katsnelson, M. I., Novoselov, K. S., Tudorovskiy, T., Grigorieva, I. V., MacDonald, A. H., Watanabe, K., Taniguchi, T., and Ponomarenko, L. A. (2012). Strong coulomb drag and broken symmetry in double-layer graphene, Nature Phys. 8, pp. 896–901. Green, M. A. and Pillai, S. (2012). Harnessing plasmonics for solar cells, Nature Photonics 6, pp. 130–132. Grigorenko, A. N., Polini, M., and Novoselov, K. S. (2012). Graphene plasmonics, Nature Photonics 6, pp. 749–758. Gu, B., Kwong, N. H., and Binder, R. (2013). Relation between the interband dipole and momentum matrix elements in semiconductors, Phys. Rev. B 87, p. 125301. Gullans, M., Chang, D. E., Koppens, F. H. L., de Abajo, F. J. G., and Lukin, M. D. (2013). Single-photon nonlinear optics with graphene plasmons, Phys. Rev. Lett. 111, p. 247401. Gupta, B. D., Srivastava, S. K., and Verma, R. (2015). Fiber Optic Sensors Based on Plasmonics (World Scientific, Singapore). Gusynin, V. P., Sharapov, S. G., and Carbotte, J. P. (2009). On the universal ac optical background in graphene, New J. Phys. 11, p. 095013. Haes, A. J., Haynes, C. L., McFarland, A. D., Schatz, G. C., Duyne, R. P. V., and Zou, S. (2005). Plasmonic materials for surface-enhanced sensing and spectroscopy, MRS Bulletin 30, pp. 368–375. Hall, E. H. (1879). On a new action of the magnet on electric currents, American Journal of Mathematics 2, pp. 287–292. Hanson, G. W., Hassani Gangaraj, S. A., Lee, C., Angelakis, D. G., and Tame, M. (2015). Quantum plasmonic excitation in graphene and loss-insensitive propagation, Phys. Rev. A 92, p. 013828. Heeg, S., Fernandez-Garcia, R., Oikonomou, A., Schedin, F., Narula, R., Maier, S. A., Vijayaraghavan, A., and Reich, S. (2013). Polarized plasmonic enhancement by au nanostructures probed through raman scattering of suspended graphene, Nano Lett. 13, pp. 301–308. Heeres, R. W., Kouwenhoven, L. P., and Zwiller, V. (2013). Quantum interference in plasmonic circuits, Nature Nanotechnology 8, pp. 719–722. Hessel, A. and Oliner, A. A. (1965). A new theory of wood’s anomalies on optical gratings, Appl. Optics 4, pp. 1275–1297.

page 410

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Bibliography

9in x 6in

b2445-mas

411

Hoggard, A., Wang, L.-Y., Ma, L., Fang, Y., You, G., Olson, J., Liu, Z., Chang, W.-S., Ajayan, P. M., and Link, S. (2013). Using the plasmon linewidth to calculate the time and efficiency of electron transfer between gold nanorods and graphene, ACS Nano 7, pp. 11209–11217. Hopfield, J. J. (1958). Theory of the contribution of excitons to the complex dielectric constant of crystals, Phys. Rev. 112, p. 1555. Huidobro, P. A., Nesterov, M. L., Martín-Moreno, L., and García-Vidal, F. J. (2010). Transformation optics for plasmonics, Nano Lett. 10, pp. 1985– 1990. Huidobro, P. A., Nikitin, A. Y., González-Ballestero, C., Martín-Moreno, L., and García-Vidal, F. J. (2012). Superradiance mediated by graphene surface plasmons, Phys. Rev. B 85, p. 155438. Hwang, E. H. and Sarma, S. D. (2007). Dielectric function, screening, and plasmons in two-dimensional graphene, Phys. Rev. B 75, p. 205418. Hwang, E. H., Sensarma, R., and Sarma, S. D. (2010). Plasmon-phonon coupling in graphene, Phys. Rev. B 82, p. 195406. Ishikawa, A. and Tanaka, T. (2013). Plasmon hybridization in graphene metamaterials, Appl. Phys. Lett. 102, p. 253110. Jablan, M., Buljan, H., and Soljačić, M. (2009). Plasmonics in graphene at infrared frequencies, Phys. Rev. B 80, p. 245435. Jablan, M., Soljačić, M., and Buljan, H. (2013). Plasmons in graphene: Fundamental properties and potential applications, Proc. IEEE 101, pp. 1689 – 1704. Jackson, J. D. (1998). Classical Electrodynamics, 3rd edn. (Wiley, New York). Jacob, Z. (2012). Quantum plasmonics, MRS Bulletin 37, pp. 761–767. Jacob, Z. (2014). Hyperbolic phonon-polaritons, Nature Materials 13, pp. 1081– 1083. Jacob, Z. and Shalaev, V. M. (2011). Plasmonics goes quantum, Science 28, pp. 463–464. Jauho, A. (1998). Quantum transport theory, in E. Schöll (ed.), Theory of Transport Properties of Semiconductor Nanostructures, Electronic Materials Series, Vol. 4 (Springer), pp. 127–171. Jishi, R. A. (2014). Feynman Diagram Techniques in Condensed Matter Physics (Cambridge University Press, Cambridge). Johansson, P. (2011). Electromagnetic green’s function for layered systems: Applications to nanohole interactions in thin metal films, Phys. Rev. B 83, p. 195408. Johnson, P. B. and Christy, R. W. (1972). Optical constants of the noble metals, Phys. Rev. B 6, pp. 4370–4379. Ju, L., Geng, B., Horng, J., Girit, C., Martin, M., Hao, Z., Bechtel, H. A., Liang, X., Zettl, A., Shen, Y. R., and Wang, F. (2011). Graphene plasmonics for tunable terahertz metamaterials, Nature Nanotechnology 6, pp. 630–634. Juan, M. L., Righini, M., and Quidant, R. (2011). Plasmon nano-optical tweezers, Nature Photonics 5, pp. 349–356. Kabashin, A. V., Evans, P., Pastkovsky, S., Hendren, W., Wurtz, G. A., Atkinson, R., Pollard, R., Podolskiy, V. A., and Zayats, A. V. (2009). Plasmonic

page 411

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

412

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

nanorod metamaterials for biosensing, Nature Materials 8, pp. 867 – 871. Kaipa, C. S. R., Yakovlev, A. B., Hanson, G. W., Padooru, Y. R., Medina, F., and Mesa, F. (2012). Enhanced transmission with a graphene-dielectric microstructure at low-terahertz frequencies, Phys. Rev. B 85, p. 245407. Kamat, P. V. (2010). Graphene-based nanoarchitectures. anchoring semiconductor and metal nanoparticles on a two-dimensional carbon support, J. Phys. Chem. Lett. 1, pp. 520 – 527. Kaminer, I., Katan, Y. T., Buljan, H., Shen, Y., Ilic, O., López, J. J., Wong, L. J., Joannopoulos, J. D., and Soljaçić, M. (2015). Quantum Čerenkov effect from hot carriers in graphene: An efficient plasmonic source, arXiv:1510.00883 [physics.optics] , 1. Kang, N. (2015). Green’s Function for Poisson Equation in Layered NanoStructures including Graphene, Master’s thesis, University of Waterloo. Kasry, A., Ardakani, A. A., Tulevski, G. S., Menges, B., Copel, M., and Vyklicky, L. (2012). Highly efficient fluorescence quenching with graphene, J. Phys. Chem. C 116, pp. 2858–2862. Katsnelson, M. I. (2011). Coulomb drag in graphene single layers separated by a thin spacer, Phys. Rev. B 84, p. 041407(R). Kauranen, M. and Zayats, A. V. (2012). Nonlinear plasmonics, Nature Photonics 6, pp. 737–748. Khavasi, A. (2015). Design of ultra-broadband graphene absorber using circuit theory, J. Opt. Soc. Am. B 32, pp. 1941–1946. Khavasi, A. and Rejaei, B. (2014). Analytical modeling of graphene ribbons as optical circuit elements, IEEE J. Quantum Electron. 50, pp. 397–403. Khurgin, J. B. (2015). How to deal with the loss in plasmonics and metamaterials, Nature Nanotechnology 10, pp. 2–6. Khurgin, J. B. and Boltasseva, A. (2012). Reflecting upon the losses in plasmonics and metamaterials, MRS Bulletin 37, pp. 768–779. Kim, J. T., Yu, Y.-J., Choi, H., and Choi, C.-G. (2014). Graphene-based plasmonic photodetector for photonic integrated circuits, Opt. Express 22, pp. 803–808. Kim, S., Jo, I., Nah, J., Yao, Z., Banerjee, S. K., and Tutuc, E. (2011). Coulomb drag of massless fermions in graphene, Phys. Rev. B 83, p. 161401. Kitamura, R., Pilon, L., and Jonasz, M. (2007). Optical constants of silica glass from extreme ultraviolet to far infrared at near room temperature, Appl. Opt. 46, pp. 8118–8133. Klimov, V. (2014). Nanoplasmonics (Pan Stanford). Kneipp, K. (2007). Surface-enhanced raman scattering, Phys. Today 60, pp. 40– 46. Koch, R. J., Seyller, T., and Schaefer, J. A. (2010). Strong phonon-plasmon coupled modes in the graphene/silicon carbide heterosystem, Phys. Rev. B 82, p. 201413. Konstantatos, G., Badioli, M., Gaudreau, L., Osmond, J., Bernechea, M., de Arquer, F. P. G., Gatti, F., and Koppens, F. H. L. (2012). Hybrid graphenequantum dot phototransistors with ultrahigh gain, Nature Nanotechnology 7, pp. 363 – 368.

page 412

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Bibliography

9in x 6in

b2445-mas

413

Koppens, F. H. L., Chang, D. E., and de Abajo, F. J. G. (2011). Graphene plasmonics: A platform for strong light-matter interactions, Nano Lett. 11, pp. 3370 – 3377. Koppens, F. H. L., Mueller, T., Avouris, P., Ferrari, A. C., Vitiello, M. S., and Polini, M. (2014). Photodetectors based on graphene, other twodimensional materials and hybrid systems, Nature Nanotechnology 9, pp. 780–793. Kort-Kamp, W. J. M., Amorim, B., Bastos, G., Pinheiro, F. A., Rosa, F. S. S., Peres, N. M. R., and Farina, C. (2015). Active magneto-optical control of spontaneous emission in graphene, Phys. Rev. B 92, p. 205415. Kotov, V. N., Uchoa, B., Pereira, V. M., Guinea, F., and Castro Neto, A. H. (2012). Electron-electron interactions in graphene: Current status and perspectives, Rev. Mod. Phys. 84, pp. 1067–1125. Kragler, R. and Thomas, H. (1980). Dielectric function in the relaxation-time approximation generalized to electronic multiple-band systems, Z. Physik B - Condensed Matter 39, pp. 99–107. Kravets, V. G., Jalil, R., Kim, Y.-J., Ansell, D., Aznakayeva, D. E., Thackray, B., Britnell, L., Belle, B. D., Withers, F., Radko, I. P., Han, Z., Bozhevolnyi, S. I., Novoselov, K. S., Geim, A. K., and Grigorenko, A. N. (2014). Graphene-protected copper and silver plasmonics, Scientific Reports 4, p. 5517. Kravets, V. G., Schedin, F., Jalil, R., Britnell, L., Novoselov, K. S., and Grigorenko, A. N. (2012). Surface hydrogenation and optics of a graphene sheet transferred onto a plasmonic nanoarray, The Journal of Physical Chemistry C 116, pp. 3882–3887. Kretinin, A. V., Cao, Y., Tu, J. S., Yu, G. L., Jalil, R., Novoselov, K. S., Haigh, S. J., Gholinia, A., Mishchenko, A., Lozada, M., Georgiou, T., Woods, C. R., Withers, F., Blake, P., Eda, G., Wirsig, A., Hucho, C., Watanabe, K., Taniguchi, T., Geim, A. K., and Gorbachev, R. V. (2014). Electronic properties of graphene encapsulated with different two-dimensional atomic crystals, Nano Lett. 14, pp. 3270 – 3276. Kretschmann, E. and Raether, H. (1968). Radiative decay of nonradiative surface plasmon excited by light, Z. Naturf. A 23, pp. 2135–2136. Kumar, A., Low, T., Fung, K. H., Avouris, P., and Fang, N. X. (2015). Tunable light-matter interaction and the role of hyperbolicity in graphene-hbn system, Nano Lett. 15, pp. 3172–3180. Lee, C., Kim, J. Y., Bae, S., Kim, K. S., Hong, B. H., and Choi, E. J. (2011). Optical response of large scale single layer graphene, Appl. Phys. Lett. 98, p. 071905. Lee, C., Wei, X., Kysar, J. W., and Hone, J. (2008). Measurement of the elastic properties and intrinsic strength of monolayer graphene, Science 321, 5887, pp. 385–388. Lee, S. H., Choi, M., Kim, T.-T., Lee, S., Liu, M., Yin, X., Choi, H. K., Lee, S. S., Choi, C.-G., Choi, S.-Y., Zhang, X., and Min, B. (2012). Switching terahertz waves with gate-controlled active graphene metamaterials, Nature Materials 11, pp. 936 – 941.

page 413

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

414

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Lekner, J. (1991). Reflection and refraction by uniaxial crystals, J. Phys.: Condens. Matter 3, pp. 6121–6133. Li, E.-P. and Chu, H.-S. (2014). Plasmonic Nanoelectronics and Sensing (Cambridge). Li, Z. Q., Henriksen, E. A., Jiang, Z., Hao, Z., Martin, M. C., Kim, P., Stormer, H. L., and Basov, D. N. (2008). Dirac charge dynamics in graphene by infrared spectroscopy, Nature Phys. 4, pp. 532–535. Liang, Z., Sun, J., Jiang, Y., Jiang, L., and Chen, X. (2014). Plasmonic enhanced optoelectronic devices, Plasmonics 9, pp. 859–866. Lim, D.-K., Barhoumi, A., Wylie, R. G., Reznor, G., Langer, R. S., and Kohane, D. S. (2013). Enhanced photothermal effect of plasmonic nanoparticles coated with reduced graphene oxide, Nano Lett. 13, pp. 4075–4079. Lin, I.-T. and Liu, J.-M. (2014). Optimization of double-layer graphene plasmonic waveguides, Appl. Phys. Lett. 105, p. 061116. Lindhard, J. (1954). On the properties of a gas of charged particles, Mat.-Fys. Medd. K. Dan. Vidensk. Selsk. 28, pp. 1 – 57. Ling, X., Xie, L., Fang, Y., Xu, H., Zhang, H., Kong, J., Dresselhaus, M. S., Zhang, J., and Liu, Z. (2010). Can graphene be used as a substrate for raman enhancement? Nano Lett. 10, pp. 553–561. Liu, C.-Y., Liang, K.-C., Chen, W., hao Tu, C., Liu, C.-P., and Tzeng, Y. (2011a). Plasmonic coupling of silver nanoparticles covered by hydrogen-terminated graphene for surface-enhanced raman spectroscopy, Opt. Express 19. Liu, F., Qian, C., and Chong, Y. D. (2015a). Directional excitation of graphene surface plasmons, Opt. Express 23, pp. 2383–2391. Liu, H., Sun, S., Wu, L., and Bai, P. (2014a). Optical near-field enhancement with graphene bowtie antennas, Plasmonics 9, pp. 845–850. Liu, P. Q., Valmorra, F., Maissen, C., and Faist, J. (2015b). Electrically tunable graphene anti-dot array terahertz plasmonic crystals exhibiting multi-band resonances, Optica 2, pp. 135 – 140. Liu, S., Hu, M., Zhang, Y., Li, Y., and Zhong, R. (2009). Electromagnetic diffraction radiation of a subwavelength-hole array excited by an electron beam, Phys. Rev. E 80, p. 036602. Liu, S., Zhang, C., Hu, M., Chen, X., Zhang, P., Gong, S., Zhao, T., and Zhong, R. (2014b). Coherent and tunable terahertz radiation from graphene surface plasmon polaritons excited by an electron beam, Applied Physics Letters 104, 201104. Liu, Y., Cheng, R., Liao, L., Zhou, H., Bai, J., Liu, G., Liu, L., Huang, Y., and Duan, X. (2011b). Plasmon resonance enhanced multicolour photodetection by graphene, Nature Communications 2, 579. Liu, Y. and Willis, R. F. (2010). Plasmon-phonon strongly coupled mode in epitaxial graphene, Phys. Rev. B 81, p. 081406. Liu, Y., Willis, R. F., Emtsev, K. V., and Seyller, T. (2008). Plasmon dispersion and damping in electrically isolated two-dimensional charge sheets, Phys. Rev. B 78. Liua, Y. and Zhang, X. (2011). Metamaterials: a new frontier of science and technology, Chem. Soc. Rev. 40, pp. 2494–2507.

page 414

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Bibliography

9in x 6in

b2445-mas

415

Llatser, I., Kremers, C., Cabellos-Aparicio, A., Jornet, J. M., Alarcón, E., and Chigrin, D. N. (2012). Graphene-based nano-patch antenna for terahertz radiation, Photonics and Nanostructures - Fundamentals and Applications 10, pp. 353–358. Low, T. and Avouris, P. (2014). Graphene plasmonics for terahertz to mid-infrared applications, ACS Nano 8, pp. 1086–1101. Low, T., Guinea, F., Yan, H., Xia, F., and Avouris, P. (2014a). Novel mid-infrared plasmonic properties of bilayer graphene, Phys. Rev. Lett. 112, p. 116801. Low, T., Roldán, R., Wang, H., Xia, F., Avouris, P., Moreno, L. M., and Guinea, F. (2014b). Plasmons and screening in monolayer and multilayer black phosphorus, Phys. Rev. Lett. 113, p. 106802. Lu, J.-K. (1993). Boundary Value Problems for Analytic Functions (World Scientific, Singapore). Luo, X., Qiu, T., Lu, W., and Ni, Z. (2013). Plasmons in graphene: Recent progress and applications, Materials Science and Engineering R 74, pp. 351 – 376. Luxmoore, I. J., Gan, C. H., Liu, P. Q., Valmorra, F., Li, P., Faist, J., and Nash, G. R. (2014). Strong coupling in the far-infrared between graphene plasmons and the surface optical phonons of silicon dioxide, ACS Photonics 1, p. 1151. Ma, R.-M., Oulton, R. F., Sorger, V. J., and Zhang, X. (2013). Plasmon lasers: coherent light source at molecular scales, Laser Photon. Rev. 7, pp. 1–21. MacDonald, K. F., Sámson, Z. L., Stockman, M. I., and Zheludev, N. I. (2009). Ultrafast active plasmonics, Nature Photonics 3, pp. 55–58. Mahan, G. D. (2000). Many-Particle Physics, 3rd edn. (Springer, New York). Maier, S. A. (2007). Plasmonics: Fundamentals and Applications (Springer, New York). Manjavacas, A., Marchesin, F., Thongrattanasiri, S., Koval, P., Nordlander, P., Sánchez-Portal, D., and de Abajo, F. J. G. (2013). Tunable molecular plasmons in polycyclic aromatic hydrocarbons, ACS Nano 7, pp. 3635–3643. Manjavacas, A., Nordlander, P., and de Abajo, F. J. G. (2012a). Plasmon blockade in nanostructured graphene, ACS Nano 6, pp. 1724 – 1731. Manjavacas, A., Thongrattanasiri, S., Chang, D. E., and de Abajo, F. J. G. (2012b). Temporal quantum control with graphene, New J. Phys. 14, p. 123020. Manjavacas, A., Thongrattanasiri, S., and de Abajo, F. (2015). Plasmons driven by single electrons in graphene nanoislands, Nanophotonics 2, pp. 139–151. Manjavacas, A., Thongrattanasiri, S., Greffet, J.-J., and de Abajo, F. J. G. (2014). Graphene optical-to-thermal converter, Appl. Phys. Lett. 105, p. 211102. Manzoni, M. T., Silveiro, I., de Abajo, F. J. G., and Chang, D. E. (201). Secondorder quantum nonlinear optical processes in graphene nanostructures, New J. Phys. 17, p. 083031. Maradudin, A. A. (1986). Electromagnetic surface excitations on rough surfaces, in R. F. Wallis, G. I. Stegeman, and T. Tamir (eds.), Electromagnetic Surface Excitations, Springer Series on Wave Phenomena, Vol. 3 (Springer Berlin Heidelberg), pp. 57–131.

page 415

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

416

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Maradudin, A. A. (2007a). The design of randomly rough surfaces that scatter waves in a specified manner, in A. A. Maradudin (ed.), Light Scattering and Nanoscale Surface Roughness, Nanostructure Science and Technology (Springer), pp. 467–488. Maradudin, A. A. (ed.) (2007b). Light Scattering and Nanoscale Surface Roughness (Springer). Maradudin, A. A. (2014). Surface electromagnetic waves on structured perfectly conducting surfaces, in A. A. Maradudin, W. L. Barnes, and J. R. Sambles (eds.), Modern Plasmonics (Elsevier), pp. 223–251. Maradudin, A. A., Barnes, W. L., and Sambles, J. R. (eds.) (2014). Modern Plasmonics (Elsevier). Markos, P. and Soukoulis, C. M. (2008). Wave Propagation: From Electrons to Photonic Crystals and Left-Handed Materials (Princeton University Press, New Jersey). Martín-Moreno, L., García-Vidal, F. J., Lezec, H. J., Pellerin, K. M., Thio, T., Pendry, J. B., and Ebbesen, T. W. (2001). Theory of extraordinary optical transmission through subwavelength hole arrays, Phys. Rev. Lett. 86, pp. 1114–1117. Maxwell, J. C. (1865). A dynamical theory of the electromagnetic field, Philosophical Transactions of the Royal Society of London 155, pp. 459–512. Menabde, S., Mason, D., Kornev, E., Lee, C., and Park, N. (2016). Direct optical probing of transverse electric mode in graphene, Scientific Reports 6, p. 21523. Mermin, N. D. (1970). Lindhard dielectric function in the relaxation-time approximation, Phys. Rev. B 1, pp. 2362–2363. Mihaila, B. (2011). Lindhard function of a d-dimensional fermi gas, arXiv:1111.5337 , pp. 1–8. Mikhailov, S. A. and Savostianova, N. A. (2005). Microwave response of a twodimensional electron stripe, Phys. Rev. B 71, p. 035320. Mikhailov, S. A. and Ziegler, K. (2007). New electromagnetic mode in graphene, Phys. Rev. Lett. 99, p. 016803. Mishchenko, A., Tu, J. S., Cao, Y., Gorbachev, R. V., Wallbank, J. R., Greenaway, M., Morozov, V. E., Morozov, S. V., Zhu, M. J., Wong, S. L., Withers, F., Woods, C. R., Kim, Y.-J., Watanabe, K., Taniguchi, T., Vdovin, E. E., Makarovsky, O., Fromhold, T. M., Falko, V. I., Geim, A. K., Eaves, L., and Novoselov, K. S. (2014). Twist-controlled resonant tunnelling in graphene-boron nitride-graphene heterostructures, Nature Nanotechnology 9, pp. 808–813. Mitrofanov, O., Yu, W., Thompson, R. J., Jiang, Y., Brener, I., Pan, W., Berger, C., de Heer, W. A., and Jiang, Z. (2013). Probing terahertz surface plasmon waves in graphene structures, Appl. Phys. Lett. 103, 11, p. 111105. Mittleman, D. M. (2013). Frontiers in terahertz sources and plasmonics, Nature Photonics 7, pp. 666–669. Mönch, W. (2010). Semiconductor Surfaces and Interfaces, 3rd edn. (Springer). Mooradian, A. and Wright, G. B. (1966). Observation of the interaction of plasmons with longitudinal optical phonons in gaas, Phys. Rev. Lett. 16, pp.

page 416

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Bibliography

9in x 6in

b2445-mas

417

999–1001. Moriya, R., Yamaguchi, T., Inoue, Y., Sata, Y., Morikawa, S., Masubuchi, S., and Machida, T. (2015). Influence of the density of states of graphene on the transport properties of graphene/mos2/metal vertical field-effect transistors, Appl. Phys. Lett. 106, p. 223103. Nakajima, S. (1955). Perturbation theory in statistical mechanics, Advances in Physics 4, pp. 363–380. Nene, P., Strait, J. H., Chan, W.-M., Manolatou, C., Kevek, J. W., Tiwari, S., McEuen, P. L., and Rana, F. (2014). Coupling of plasmon modes in graphene microstructures, Appl. Phys. Lett. 105, p. 143108. Nikitin, A. Y., Guinea, F., Garcia-Vidal, F. J., and Martin-Moreno, L. (2012a). Surface plasmon enhanced absorption and suppressed transmission in periodic arrays of graphene ribbons, Phys. Rev. B 85, p. 081405(R). Nikitin, A. Y., Guinea, F., and Martin-Moreno, L. (2012b). Resonant plasmonic effects in periodic graphene antidot arrays, Applied Physics Letters 101, p. 151119. Nikitin, A. Y., Low, T., and Martin-Moreno, L. (2014). Anomalous reflection phase of graphene plasmons and its influence on resonators, Phys. Rev. B 90, p. 041407. Niu, J., Shin, Y. J., Son, J., Lee, Y., Ahn, J.-H., and Yang, H. (2012). Shifting of surface plasmon resonance due to electromagnetic coupling between graphene and au nanoparticles, Opt. Express 20, pp. 19690 – 19696. Novoselov, K. S. and Castro Neto, A. H. (2012). Two-dimensional crystals-based heterostructures: materials with tailored properties, Physica Scripta 2012, p. 014006. Novoselov, K. S., Geim, A. K., Morozov, S. V., Jiang, D., Zhang, Y., Dubonos, S. V., Grigorieva, I. V., and Firsov, A. A. (2004). Electric field effect in atomically thin carbon films, Science 306, pp. 666–669. Novotny, L. and Hecht, B. (2014). Principles of Nano-Optics, 2nd edn. (Cambridge University Press, Cambridge). Ochiai, T. (2015). Spatially periodic modulation of optical conductivity in doped graphene by two-dimensional diffraction grating, J. Opt. Soc. Am. B 32, pp. 701–707. Otto, A. (1968). Excitation of nonradiative surface plasma waves in silver by the method of frustrated total reflection, Z. Phys. 216, pp. 398–410. Ozbay, E. (2006). Plasmonics: Merging photonics and electronics at nanoscale dimensions, Science 311, pp. 189–193. Padooru, Y. R., Yakovlev, A. B., Kaipa, C. S. R., Hanson, G. W., Medina, F., and Mesa, F. (2013). Dual capacitive-inductive nature of periodic graphene patches: Transmission characteristics at low-terahertz frequencies, Phys. Rev. B 87, p. 115401. Palik, E. D. (1997). Handbook of Optical Constants of Solids, 1st edn. (Academic Press). Pelton, M., Aizpurua, J., and Bryant, G. (2008). Metal-nanoparticle plasmonics, Laser & Photon. Rev. 2, pp. 136–159. Pelton, M. and Bryant, G. W. (2013). Introduction to Metal-Nanoparticle Plas-

page 417

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

418

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

monics, 1st edn. (John Wiley & Sons, Inc, New Jersey). Peres, N. M. R. (2010). Colloquium: The transport properties of graphene: An introduction, Rev. Mod. Phys. 82. Peres, N. M. R., Bludov, Y. V., Ferreira, A., and Vasilevskiy, M. I. (2013). Exact solution for square-wave grating covered with graphene: surface plasmonpolaritons in the terahertz range, J. Phys.: Condens. Matter 25, p. 125303. Peres, N. M. R., Bludov, Y. V., Santos, J. E., Jauho, A.-P., and Vasilevskiy, M. I. (2014). Optical bistability of graphene in the terahertz range, Phys. Rev. B 90, p. 125425. Peres, N. M. R., dos Santos, J. M. B. L., and Stauber, T. (2007). Phenomenological study of the electronic transport coefficients of graphene, Phys. Rev. B 76, p. 073412. Peres, N. M. R., Ferreira, A., Bludov, Y. V., and Vasilevskiy, M. I. (2012). Light scattering by a medium with a spatially modulated optical conductivity: the case of graphene, J. Phys.: Condens. Matter 24, p. 245303. Pettit, R. B., Silcox, J., and Vincent, R. (1975). Measurement of surface-plasmon dispersion in oxidized aluminum films, Phys. Rev. B 11, pp. 3116–3123. Polanco, J., Fitzgerald, R. M., and Maradudin, A. A. (2013). Scattering of surface plasmon polaritons by one-dimensional surface defects, Phys. Rev. B 87, p. 155417. Politano, A. and Chiarello, G. (2014). Plasmon modes in graphene: status and prospect, Nanoscale 6, pp. 10927–10940. Poole Jr. , C. P. (2004). Encyclopedic Dictionary of Condensed Matter Physics, Vol. 1, 1st edn. (Academic Press, New York). Powell, C. J. and Swan, J. B. (1959). Origin of the characteristic electron energy losses in aluminum, Phys. Rev. 115, p. 869. Pratesi, R., Toraldo di Francia, G., Ronchi, L., and Scheggi, A. M. (1962). Radiation from a charged particle in uniform straight motion through a particular stratified medium, Il Nuovo Cimento XXV, p. 756. Principi, A., Vignale, G., Carrega, M., and Polini, M. (2013). Intrinsic lifetime of dirac plasmons in graphene, Phys. Rev. B 88, p. 195405. Prodan, E., Radloff, C., Halas, N. J., and Nordlander, P. (2003). A hybridization model for the plasmon response of complex nanostructures, Science 302, pp. 419–422. Purcell, E. M. (1995). Spontaneous emission probabilities at radio frequencies, in E. Burstein and C. Weisbuch (eds.), Confined Electrons and Photons, NATO ASI Series, Vol. 340 (Springer), pp. 839–839. Quidant, R. (2012). Plasmonic tweezers—the strength of surface plasmons, MRS Bulletin 37, pp. 739–744. Raether, H. (1988). Surface Plasmons on Smooth and Rough Surfaces and on Gratings, 1st edn. (Springer Tracts in Modern Physics, New York). Rahman, T. S. and Maradudin, A. A. (1980). Surface-plasmon dispersion relation in the presence of surface roughness, Phys. Rev. B 21, pp. 2137–2143. Rayleigh, L. (1907). On the dynamical theory of gratings, Proc. R. Soc. Lond. A 79, pp. 399–416. Reece, P. J. (2008). Plasmonics: Finer optical tweezers, Nature Photonics 2, pp.

page 418

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Bibliography

9in x 6in

b2445-mas

419

333–334. Rejaei, B. and Khavasi, A. (2015). Scattering of surface plasmons on graphene by a discontinuity in surface conductivity, J. of Opt. 17, p. 075002. Ritchie, R. H. (1957). Plasma losses by fast electrons in thin films, Phys. Rev. 106, p. 874. Ritchie, R. H., Arakawa, E. T., Cowan, J. J., and Hamm, R. N. (1968). Surfaceplasmon resonance effect in grating diffraction, Phys. Rev. Lett. 21, pp. 1530–1533. Rodrigo, D., Limaj, O., DavideJanner, Etezadi, D., de Abajo, F. J. G., Pruneri, V., and Altug, H. (2015). Mid-infrared plasmonic biosensing with graphene, Science 349, 6244, pp. 165–168. Rothwell, E. J. and Cloud, M. J. (2009). Electromagnetics, 2nd edn. (CRC Press). Rouhi, N., Capdevila, S., Jain, D., Zand, K., Wang, Y., Brown, E., Jofre, L., and Burke, P. (2012). Terahertz graphene optics, Nano Research 5, pp. 667–678. Saleh, B. E. A. and Teich, M. C. (2012). Fundamentals of Photonics, 2nd edn. (Wiley). Sambles, J. R., Bradberya, G. W., and Yang, F. (1991). Optical excitation of surface plasmons: An introduction, Contemporary Physics 32, pp. 173– 183. Sánchez-Gil, J. A. and Maradudin, A. A. (1999). Near-field and far-field scattering of surface plasmon polaritons by one-dimensional surface defects, Phys. Rev. B 60, pp. 8359–8367. Santos, J. E., Vasilevskiy, M. I., Peres, N. M. R., Smirnov, G., and Bludov, Y. V. (2014). Renormalization of nanoparticle polarizability in the vicinity of a graphene-covered interface, Phys. Rev. B 90, p. 235420. Sarid, D. and Challener, W. (2010). Modern Introduction to Surface Plasmons: Theory, Mathematica Modeling, and Applications (Cambridge University Press, Cambridge). Satou, A. and Mikhailov, S. A. (2007). Excitation of two-dimensional plasmon polaritons by an incident electromagnetic wave at a contact, Phys. Rev. B 75, p. 045328. Schieber, D. and Schächter, L. (2001). Wake field of an electron bunch moving parallel to a dielectric cylinder, Phys. Rev. E 64, p. 056503. Schiefele, J., Pedrós, J., Sols, F., Calle, F., and Guinea, F. (2013). Coupling light into graphene plasmons through surface acoustic waves, Phys. Rev. Lett. 111, p. 237405. Schiefele, J., Sols, F., and Guinea, F. (2012). Temperature dependence of the conductivity of graphene on boron nitride, Phys. Rev. B 85, p. 195420. Schlücker, S. (2014). Surface-enhanced raman spectroscopy: Concepts and chemical applications, Angew. Chem. Int. Ed. 53, pp. 4756 – 4795. Sensale-Rodriguez, B., Yan, R., Zhu, M., Jena, D., Liu, L., and Grace Xing, H. (2012). Efficient terahertz electro-absorption modulation employing graphene plasmonic structures, Appl. Phys. Lett. 101, 26, p. 261115. Sharma, B., Frontiera, R. R., Henry, A.-I., Ringe, E., and Duyne, R. P. V. (2012). Sers: Materials, applications, and the future, Materials Today 15, pp. 16 – 25.

page 419

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

420

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Sheng, P., Stepleman, R. S., and Sanda, P. N. (1982). Exact eigenfunctions for square-wave gratings: Application to diffraction and surface-plasmon calculations, Phys. Rev. B 26, pp. 2907–2916. Shung, K. W. K. (1986). Dielectric function and plasmon structure of stage-1 intercalated graphite, Phys. Rev. B 34, p. 979. Shylau, A. A., Badalyan, S. M., Peeters, F. M., and Jauho, A. P. (2015). Electron polarization function and plasmons in metallic armchair graphene nanoribbons, Phys. Rev. B 91, p. 205444. Silveiro, I. and de Abajo, F. J. G. (2014). Plasmons in inhomogeneously doped neutral and charged graphene nanodisks, Appl. Phys. Lett. 104, p. 131103. Silveiro, I., Manjavacas, A., Thongrattanasiri, S., and Abajo, F. J. G. (2013). Plasmonic energy transfer in periodically doped graphene, New Journal of Physics 15, p. 033042. Slipchenko, T. M., Nesterov, M. L., Martin-Moreno, L., and Nikitin, A. Y. (2013a). Analytical solution for the diffraction of an electromagnetic wave by a graphene grating, J. Opt. 15, p. 114008. Slipchenko, T. M., Nesterov, M. L., Martin-Moreno, L., and Nikitin, A. Y. (2013b). Analytical solution for the diffraction of an electromagnetic wave by a graphene grating, J. Opt. 15 114008 15, p. 114008. Sommerfeld, A. (1899). Über die fortpflanzung elektrodynamischer wellen an längs eines drahtes, Ann. der Physik und Chemie 67, pp. 233–290. Song, B., Li, D., Qi, W., Elstner, M., Fan, C., and Fang, H. (2010). Graphene on au(111): A highly conductive material with excellent adsorption properties for high-resolution bio/nanodetection and identification, Chem. Phys. Chem. 11, pp. 585–589. Sorger, C., Preu, S., Schmidt, J., Winnerl, S., Bludov, Y. V., Peres, N. M. R., Vasilevskiy, M. I., and Weber, H. B. (2015). Terahertz response of patterned epitaxial graphene, New J. of Phys. 17, p. 053045. Sorger, V. J., Oulton, R. F., Ma, R.-M., and Zhang, X. (2012). Toward integrated plasmonic circuits, MRS Bulletin 37, pp. 728–738. Stauber, T. (2014). Plasmonics in dirac systems: from graphene to topological insulators, J. Phys.: Condens. Matter 26, p. 123201. Stauber, T., Peres, N. M. R., and Geim, A. K. (2008). Optical conductivity of graphene in the visible region of the spectrum, Phys. Rev. B 78, p. 085432. Stauber, T., Peres, N. M. R., and Guinea, F. (2007). Electronic transport in graphene: A semi-classical approach including midgap states, Phys. Rev. B 76, p. 205423. Stern, F. (1967). Polarizability of a two-dimensional electron gas, Phys. Rev. Lett. 18, p. 546. Stiles, P. L., Dieringer, J. A., Shah, N. C., and Duyne, R. P. V. (2008). Surfaceenhanced raman spectroscopy, Annu. Rev. Anal. Chem. 1, pp. 601 – 626. Stockman, M. I. (2011). Nanoplasmonics: The physics behind the applications, Phys. Today 64, pp. 39–44. Strait, J. H., Nene, P., Chan, W.-M., Manolatou, C., Tiwari, S., Rana, F., Kevek, J. W., and McEuen, P. L. (2013). Confined plasmons in graphene microstructures: Experiments and theory, Phys. Rev. B 87, p. 241410.

page 420

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Bibliography

9in x 6in

b2445-mas

421

Sule, N., Willis, K. J., Hagness, S. C., and Knezevic, I. (2014). Terahertzfrequency electronic transport in graphene, Phys. Rev. B 90, p. 045431. Sun, S., Gao, L., Liu, Y., and Sun, J. (2011a). Assembly of cdse nanoparticles on graphene for low-temperature fabrication of quantum dot sensitized solar cell, Appl. Phys. Lett. 98. Sun, Z., Gutierrez-Rubio, A., Basov, D. N., and Fogler, M. M. (2015). Hamiltonian optics of hyperbolic polaritons in nanogranules, Nano Lett. 15, pp. 4455–4460. Sun, Z., Pint, C. L., Marcano, D. C., Zhang, C., Yao, J., Ruan, G., Yan, Z., Zhu, Y., Hauge, R. H., and Tour, J. M. (2011b). Towards hybrid superlattices in graphene, Nature Communications 2, p. 1. Swathi, R. S. and Sebastian, K. L. (2009). Long range resonance energy transfer from a dye molecule to graphene has distance4 dependence, The J. of Chem. Phys. 130, p. 086101. Tame, M. S., McEnery, K. R., Ozdemir, S. K., Lee, J., Maier, S. A., and Kim, M. S. (2013). Quantum plasmonics, Nature Phys. 9, pp. 329–340. Tao, Z., Ren-Bin, Z., Min, H., Xiao-Xing, C., Ping, Z., Sen, G., and Sheng-Gang, L. (2015). Tunable terahertz radiation from arbitrary profile dielectric grating coated with graphene excited by an electron beam, Chin. Phys. B 24, p. 094102. Tassin, P., Koschny, T., and Soukoulis, C. M. (2013). Graphene for terahertz applications, Science 341, pp. 620–621. Temnov, V. V. (2012). Ultrafast acousto-magneto-plasmonics, Nature Photonics 6, pp. 728–736. Teng, Y. Y. and Stern, E. A. (1967). Plasma radiation from metal grating surfaces, Phys. Rev. Lett. 19, p. 511. Thongrattanasiri, S. and de Abajo, F. J. G. (2013). Optical field enhancement by strong plasmon interaction in graphene nanostructures, Phys. Rev. Lett. 110, p. 187401. Thongrattanasiri, S., Koppens, F. H. L., and de Abajo, F. J. G. (2012a). Complete optical absorption in periodically patterned graphene, Phys. Rev. Lett. 108, p. 047401. Thongrattanasiri, S., Manjavacas, A., and de Abajo, F. J. G. (2012b). Quantum finite-size effects in graphene plasmons, ACS Nano 6, pp. 1766–1775. Tielrooij, K. J., Orona, L., Ferrier, A., Badioli, M., Navickaite, G., Coop, S., Nanot, S., Kalinic, B., Cesca, T., Gaudreau, L., Ma, Q., Centeno, A., Pesquera, A., Zurutuza, A., de Riedmatten, H., Goldner, P., de Abajo, F. J. G., Jarillo-Herrero, P., and Koppens, F. H. L. (2015). Electrical control of optical emitter relaxation pathways enabled by graphene, Nature Phys. 11, pp. 281 – 287. Toigo, F., Marvin, A., Celli, V., and Hill, N. R. (1977). Optical properties of rough surfaces: General theory and the small roughness limit, Phys. Rev. B 15, pp. 5618–5626. Tokunaga, E., Ivanov, A. L., Nair, S. V., and Masumoto, Y. (2001). Hopfield coefficients measured by inverse polariton series, Phys. Rev. B 63, p. 233203. Tomadin, A., Guinea, F., and Polini, M. (2014). Generation and morphing of

page 421

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

422

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

plasmons in graphene superlattices, Phys. Rev. B 89, p. 224512. Toropov, A. A. and Shubina, T. V. (2015). Plasmonic Effects in MetalSemiconductor Nanostructures (Oxford). Torre, I., Tomadin, A., Krahne, R., Pellegrini, V., and Polini, M. (2015). Electrical plasmon detection in graphene waveguides, Phys. Rev. B 91, p. 081402(R). Turbadar, T. (1959). Complete absorption of light by thin metal films, Proceedings of the Physical Society 73, p. 40. Tymchenko, M., Nikitin, A. Y., and Martín-Moreno, L. (2013). Faraday rotation due to excitation of magnetoplasmons in graphene microribbons, ACS Nano 7, 11, pp. 9780–9787. Urich, A., Pospischil, A., Furchi, M. M., Dietze, D., Unterrainer, K., and Mueller, T. (2012). Silver nanoisland enhanced raman interaction in graphene, Appl. Phys. Lett. 101, p. 153113. Vakil, A. and Engheta, N. (2011). Transformation optics using graphene, Science 332, pp. 1291 – 1294. van Hulst, N. F. (2012). Nanophotonics: Plasmon quantum limit exposed, Nature Nanotechnology 7, pp. 775 – 777. Vasić, B., Isić, G., and Gajić, R. (2013). Localized surface plasmon resonances in graphene ribbon arrays for sensing of dielectric environment at infrared frequencies, J. Appl. Phys. 113, p. 013110. Velizhanin, K. A. (2015). Geometric universality of plasmon modes in graphene nanoribbon arrays, Phys. Rev. B 91, p. 125429. Velizhanin, K. A. and Efimov, A. (2011). Probing plasmons in graphene by resonance energy transfer, Phys. Rev. B 84, p. 085401. Vesseur, E. J. R., Aizpurua, J., Coenen, T., Reyes-Coronado, A., Batson, P. E., and Polman, A. (2012). Plasmonic excitation and manipulation with an electron beam, MRS Bulletin 37, pp. 752–760. Vladimirov, V. S. (1971). Equations of Mathematical Physics (Dekker, New York). Vo-Dinh, T., Fales, A. M., Griffin, G. D., Khoury, C. G., Liu, Y., Ngo, H., Norton, S. J., Register, J. K., Wang, H.-N., and Yuan, H. (2013). Plasmonic nanoprobes: from chemical sensing to medical diagnostics and therapy, Nanoscale 5, pp. 10127–10140. Voronovich, A. G. (2007). Rayleigh hypothesis, in A. A. Maradudin (ed.), Light Scattering and Nanoscale Surface Roughness, Nanostructure Science and Technology (Springer), pp. 93–105. Wachsmuth, P., Hambach, R., Benner, G., and Kaiser, U. (2014). Plasmon bands in multilayer graphene, Phys. Rev. B 90, p. 235434. Wang, P., Liang, O., Zhang, W., Schroeder, T., and Xie, Y.-H. (2013). Ultrasensitive graphene-plasmonic hybrid platform for label-free detection, Advanced Materials 25, pp. 4918 – 4924. Wang, P., Zhang, W., Liang, O., Pantoja, M., Katzer, J., Schroeder, T., and Xie, Y.-H. (2012a). Giant optical response from graphene–plasmonic system, ACS Nano 6, pp. 6244–6249. Wang, W. (2012). Plasmons and optical excitations in graphene rings, J. of Phys.: Cond. Matt. 24, p. 402202. Wang, W., Apell, P., and Kinaret, J. (2011). Edge plasmons in graphene nanos-

page 422

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Bibliography

9in x 6in

b2445-mas

423

tructures, Phys. Rev. B 84, p. 085423. Wang, W., Apell, S. P., and Kinaret, J. M. (2012b). Edge magnetoplasmons and the optical excitations in graphene disks, Phys. Rev. B 86, p. 125450. Wang, W., Christensen, T., Jauho, A.-P., Thygesen, K. S., Wubs, M., and Mortensen, N. A. (2015). Plasmonic eigenmodes in individual and bow-tie graphene nanotriangles, Scientific Reports 5, 9535. Wang, W. and Kinaret, J. M. (2013). Plasmons in graphene nanoribbons: Interband transitions and nonlocal effects, Phys. Rev. B 87, p. 195424. Wang, W., Kinaret, J. M., and Apell, S. P. (2012c). Excitation of edge magnetoplasmons in semi-infinite graphene sheets: Temperature effects, Phys. Rev. B 85, p. 235444. Wang, W., Li, B.-H., Mortensen, N. A., and Christensen, J. (2016). Localized surface plasmons in vibrating graphene nanodisks, Nanoscale 8, p. 3809. Weber, M. L. and Willets, K. A. (2012). Nanoscale studies of plasmonic hot spots using super-resolution optical imaging, MRS Bulletin 37, pp. 745–751. Weinberg, S. (1996). The Quantum Theory of Fields, Vols. 1, 2 and 3 (Cambridge University Press, New York). Wijaya, E., Lenaerts, C., Maricot, S., Hastanin, J., Habraken, S., Vilcot, J.P., Boukherroub, R., and Szunerits, S. (2011). Surface plasmon resonancebased biosensors: From the development of different {SPR} structures to novel surface functionalization strategies, Current Opinion in Solid State and Materials Science 15, pp. 208 – 224. Willets, K. A. and Duyne, R. P. V. (2007). Localized surface plasmon resonance spectroscopy and sensing, Annu. Rev. Phys. Chem. 58, pp. 267–297. Withers, F., Bointon, T. H., Dubois, M., Russo, S., and Craciun, M. F. (2011). Nanopatterning of fluorinated graphene by electron beam irradiation, Nano Lett. 11, pp. 3912 – 3916. Woessner, A., Lundeberg, M. B., Gao, Y., Principi, A., Alonso-González, P., Carrega, M., Watanabe, K., Taniguchi, T., Vignale, G., Polini, M., Hone, J., Hillenbrand, R., and Koppens, F. H. L. (2015). Highly confined low-loss plasmons in graphene-boron nitride heterostructures, Nature Materials 14, pp. 421–425. Wood, R. W. (1902). On a remarkable case of uneven distribution of light in a diffraction grating spectrum, Philosophical Magazine 4, pp. 396–402. Wooten, F. (1972). Optical Properties of Solids (Academic Press, New York). Wu, J., Zhou, C., Yu, J., Cao, H., Li, S., and Jia, W. (2014a). Design of infrared surface plasmon resonance sensors based on graphene ribbon arrays, Optics and Laser Technology 59, pp. 99 – 103. Wu, J.-W., Hawrylak, P., Eliasson, G., Quinn, J., and Fetter, A. (1986a). Magnetoplasma surface waves on the lateral surface of a semiconductor superlattice, Solid State Communications 58, 11, pp. 795–798. Wu, J.-W., Hawrylak, P., Eliasson, G., and Quinn, J. J. (1986b). Theory of the lateral surface magnetoplasmon in a semiconductor superlattice, Phys. Rev. B 33, pp. 7091–7098. Wu, J. W., Hawrylak, P., and Quinn, J. J. (1985). Charge-density excitation on a lateral surface of a semiconductor superlattice and edge plasmons of a

page 423

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

424

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

two-dimensional electron gas, Phys. Rev. Lett. 55, pp. 879–882. Wu, J.-Y., Gumbsand, G., and Lin, M.-F. (2014b). Combined effect of stacking and magnetic field on plasmon excitations in bilayer graphene, Phys. Rev. B 89, p. 165407. Wu, L., Chu, H. S., Koh, W. S., and Li, E. P. (2010). Highly sensitive graphene biosensors based on surface plasmon resonance, Opt. Express 18, pp. 14395 – 14400. Wunsch, B., Stauber, T., Sols, F., and Guinea, F. (2006). Dynamical polarization of graphene at finite doping, New J. Phys. 8, p. 318. Xiao, S., Zhu, X., Li, B.-H., and Mortensen, N. A. (2016). Graphene-plasmon polaritons: From fundamental properties to potential applications, Front. Phys. 11, p. 117801. Xu, G., Liu, J., Wang, Q., Hui, R., Chen, Z., Maroni, V. A., and Wu, J. (2012a). Graphene: Plasmonic graphene transparent conductors, Adv. Mater. 24, pp. 1521 – 4095. Xu, W., Ling, X., Xiao, J., Dresselhaus, M. S., Kong, J., Xu, H., Liu, Z., and Zhang, J. (2012b). Surface enhanced raman spectroscopy on a flat graphene surface, Proceedings of the National Academy of Sciences 109, 24, pp. 9281– 9286. Yamaguchi, T., Moriya, R., Inoue, Y., Morikawa, S., Masubuchi, S., Watanabe, K., Taniguchi, T., and Machida, T. (2014). Tunneling transport in a few monolayer-thick ws2/graphene heterojunction, Appl. Phys. Lett. 105, p. 223109. Yamamoto, K., Tani, M., and Hangyo, M. (2007). Terahertz time-domain spectroscopy of imidazolium ionic liquids, J. Phys. Chem. B 111, pp. 4854–4859. Yan, H., Li, X., Chandra, B., Tulevski, G., Wu, Y., Freitag, M., Zhu, W., Avouris, P., and Xia, F. (2012a). Tunable infrared plasmonic devices using graphene/insulator stacks, Nature Nanotechnology 7, pp. 330–334. Yan, H., Li, Z., Li, X., Zhu, W., Avouris, P., and Xia, F. (2012b). Infrared spectroscopy of tunable dirac terahertz magneto-plasmons in graphene, Nano Lett. 12, pp. 3766–3771. Yan, H., Low, T., Zhu, W., Wu, Y., Freitag, M., Li, X., Guinea, F., Avouris, P., and Xia, F. (2013). Damping pathways of mid-infrared plasmons in graphene nanostructures, Nat. Photonics 7, pp. 394–399. Yan, H., Xia, F., Li, Z., and Avouris, P. (2012c). Plasmonics of coupled graphene micro-structures, New J. Phys. 14, p. 125001. Yao, Y., Kats, M. A., Genevet, P., Yu, N., Song, Y., Kong, J., and Capasso, F. (2013). Broad electrical tuning of graphene-loaded plasmonic antennas, Nano Lett. 13, pp. 1257–1264. Yeung, K. Y. M., Chee, J., Song, Y., Kong, J., and Ham, D. (2015). Symmetry engineering of graphene plasmonic crystals, Nano Lett. 15, pp. 5001–5009. Yeung, K. Y. M., Chee, J., Yoon, H., Song, Y., Kong, J., and Ham, D. (2014). Far-infrared graphene plasmonic crystals for plasmonic band engineering, Nano Lett. 14, pp. 2479–2484. Yin, P. T., Kim, T.-H., Choi, J.-W., and Lee, K.-B. (2013). Prospects for graphene-nanoparticle-based hybrid sensors, Phys. Chem. Chem. Phys. 15,

page 424

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Bibliography

9in x 6in

b2445-mas

425

pp. 12785 – 12799. Yusoff, A. R. B. M. (2014). Graphene Optoelectronics: Synthesis, Characterization, Properties, and Applications (Wiley). Zayats, A. V., Smolyaninov, I. I., and Maradudin, A. A. (2005). Nano-optics of surface plasmon polaritons, Physics Reports 408, pp. 131–314. Zeng, S., Hu, S., Xia, J., Anderson, T., Dinh, X.-Q., Meng, X.-M., Coquet, P., and Yong, K.-T. (2015). Graphene-mos2 hybrid nanostructures enhanced surface plasmon resonance biosensors, Sensors and Actuators B: Chemical 207, pp. 801–810. Zenneck, J. (1907). Uber die fortpflanztmg ebener elektro-magnetischer wellen langs einer ebenen leiterflache und ihre beziehung zur drahtlosen telegraphie, Annalen der Physik 23, pp. 846–866. Zettili, N. (2009). Quantum Mechanics, 2nd edn. (Wiley, West Sussex). Zhan, T., Han, D., Hu, X., Liu, X., Chui, S.-T., and Zi, J. (2014). Tunable terahertz radiation from graphene induced by moving electrons, Phys. Rev. B 89, p. 245434. Zhan, T., Shi, X., Dai, Y., Liu, X., and Zi, J. (2013). Transfer matrix method for optics in graphene layers, J. Phys.: Condens. Matter 25, p. 215301. Zhang, J., Sun, Y., Xu, B., Zhang, H., Gao, Y., Zhang, H., and Song, D. (2013). A novel surface plasmon resonance biosensor based on graphene oxide decorated with gold nanorod-antibody conjugates for determination of transferrin, Biosensors and Bioelectronics 45, pp. 230 – 236. Zhang, J., Xiao, S., Wubs, M., and Mortensen, N. A. (2011). Surface plasmon wave adapter designed with transformation optics, ACS Nano 5, pp. 4359– 4364. Zhang, Q., Li, X., Hossain, M. M., Xue, Y., Zhang, J., Song, J., Liu, J., Turner, M. D., Fan, S., Bao, Q., and Gu, M. (2014). Graphene surface plasmons at the near-infrared optical regime, Scientific Reports 4, p. 6559. Zhao, Y., Chen, G., Du, Y., Xu, J., Wu, S., Qu, Y., and Zhu, Y. (2014). Plasmonic-enhanced raman scattering of graphene on growth substrates and its application in sers, Nanoscale 6, pp. 13754 – 13760. Zhao, Y., Hu, X., Chen, G., Zhang, X., Tan, Z., Chen, J., Ruoff, R. S., Zhu, Y., and Lu, Y. (2013). Infrared biosensors based on graphene plasmonics: modeling, Phys. Chem. Chem. Phys. 15, pp. 17118 – 17125. Zheludev, N. I. and Kivshar, Y. S. (2012). From metamaterials to metadevices, Nature Materials 11, pp. 917 – 924. Zheng, Y. B., Kiraly, B., Weiss, P. S., and Huang, T. J. (2012). Molecular plasmonics for biology and nanomedicine, Nanomedicine 7, pp. 751 – 770. Zhu, A. Y. and Cubukcu, E. (2015). Graphene nanophotonic sensors, 2D Materials 2, p. 032005. Zhu, J., Liu, Q. H., and Lin, T. (2013a). Manipulating light absorption of graphene using plasmonic nanoparticles, Nanoscale 5, pp. 7785 – 7789. Zhu, J. J., Badalyan, S. M., and Peeters, F. M. (2013b). Plasmonic excitations in coulomb-coupled n-layer graphene structures, Phys. Rev. B 8, p. 085401. Zhu, X., Shi, L., Schmidt, M. S., Boisen, A., Hansen, O., Zi, J., Xiao, S., and Mortensen, N. A. (2013c). Enhanced light–matter interactions in graphene-

page 425

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

426

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

covered gold nanovoid arrays, Nano Lett. 13, pp. 4690–4696. Zhu, X., Wang, W., Yan, W., Larsen, M. B., Bøggild, P., Pedersen, T. G., Xiao, S., Zi, J., and Mortensen, N. A. (2014). Plasmon-phonon coupling in largearea graphene dot and antidot arrays fabricated by nanosphere lithography, Nano Lett. 14, pp. 2907 – 2913. Zhu, X., Yan, W., Uhd Jepsen, P., Hansen, O., Asger Mortensen, N., and Xiao, S. (2013d). Experimental observation of plasmons in a graphene monolayer resting on a two-dimensional subwavelength silicon grating, Appl. Phys. Lett. 102, p. 131101. Ziman, J. M. (1972). Principles of the theory of solids, 2nd edn. (Cambridge University Press, Cambridge).

page 426

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Index

π-bonds, 17 π-orbitals, 17 σ-bonds, 17 p-polarized, 68, 75 p−polarization, 291 s−polarized, 367 Čerenkov radiation, 143 2D chalcogenides, 9 2D material, 17 2D plasmons, 119 2D polarizability, 34

Bloch surface waves, 170 Boltzmann’s equation, 34, 320, 344, 355 bound modes, 51 boundary conditions, 14, 49, 198, 271, 283, 357 boundary element method, 194, 208 Brillouin zone, 19, 20, 22 bubble diagram, 29 carbon atom, 17 carbon-carbon distance, 18, 19 charge-density oscillations, 78 chemical potential, 327, 329 chemical sensor, 296 cloaking, 9 collisionless case, 35 concentration of electromagnetic energy, 159 conducting oxides, 5 conduction band, 19, 21 conductivity, 24 conductivity step, 239 conductivity tensor, 115 constitutive relation, 15 continous wave (CW), 185 continuity equation, 12 Coulomb potential, 339 CVD-grown graphene, 165 cyclotronic motion, 119

absorbance, 43, 167, 274 absorption, 73 acoustic mode, 92, 99 AFM, 141 air-hBN interface, 126 allotrope, 17 anomalous scattering phase, 296 anti-crossing, 107 antidots periodic lattices, 268 antisymmetric mode, 61 aromatic hydrocarbons, 9 atomic force microscope, 141 atomically thin materials, 9 attenuated total reflection, 134 ballistic transport, 17 Bernal stacking, 141 biochemical sensing, 8 biomedicine, 9 biomolecules, 6

damping channels, 4 427

page 427

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

428

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

Das, 34 decaying rate, 125, 290 density-density correlation, 29 diagrammatic method, 29 diagrammatic representation of the dielectric function, 337 diamond, 17 dichalcogenides, 295 dielectric constant, 48, 114 dielectric function, 48, 50 dielectric grating, 267 dielectric-metal interface, 57 diffraction grating, 163 diffraction limit, 4 diffraction order, 169 diffusion coefficient, 356 Dirac cones, 19 Dirac electrons, 30 Dirac equation, 5 Dirac fermions, 17, 21 Dirac Hamiltonian, 120 Dirac points, 5, 19, 21, 22 discrete-dipole approximation, 194 dispersion curve, 70, 131 dispersion relation, 49, 59, 143 double layer graphene, 28, 86 Drude model, 14, 15, 24, 28 Drude peak, 177 dyadic Green’s function, 386, 394 dynamical conductivity, 25, 86 dynamical susceptibility, 29 effective-mass approximation, 19 eigenvalue problem, 21 electric displacement, 12, 254 electric field, 12, 15, 52, 60, 159 electric permittivity of vacuum, 12 electro-optical modulation, 8 electromagnetic field, 395 electron beam, 143 electron energy loss spectroscopies (EELS), 81 electron-hole pairs, 31 electron-loss spectroscopy, 62 electronic configuration, 17 electronic mobility, 17

electrostatic limit, 200, 253 epitaxial growth, 183 epitaxial methods, 164 equation of motion, 28, 314, 330, 375 evanescent tails, 61 Förster resonant energy transfer (FRET), 281 Förster resonance, 8 Fano, 1 fast electrons, 25 femtoseconds pump-probe measurements, 297 Fermi distribution function, 24, 283 Fermi energy, 24, 25 Fermi velocity, 20 Fermi’s golden rule, 21, 22 field confinement, 54 fine structure constant, 23 finite damping, 51 finite element method, 194 finite-difference time-domain, 194 Fröhlich interaction, 101 free electron gas, 48, 104 free-standing, 61 frequency-dependent conductivity, 12 Fresnel coefficients, 45, 127, 369 Fuchs-Kliewer excitations, 103 GaAs/AlGaAs, 86 Gallium-Arsenide, 132 Gauss-Laguerre quadrature, 260 Gaussian groove, 253, 259 gold nano-disks, 297 graphane, 166 graphene, 9 graphene disks, 6, 9, 232 graphene lattice, 17 graphene multilayers, 296 graphene nanostructures, 193 graphene plasmonics, 4 graphene ribbons, 9, 167, 193 graphene rings, 226 graphene surface plasmons, 4, 251 graphene/SiO2 , 106 grating coupling, 51, 131

page 428

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

Index

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

grating period, 131 Green’s functions, 195, 199, 289, 337, 375, 388, 394, 399 Green’s theorem, 254 Hall current, 345 harmonic time dependence, 15 hBN, 9, 101, 124 Heaviside step-function, 26, 317 Helmholtz equations, 14 Hermite polynomials, 120 hexagonal Boron Nitride, 292 high-frequency mode, 61 homogeneous rope, 380 honeycomb lattice, 17 hopping integral, 18 HREELS, 104 hyperbolic behavior, 128 hyperbolic material, 292, 296 hyperbolicity of type I and II, 124 image dipole, 285 infrared light sources, 295 infrared spectroscopy, 123 inhomogeneous doping, 239 integro-differential equation, 203 interband transitions, 16, 25, 26 intraband conductivity, 319 intraband contribution, 86 intraband transitions, 25 Jacobi’s polynomials, 234 Kretschmann configuration, 134 Kubo’s formula, 26 Landau damping, 31, 33, 85 Landau levels, 121 Laplace’s equation, 258 Legendre’s polynomials, 204 Levi-Civita symbol, 344 light absorption, 278 light line, 131 light-matter interaction, 24 Lindhard dielectric function, 28 Lindhard polarization, 31, 33

9in x 6in

b2445-mas

429

linear algebra, 171, 204 LO phonons, 102 localized surface plasmon-polaritons, 2, 295 long-lived plasmons, 31 longitudinal conductivity, 323, 373 longitudinal projector, 324 longitudinal RPA dielectric function, 95 Lorentz force, 112 Lorentz gauge, 144 Lorentz oscillators, 16, 179 Lorentzian groove, 253 loss function, 99 losses, 4 lossless conductor, 62 low energy Hamiltonian, 19 low-frequency mode, 61 Lyddane-Sachs-Teller relation, 102 magnetic field, 12, 60, 69, 113, 371 magnetic induction, 12 magnetic permeability, 12 magneto-optical conductivity, 121 magneto-optical tensor, 345 magneto-plasmons, 9, 112, 114, 122 Maxwell’s equations, 12, 48, 68 metal stripe, 298 metal-semiconductor plasmonics, 3 metallic contact, 149, 153 metallic grating, 1 metallic nanoparticles, 7, 8 metallic-dielectric interface, 281 metamaterials, 5, 8, 163 micro-ribbons, 163 mid-IR, 5, 28, 74 Mikhailov, S., 149 minimal coupling, 21 modified Bessel functions, 201 momentum operator, 20 momentum space, 20, 29 monochromatic electromagnetic wave, 150 MoS2 , 9 multipolar orders, 195

page 429

April 5, 2016

14:13

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

430

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

An Introduction to Graphene Plasmonics

nano-antennas, 6 nano-imaging, 141 nano-ribbons, 164 nanoparticles, 2, 8, 297 nanophotonics, 1 near-field evanescent components, 140 near-field optical microscopies, 140 NIR-vis, 9 noble metals, 16 non-linear optical response of graphene, 297 non-linear phenomena, 3, 9 non-local effects, 13, 28 non-local effects in the optical conductivity, 25 non-local optical conductivity, 32 non-radiative transition-rate, 287 normal vector, 270 Ohm’s law, 12, 256 Ohmic losses, 54, 177 optical absorption, 8 optical communications, 9 optical conductivity, 15, 24, 26, 316 optical deformation potential, 101 optical mode, 92 Otto configuration, 134 oxides, 9 particle-hole symmetry, 19 Paul Drude, 14 Pauli blocking, 26, 79 Pauli matrices, 20 Peierls substitution, 120 penetration depth, 55 perfect conductor, 64 periodic conductivity, 166 periodic graphene-based structures, 163 periodically modulated conductivity, 167 perturbation theory, 22, 29 Pettit, 62 phonon-polaritons, 297 phosphorene, 296 photodetection, 7, 8

plane-wave expansion, 13 Plasmon dispersion, 45 plasmon’s wavevector, 50 plasmon-phonon-polaritons, 102, 110 plasmonic hot-spots, 1 plasmonic integrated circuitry, 1 plasmonics, 295 Plemelj formulae, 243 Poisson’s equation, 195, 339 polarizability, 29, 30 polarization vectors, 384 polarizers, 9 prism coupling, 51, 134 propagation length, 54, 55 Purcell effect, 124 Purcell factor, 292 quantum emitter, 289 quantum plasmonics, 1, 3 radiating dipole, 375 random rough surface, 143 random-phase approximation, 28 Rayleigh method, 351 Rayleigh, Lord, 1 real space, 20 rectangular-box conductivity-profile, 201 reflectance, 167, 171, 274, 367 regular Bessel functions, 276 relaxation time, 15, 327 relaxation-time approximation, 34 resonant light, 149 Reststrahlen bands , 297 Riemann-Hilbert problem, 242 rope Green’s functions, 380 rope Lagrangian, 375 rope reflection coefficient, 378 rope transmission coefficient, 378 rotation matrix, 397 RPA dielectric function, 31, 333 RPA-RT, 83 Rydberg atoms, 281 Satou, A., 149 scalar potential, 145

page 430

April 5, 2016

14:13

An Introduction to Graphene Plasmonics

9in x 6in

b2445-mas

Downloaded from www.worldscientific.com by LA TROBE UNIVERSITY on 10/21/18. Re-use and distribution is strictly not permitted, except for Open Access articles.

Index

scattering of GSPs, 166 scattering rate, 15, 34 screening potential, 28 second quantization, 314 semi-classical magneto-optical conductivity, 118 semi-infinite insulators, 68 semiconductors, 19 SiC, 104, 183 silica, 54 silicene, 296 silicon carbide, 105, 298 silver, 54 sine-grating, 267 Sommerfeld, A., 1 Sommerfeld-Zenneck wave, 51 spatial confinement, 7 spectroscopy, 8 speed of light, 20 spin-polarized plasmonics, 1 splitting of the plasmonic band, 95 static response, 34 Stoke’s theorem, 14 strain, 167 surface acoustic waves, 9 surface optical phonons, 102 surface phonon-polaritons, 125 surface phonons, 101 surface plasmon-polaritons, 47, 67, 149, 261, 267, 271, 286, 295 surface-enhanced Raman scattering, 7

431

TO phonon, 103 transformation optics, 8 transition metal nitrides, 5 transition rate, 22 transmittance, 23, 167, 171, 274, 367 transverse electric, 5, 85 transverse magnetic, 5, 48 transverse optical phonon, 102 transverse projector, 324 Tubadar, T., 2 two-dimensional metal, 149 ultrafast plasmonics, 3 ultraviolet, 16 uniaxial crystal, 125 unidirectional excitation, 298 vacuum impedance, 115 vacuum permittivity, 24 valence band, 19, 21 valley degeneracy, 22 van der Waals heterostructures, 296 vector potential, 21, 22, 144 visibility, 183 visible, 16 Wannier basis, 18 WeS2 , 9 Wigner-Seitz cell, 18 Wood’s anomalies, 1 Zenneck, J., 1

T-matrix, 35 tangent vector, 270 TE surface modes, 85 TE surface plasmons, 115 temporal dispersion, 13 tensor product, 392 terahertz time-domain spectroscopy (TDS), 185 thermal conductivity, 17 Thomson, J. J., 14 THz, 5 THz plasmons, 164 time-dependent electric field, 313 TM surface plasmon-polaritons, 54

page 431